Many books on new smart materials are available, but specialized analysis of particular topics is still in high demand.
299 78 57MB
English Pages 424  Year 2020
616 149 11MB Read more
610 114 54MB Read more
599 57 24MB Read more
Nanotechnology in Fuel Cells focuses on the use of nanotechnology in macroscopic and nanosized fuel cells to enhance the
345 75 11MB Read more
Content: OVERVIEW ; 1. Nanocomposite and Nanostructured Coatings ; NANOSTRUCTURED MATERIALS ; 2. Encapsulation of Clay P
933 103 47MB Read more
Nanotechnology in Fuel Cells focuses on the use of nanotechnology in macroscopic and nanosized fuel cells to enhance the
254 106 13MB Read more
Nanotechnology in Smart Textiles considers various aspects of nanotechnology includingan extensive overview of nanotechn
732 131 49MB Read more
Table of contents :
Table of Contents
Part I: Advanced Cement-Based Composites
1: Nanoinclusions for Cementitious Materials
1.2 Dispersion of Nanoinclusions in a Cementitious Matrix
1.3 Nanoinclusions for Cement-Based Materials
1.3.1 Carbon-Based Inclusions
18.104.22.168 Carbon nanotubes
22.214.171.124 Carbon nanofibers
126.96.36.199 Graphene nanoplatelets
188.8.131.52 Carbon black
184.108.40.206 Graphene oxide
1.3.2 Metallic Nanoinclusions
220.127.116.11 Silver nanoparticle
1.3.3 Noncarbon Nanoinclusions
18.104.22.168 Cement nanoparticles
1.4 Safety of Nanomaterials
1.5 Discussion and Conclusion
2: Dispersion Techniques of Nanoinclusions in Cement Matrixes
2.1 Carbon Nanotubes Chemical Structure and Properties
2.2 Dispersion Techniques of Carbon Nanotubes Similia Similibus Solvuntur?
2.2.1 Physical Methods for CNT Dispersion
22.214.171.124 Ultrasonication physical method
2.2.2 Chemical Methods for CNT Dispersion
126.96.36.199 Surfactants structure, properties, and solubilizing capabilities
2.3 Dispersion of Carbon Nanotubes in Water with Surfactants Similia Similibus Solvuntur (with the Help of Ultrasonication)
2.3.1 Optimization of CNT Dispersion with Surfactants
188.8.131.52 Commercially available surfactants for CNT dispersions
184.108.40.206 Increasing CNT dispersion with the use of properly designed surfactants
3: Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation in Composite Cement–Based Sensors Filled with Carbon Black
3.2 SEBS-CB Sensors
3.2.2 Sensor Fabrication
3.3.1 Mix Proportions
3.3.2 Quality Control
3.3.4 Electromechanical Model
3.4 Results and Discussion
3.4.1 Percolation Thresholds
3.4.2 Strain Sensitivity
4: Advancements in Silica Aerogel–Based Mortars
4.2 Silica-Based Aerogel
4.3 Aerogel-Based Mortars
4.4 Performance of Aerogel-Based Mortars
5: Multifunctional Cement-Based Carbon Nanocomposites
5.2 Design and Manufacture of Multifunctional Cement-Based Carbon Nanocomposites
5.3 Behaviors of Multifunctional Cement-Based Carbon Nanocomposites
5.3.1 Mechanical Behaviors
5.3.2 Electrically Conductive Behavior
5.3.3 Sensing Behavior
5.3.4 Damping Behavior
5.3.5 Electromagnetic Shielding/Absorbing Behaviors
5.3.6 Self-Heating Behavior
6: Analysis and Modeling of Electromechanical Properties of Cement-Based Nanocomposites
6.2 Electrically Conductive and Electromechanical Mechanisms
6.2.1 Basic Principles of Electrical Conduction
220.127.116.11 Contacting conduction
18.104.22.168 Tunneling conduction and/or field emission conduction
22.214.171.124 Ionic conduction
6.2.2 Electrically Conductive Mechanisms
6.2.3 Electromechanical Mechanisms
6.3 Analysis of Electromechanical Properties
6.3.1 Electrical Resistivity
6.3.2 Impedance or Electrical Reactance
6.3.3 Electric Capacitance
6.3.4 Electrical Impedance Tomography
6.4 Modeling of Electromechanical Properties
6.4.1 Model Based on Tunneling Conduction
6.4.2 Model Based on Field Emission Conduction
6.4.3 Model Based on a Lumped Circuit
7: Evaluation of Mechanical Properties of Cement-Based Composites with Nanomaterials
7.5 Nano–Iron Oxide
7.7 Nanocarbon Materials
7.7.1 Graphene Nanoplatelets
7.7.2 Carbon Nanofibers
7.7.3 Carbon Nanotubes
7.8 Other Nanoparticles
7.9 Future Perspective
8: Micromechanics Modeling of Nanomodified Cement-Based Composites Carbon Nanotube
8.1 Introduction and Synopsis
8.2 Micromechanics Modeling of the Mechanical Properties of Nanomodified Composites
8.2.1 Fundamentals of Mean-Field Homogenization
8.2.2 Eshelby's Equivalent Inclusion
8.2.3 The Mori–Tanaka Approach
8.2.4 Self-Consistent Effective-Medium Approach
8.2.5 Extended Eshelby–Mori–Tanaka Approaches
8.2.6 Modeling of CNT Waviness
8.2.7 Modeling of CNT Agglomeration
8.3 Micromechanics Modeling of the Electrical Properties of CNT-Reinforced Composites
8.3.1 Physical Mechanisms Governing the Electrical Conductivity of CNT-Reinforced Composites
126.96.36.199 Tunneling resistance thickness and conductivity of the interface
188.8.131.52 Nanoscale composite cylinder model for CNTs
8.3.2 Percolation Threshold Estimates
8.3.3 Micromechanics Model for the Overall Conductivity of CNT-Reinforced Composites
184.108.40.206 Waviness and agglomeration effects
8.3.4 Micromechanics Model for the Piezoresistivity of CNT-Reinforced Composites
220.127.116.11 Volume expansion and reorientation of CNTs
18.104.22.168 Change in the conductive networks
22.214.171.124 Change in the tunneling resistance
9: Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
9.2 State of the Art of Nanomodified Structures
9.3 Cement-Based Sensors for Structural Health Monitoring
9.4 Structures with Embedded Cement-Based Sensors
9.5 Structures Made of Nanomodified Cement-Based Materials
Part II: Innovative Applications of Advanced Cement-Based Nanocomposites
10: Cement-Based Piezoresistive Sensors for Structural Monitoring
10.2 Various Types of Cement-Based Sensors
10.2.2 Cement-Based Composites
10.2.3 Carbon-Based Materials (Conductive Fillers)
10.2.4 Dispersion of Carbon-Based Nanomaterials in Cement-Based Composites
10.2.5 Preparation of Cement-Based Sensors and Test Configurations
10.2.6 Self-Sensing Properties by Various Carbon-Based Materials
10.3 Practical Applications of Cement-Based Sensors
11: Enhancing PCM Cement-Based Composites with Nanoparticles
11.2 Incorporation of PCM in Concrete, Mortar, or Cement
11.3 Enhancing PCM Microcapsules with Nanoparticles for Cement-Based Composites
12: Cement-Based Composites with PCMs and Nanoinclusions for Thermal Storage
12.2 Thermal Energy Storage
12.2.1 Sensible Heat Thermal Storage
12.2.2 Latent Heat Thermal Storage
12.3 Phase Change Materials
12.4 Cement-Based Composites with PCMs
12.4.1 Incorporation of PCMs in Cement-Based Materials Obtained with the Immersion Method
12.4.2 Incorporation of PCMs in Cement-Based Materials Obtained with Direct Mixing
12.4.3 Incorporation of PCMs in Cement-Based Materials Obtained with the Impregnation Method
12.5 PCMs and Nanoinclusions for Cement-Based Materials
12.5.1 Selection of PCMs
12.5.2 Selection of Nanoparticles
12.5.3 PCMs and Nanoinclusions for Cement-Based Materials
12.5.4 NEPCM-Cement-Based Materials for Building and Construction Applications
12.5.5 Recent Developments in NEPCM-Cement-Based Materials for High-Temperature Thermal Storage
13: Self-Heating Conductive Cement-Based Nanomaterials
13.2 Heating/Cooling Model
13.3 Stage of Heating Produced by the Application of Electric Current
13.4 Stage of Cooling
14: Functional Cementitious Composites for Energy Harvesting and Civil Engineering Applications an Overview
14.2 Composite Materials and Their Constituents
14.2.1 Major Phases
126.96.36.199 Matrix phase
188.8.131.52 Dispersed (reinforcing) phase
184.108.40.206 Interface in the composite structure
14.2.2 Design of Composites Connectivity Models
14.3 Composite Materials with Piezoelectric, Ferroelectric, and Pyroelectric Functionalities
14.3.2 Physics and Chemistry of Composite Materials
14.4 Fabrication of Composites
14.4.1 Fabrication of Polymer-Ceramic Composites
14.4.2 Fabrication of Cement-Ceramic Composites
14.5 Ambient Energy Harvesting and Structural Health Monitoring of Civil Structures via Cement Nanocomposites
14.5.1 Energy Harvesting via Cement Nanocomposites
220.127.116.11 Single-crystal-based materials
18.104.22.168 Polycrystalline-based materials
22.214.171.124 Charge storage via the pyroelectric effect
126.96.36.199 Thermal energy harvesting from pavements via modeling and simulation
188.8.131.52 Waste heat harvesting via thermoelectric cement composites
184.108.40.206 Electric power harvesting via application of piezoelectric transducers in pavements
14.5.2 Functional Cement-Based Nanocomposites for Structural Health Monitoring in Civil Engineering and Sensor Applications
14.6 Summary and Future Outlook
15: Addition of Carbon Nanofibers to Cement Pastes for Electromagnetic Interference Shielding in Construction Applications
15.1.1 Shielding by Reflection
15.1.2 Shielding by Absorption
15.1.3 Shielding by Multiple Reflections
15.1.4 Shielding Effectiveness
15.2.1 Materials and Specimens
15.2.2 Testing Procedures
15.3 Results and Discussion
16: Perspectives and Challenges of Nanocomposites
Nanotechnology in Cement-Based Construction edited by
Antonella D’Alessandro Annibale Luigi Materazzi Filippo Ubertini
Annibale Luigi Materazzi
Published by Jenny Stanford Publishing Pte. Ltd. Level 34, Centennial Tower 3 Temasek Avenue Singapore 039190 Email: [email protected] Web: www.jennystanford.com British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library. Nanotechnology in Cement-Based Construction c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the publisher.
For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.
ISBN 978-981-4800-76-1 (Hardcover) ISBN 978-0-429-32849-7 (eBook)
ADVANCED CEMENT-BASED COMPOSITES
1 Nanoinclusions for Cementitious Materials Antonella D’Alessandro 1.1 Introduction 1.2 Dispersion of Nanoinclusions in a Cementitious
Matrix 1.3 Nanoinclusions for Cement-Based Materials 1.3.1 Carbon-Based Inclusions 220.127.116.11 Carbon nanotubes 18.104.22.168 Carbon nanofibers 22.214.171.124 Graphene nanoplatelets 126.96.36.199 Carbon black 188.8.131.52 Graphene oxide 1.3.2 Metallic Nanoinclusions 184.108.40.206 Nano-TiO2 220.127.116.11 Nano-Fe2 O3 18.104.22.168 Silver nanoparticles 22.214.171.124 Nano-Al2 O3 126.96.36.199 Nano-ZnO 188.8.131.52 Nano-ZrO2 184.108.40.206 Nano-MgO 1.3.3 Noncarbon Nanoinclusions 220.127.116.11 Nano-SiO2 18.104.22.168 Nano-CaCO2 22.214.171.124 Nanoclay 126.96.36.199 Cement nanoparticles
1.4 Safety of Nanomaterials 1.5 Discussion and Conclusion 2 Dispersion Techniques of Nanoinclusions in Cement Matrixes Matteo Tiecco 2.1 Carbon Nanotubes: Chemical Structure and Properties 2.2 Dispersion Techniques of Carbon Nanotubes: Similia Similibus Solvuntur? 2.2.1 Physical Methods for CNT Dispersion 188.8.131.52 Ultrasonication physical method 2.2.2 Chemical Methods for CNT Dispersion 184.108.40.206 Surfactants: structure, properties, and solubilizing capabilities 2.3 Dispersion of Carbon Nanotubes in Water with Surfactants: Similia Similibus Solvuntur (with the Help of Ultrasonication) 2.3.1 Optimization of CNT Dispersion with Surfactants 220.127.116.11 Commercially available surfactants for CNT dispersions 18.104.22.168 Increasing CNT dispersion with the use of properly designed surfactants 3 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation in Composite Cement–Based Sensors Filled with Carbon Black Simon Laﬂamme and Filippo Ubertini 3.1 Introduction 3.2 SEBS-CB Sensors 3.2.1 Materials 3.2.2 Sensor Fabrication 3.3 Methodology 3.3.1 Mix Proportions 3.3.2 Quality Control 3.3.3 Measurements 3.3.4 Electromechanical Model 3.4 Results and Discussion 3.4.1 Percolation Thresholds
16 17 25
25 27 28 29 31 31
34 36 37 39
49 49 52 52 52 55 55 56 57 58 59 59
3.4.2 Strain Sensitivity 3.5 Conclusion 4 Advancements in Silica Aerogel–Based Mortars ´ Antonio Soares, Inˆes Flores-Colen, and Jorge de Brito 4.1 Introduction 4.1.1 Nanomaterials 4.2 Silica-Based Aerogel 4.3 Aerogel-Based Mortars 4.4 Performance of Aerogel-Based Mortars 4.5 Conclusions 5 Multifunctional Cement-Based Carbon Nanocomposites Liqing Zhang, Siqi Ding, Sufen Dong, Xun Yu, and Baoguo Han 5.1 Introduction 5.2 Design and Manufacture of Multifunctional
Cement-Based Carbon Nanocomposites 5.3 Behaviors of Multifunctional Cement-Based Carbon
Nanocomposites 5.3.1 Mechanical Behaviors 5.3.2 Electrically Conductive Behavior 5.3.3 Sensing Behavior 5.3.4 Damping Behavior 5.3.5 Electromagnetic Shielding/Absorbing
Behaviors 5.3.6 Self-Heating Behavior 5.3.7 Durability 5.4 Conclusions 6 Analysis and Modeling of Electromechanical Properties of
Cement-Based Nanocomposites Siqi Ding, Liqing Zhang, Xun Yu, Yiqing Ni, and Baoguo Han 6.1 Introduction 6.2 Electrically Conductive and Electromechanical
Mechanisms 6.2.1 Basic Principles of Electrical Conduction 22.214.171.124 Contacting conduction 126.96.36.199 Tunneling conduction and/or ﬁeld
188.8.131.52 Ionic conduction 6.2.2 Electrically Conductive Mechanisms 6.2.3 Electromechanical Mechanisms 6.3 Analysis of Electromechanical Properties 6.3.1 Electrical Resistivity 6.3.2 Impedance or Electrical Reactance 6.3.3 Electric Capacitance 6.3.4 Electrical Impedance Tomography 6.4 Modeling of Electromechanical Properties 6.4.1 Model Based on Tunneling Conduction 6.4.2 Model Based on Field Emission Conduction 6.4.3 Model Based on a Lumped Circuit 6.5 Conclusion 7 Evaluation of Mechanical Properties of Cement-Based
Composites with Nanomaterials Pedro de Almeida Car´ısio, Oscar Aurelio Mendoza Reales, and Romildo Dias Toledo Filho 7.1 Introduction 7.2 Nanosilica 7.3 Nanotitania 7.4 Nanoalumina 7.5 Nano–Iron Oxide 7.6 Nanoclay 7.7 Nanocarbon Materials 7.7.1 Graphene Nanoplatelets 7.7.2 Carbon Nanoﬁbers 7.7.3 Carbon Nanotubes 7.8 Other Nanoparticles 7.9 Future Perspective 8 Micromechanics Modeling of Nanomodified Cement-Based
Composites: Carbon Nanotubes Enrique Garc´ıa-Mac´ıas, Rafael Castro-Triguero, and ´ Andr´es Saez 8.1 Introduction and Synopsis 8.2 Micromechanics Modeling of the Mechanical
Properties of Nanomodified Composites
8.2.1 Fundamentals of Mean-Field Homogenization 175
8.2.2 Eshelby’s Equivalent Inclusion 180
8.2.3 The Mori–Tanaka Approach 183
8.2.4 Self-Consistent Effective-Medium Approach 183
8.2.5 Extended Eshelby–Mori–Tanaka Approaches 184
8.2.6 Modeling of CNT Waviness 185
8.2.7 Modeling of CNT Agglomeration 189
8.3 Micromechanics Modeling of the Electrical Properties
of CNT-Reinforced Composites 191
8.3.1 Physical Mechanisms Governing the Electrical
Conductivity of CNT-Reinforced Composites 192
184.108.40.206 Tunneling resistance: thickness and
conductivity of the interface 193
220.127.116.11 Nanoscale composite cylinder model
for CNTs 194
8.3.2 Percolation Threshold Estimates 195
8.3.3 Micromechanics Model for the Overall
Conductivity of CNT-Reinforced Composites 199
18.104.22.168 Waviness and agglomeration eﬀects 202
8.3.4 Micromechanics Model for the Piezoresistivity
of CNT-Reinforced Composites 203
22.214.171.124 Volume expansion and reorientation
of CNTs 203
126.96.36.199 Change in the conductive networks 205
188.8.131.52 Change in the tunneling resistance 206
8.4 Summary 209
9 Use of Carbon Cement–Based Sensors for Dynamic
Monitoring of Structures Andrea Meoni, Antonella D’Alessandro, Filippo Ubertini, and
Annibale Luigi Materazzi
9.1 Introduction 9.2 State of the Art of Nanomodified Structures 9.3 Cement-Based Sensors for Structural Health
Monitoring 9.4 Structures with Embedded Cement-Based Sensors 9.5 Structures Made of Nanomodified Cement-Based
9.6 Comments 9.7 Conclusion
INNOVATIVE APPLICATIONS OF ADVANCED
10 Cement-Based Piezoresistive Sensors for Structural
Ilhwan You, Seung-Jung Lee, and Doo-Yeol Yoo 10.1 Introduction 249
10.2 Various Types of Cement-Based Sensors 252
10.2.1 Piezoresistivity 252
10.2.2 Cement-Based Composites 253
10.2.3 Carbon-Based Materials (Conductive
10.2.4 Dispersion of Carbon-Based Nanomaterials
in Cement-Based Composites 256
10.2.5 Preparation of Cement-Based Sensors and
Test Configurations 258
10.2.6 Self-Sensing Properties by Various
Carbon-Based Materials 260
10.3 Practical Applications of Cement-Based Sensors 265
10.4 Conclusions 271
11 Enhancing PCM Cement-Based Composites with
Nanoparticles Luisa F. Cabeza and Anna Laura Pisello 11.1 Introduction 11.2 Incorporation of PCM in Concrete, Mortar,
or Cement 11.3 Enhancing PCM Microcapsules with Nanoparticles
for Cement-Based Composites 12 Cement-Based Composites with PCMs and Nanoinclusions
for Thermal Storage Manila Chieruzzi and Luigi Torre 12.1 Introduction 12.2 Thermal Energy Storage
12.2.1 Sensible Heat Thermal Storage 12.2.2 Latent Heat Thermal Storage Phase Change Materials Cement-Based Composites with PCMs 12.4.1 Incorporation of PCMs in Cement-Based Materials Obtained with the Immersion Method 12.4.2 Incorporation of PCMs in Cement-Based Materials Obtained with Direct Mixing 12.4.3 Incorporation of PCMs in Cement-Based Materials Obtained with the Impregnation Method PCMs and Nanoinclusions for Cement-Based Materials 12.5.1 Selection of PCMs 12.5.2 Selection of Nanoparticles 12.5.3 PCMs and Nanoinclusions for Cement-Based Materials 12.5.4 NEPCM-Cement-Based Materials for Building and Construction Applications 12.5.5 Recent Developments in NEPCM-Cement-Based Materials for High-Temperature Thermal Storage Conclusions
13 Self-Heating Conductive Cement-Based Nanomaterials E. Seva, O. Galao, F. J. Baeza, E. Zornoza, R. Navarro, and P. Garc´es 13.1 Introduction 13.2 Heating/Cooling Model 13.3 Stage of Heating Produced by the Application of Electric Current 13.4 Stage of Cooling 14 Functional Cementitious Composites for Energy Harvesting and Civil Engineering Applications: An Overview Ashok Batra, Aschalew Kassu, Bir Bohara, Timir B. Roy, and Antonella D’Alessandro 14.1 Introduction
290 291 291 294
300 307 308 308 309 316
319 320 327
327 331 332 333
14.2 Composite Materials and Their Constituents 14.2.1 Major Phases 184.108.40.206 Matrix phase 220.127.116.11 Dispersed (reinforcing) phase 18.104.22.168 Interface in the composite structure 14.2.2 Design of Composites: Connectivity Models 14.3 Composite Materials with Piezoelectric, Ferroelectric, and Pyroelectric Functionalities 14.3.1 Classification 14.3.2 Physics and Chemistry of Composite Materials 14.4 Fabrication of Composites 14.4.1 Fabrication of Polymer-Ceramic Composites 14.4.2 Fabrication of Cement-Ceramic Composites 14.5 Ambient Energy Harvesting and Structural Health Monitoring of Civil Structures via Cement Nanocomposites 14.5.1 Energy Harvesting via Cement Nanocomposites 22.214.171.124 Single-crystal-based materials 126.96.36.199 Polycrystalline-based materials 188.8.131.52 Charge storage via the pyroelectric eﬀect 184.108.40.206 Thermal energy harvesting from pavements via modeling and simulation 220.127.116.11 Waste heat harvesting via thermoelectric cement composites 18.104.22.168 Electric power harvesting via application of piezoelectric transducers in pavements 14.5.2 Functional Cement-Based Nanocomposites for Structural Health Monitoring in Civil Engineering and Sensor Applications 14.6 Summary and Future Outlook
344 344 344 345 345 346 347 347 349 350 350 350
351 351 355 356 360
15 Addition of Carbon Nanofibers to Cement Pastes for
Electromagnetic Interference Shielding in Construction
Applications E. Zornoza, O. Galao, F. J. Baeza, and P. Garc´es 15.1 Introduction 15.1.1 Shielding by Reﬂection 15.1.2 Shielding by Absorption 15.1.3 Shielding by Multiple Reﬂections 15.1.4 Shielding Eﬀectiveness 15.2 Experimental 15.2.1 Materials and Specimens 15.2.2 Testing Procedures 15.3 Results and Discussion 15.4 Conclusions
16 Perspectives and Challenges of Nanocomposites Antonella D’Alessandro, Filippo Ubertini, and
Annibale Luigi Materazzi
In recent years, developments in the ﬁeld of nanotechnology have impressively increased because of extensive scientiﬁc and technological research. Now they involve, among others, branches like science, medicine, and engineering. While many books are now on the market, the demand for specialized references that go in depth into single topics still remains. In this general frame, this book focuses on the application of nanotechnology to cement-based materials for civil engineering applications. It is aimed at giving both scholars and practitioner engineers up to-date information about recent developments and perspectives in this ﬁeld, with special reference to the topics that seem susceptible to major developments in the near future. In fact, while in the past, nanoinclusions into cement-based composites had the main purpose of increasing the mechanical strength, today it is possible to give materials many interesting and useful properties. This book is divided into two parts. The ﬁrst part, “Advanced Cement-Based Composites,” comprises nine chapters and presents novelties in the production of cemen titious nanocomposites. Special attention is paid to the types of nanoinclusions, to novel techniques to mix the components, and to the analysis of the properties that can be achieved by paste, mortar, or concrete if they are added with nanoinclusions. The second part, “Innovative Applications of Advanced CementBased Nanocomposites,” is devoted to the analysis of the new properties that can be given to nanocomposites.
Among them, very promising is the capability of sensing mechanical strain, which can lead to the production of embedded sensors for dynamic monitoring of structures. They can measure internal forces as well as detect damage. Moreover the use of phase-changing materials gives the nanocomposite the capability of storing and releasing heat, with evident possibility of application in the ﬁeld of heating and cooling apartments, houses, and industrial plants. Finally, they can collect energy from the environment (energy harvesting), as well eﬃciently shield electromagnetic waves. Annibale Luigi Materazzi 2020
ADVANCED CEMENT-BASED COMPOSITES
Nanoinclusions for Cementitious Materials Antonella D’Alessandro Department of Civil and Environmental Engineering, University of Perugia, Via G. Duranti 93, 06125 Perugia, Italy [email protected]
The development of nanotechnology allows the progress of several disciplines. New devices permit us to investigate materials and objects in depth and detect characteristics and properties at the nanoscale. Moreover, the production of always more novel nanomaterials with enhanced capabilities determines the nano engineering of composite devices with potentialities not possible before. In the ﬁeld of engineering, the availability of new micro and nanoparticles, above all the carbon-based ones, produces multi functional composite materials by adding inclusions in the original matrix. Concrete and cementitious materials result particularly suitable for a nano- or micromodiﬁcation due to the composite nature that characterizes them and the presence of micro- and nano-elements in their structure. The application of cement-based materials doped with nanoﬁllers in concrete structures, such as buildings, bridges, and pavements, enables us to improve their performance, to detect degradations and damages during the service
Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
4 Nanoinclusions for Cementitious Materials
life, and consequently to increase the safety of the users of such structures and infrastructures.
1.1 Introduction Diﬀerent types of inclusions for cementitious materials, with various characteristics and properties, are available in the market and their number is constantly growing. The most adopted particles in the ﬁeld of engineering are the carbon-based ones and oxides, such as nanosilica and nanotitania. Their applicability is strictly related to the good dispersion of the ﬁller into the matrix in order to obtain a homogeneous material. Fillers can be particles or ﬁbers: both types exhibit beneﬁts and disadvantages. Indeed, ﬁbrous particles possess a higher aspect ratio, which is the ratio between length and diameter, related to enhanced electrical and mechanical performances but also related to the diﬃculty in obtaining a good dispersion and to a greater tendency to be damaged during the mixing . This chapter is aimed at describing the main particles suitable for cement-based materials, the main dispersing techniques of nanoinclusions in a cementitious matrix, and the issues related to the eﬀects on health and on the environment related to their use.
1.2 Dispersion of Nanoinclusions in a
An optimal dispersion of inclusions in a material determines (i) the reliability and stability of the sensing and mechanical properties, (ii) the enhancement of the ﬁller eﬃciency, and (iii) the decrease of the mechanical energy for mixing . The dispersability of an inclusion depends on its hydrophilicity—because the cement-based materials are water based—and on its predisposition of producing agglomerations, due to the mutual forces between the elements forming the ﬁllers. There are three main methods used to disperse nanoinclusions in a cement matrix: using dispersants, by mechanical mixing, and using sonication (Fig. 1.1). Dispersants can be sur
Dispersion of Nanoinclusions in a Cementitious Matrix 5
Figure 1.1 Dispersion methods (a) using dispersants, (b) through mechan ical mixing, and (c) by sonication.
factants and mineral admixtures (Fig. 1.1a). The former possess a particular chemical composition able to disperse by wetting, electrostatic repulsion, or steric hindrance eﬀect . The mineral admixtures act with gradation, adsorption, and separation eﬀects. However, some of the eﬀective surfactants are not compatible with cementitious materials and with their applications. Mechanical methods, based on milling at high speed, are not eﬀective with all types of particles and may produce damages in ﬁbrous ﬁllers due to the shear energy released during the mix (Fig. 1.1b). Often mechanical mixing is adopted in combination with ultrasonication, with an embedded probe, or through the immersion in a sonicated bath (Fig. 1.1c). Eﬀective results also are obtained through the combination of organic ligands, including polycarboxilate-based water reducers, with probe sonication . Chemical methods use covalent surface modiﬁcation through surface functionalization of nanoparticles in order to improve their chemical compatibility with the matrix, enhancing their wettability and reducing their tendency to agglomerate. However, they result in aggressive methods because the procedures might introduce structural defects and changing in peculiar properties that could aﬀect their capabilities .
6 Nanoinclusions for Cementitious Materials
An alternative innovative approach was proposed by Cwirzen et al.: the nanoparticles, as carbon nanotubes (CNTs) or carbon nanoﬁbers (CNFs), are grown on the surface of cement using a modiﬁed chemical vapor deposition method .
1.3 Nanoinclusions for Cement-Based Materials Concrete and cement-based materials are composite materials with components and pores at the nanoscale, too (Fig. 1.2). So, they are particularly suitable for nanomodiﬁcation. The addition of nanoﬁllers may enhance the concrete properties, acting on the hydration products or producing a ﬁller eﬀect. For example, the calcium-silicate-hydrate (C–S–H) gel, which determines the mechanical and physical properties—shrinkage, elasticity, creep, porosity, etc.—of cement pastes, can be modiﬁed in order to enhance durability. Besides, micro- or nanosize particles may improve the resistance of the composites through the ﬁller eﬀect or may provide new multifunctional capabilities, as thermal or electrical conductivity. There are various types of ﬁllers for cementitious ma terials, from dimensions of millimeters up to nanometers (Fig. 1.3). When the dimensions of a material decrease, important changes occur, for example, in electronic conductivity, optical absorption,
Figure 1.2 Dimensions of constituents of concrete and deﬁnition of main cement-based structural materials.
Nanoinclusions for Cement-Based Materials
Figure 1.3 Classiﬁcation of the main ﬁllers for concrete at the macro-, micro-, and nanoscale.
mechanical resistance, and chemical reactivity. The same materials can demonstrate enhanced properties at the nanosize level. The two main reasons of such behavior are the higher speciﬁc surface and the quantum eﬀects that increase the reactivity . Nanomaterials for cement-based materials can be organized into three main categories: carbon-based nanoﬁllers, metallic nanoinclusions, and other noncarbon nanoinclusions. Nanoparticles have costs 100 to 1000 times higher than Portland cement or others constituents of cement-based materials: this occurrence must be considered in the material design in relation to enhancement of the structural eﬃciency deriving from the use of such nanoparticles. So a key issue with the use of nanoﬁllers in cementitious materials is the choice of the optimal amount of addition . The main concrete properties inﬂuenced by the presence of nanoparticles are workability, cohesiveness, content of entrained air in concrete, setting times (for fresh concrete), hydration reactions, compressive strength, tensile/ﬂexural strength, modulus of elasticity, and durability (for hardened concrete) .
1.3.1 Carbon-Based Inclusions The nanoparticle ﬁllers most used for engineering applications are carbon-based ones. Carbon is the only element with stable
8 Nanoinclusions for Cementitious Materials
allotropes from the zero to the third dimension. Carbon-based ﬁllers include CNTs, CNFs, carbon black (CB), graphene nanoplatelets (GNPs), and graphene oxide (GO) . These ones are charac terized by diﬀerent morphology and aspect ratio and can be classiﬁed as 0D (nanoparticles), 1D (nanoﬁlaments), and 2D (nanosheets). Generally, their reinforcement eﬀect into composite materials proportionally increases with an increase in the aspect ratio.
22.214.171.124 Carbon nanotubes CNTs are rolled sheets of graphene arranged in cylinders. They can be single-walled CNTs (with one rolled sheet) or multiwalled CNTs (with more concentric cylinders). Single-walled CNTs have internal diameter of 0.4–2.5 nm and a length of tenths of microns; multiwalled CNTs have an average inner diameter of 5–10 nm and a length of 0.1–10 microns (Fig. 1.4a). They can be considered as 1D ﬁllers. Both types of CNTs are used to strengthen composite materials and to provide materials with conductive and thermal capabilities. Carbon atoms were arranged in a hexagonal pattern with strong covalent bonds, type σ –σ , while the tubes were connected through van der Waals forces, which determine the formation of agglomerates during their dispersion into cementitious matrices. Such undesirable structures can be limited through the use of a proper dispersion technique. CNTs appear as a black powder, with a very high speciﬁc surface area (of the order of 100–250 m2 /g) and a very low apparent density. The important properties of CNTs make them suitable for applications in diﬀerent ﬁelds. Their strength-to-weight ratio higher than other materials allows us to obtain light-strength composites, as those used for spacecraft. In cement-based materials they are adopted, above all, for increasing mechanical performance [9, 10] and for smart monitoring appli cations [11–13]. CNTs can be metals, semiconductors, or small gap semiconductors, depending on the orientation of the graphene sheets. They possess enhanced mechanical capabilities: they are highly resilient, their Young’s modulus is roughly 1.2 TPa, and their tensile strength is about a hundred times higher than that of steel .
Nanoinclusions for Cement-Based Materials
Their piezoresistive capability is used to realize composites with self-monitoring properties. Moreover, nanocement (made of CNTs within the cementitious material) has the potential to create tough, durable, high-temperature, ﬁre-resistant coatings . The liter ature shows positive mechanical performances of doped cement based materials with volume contents lower than 0.01% of CNTs [15, 16], related to a total porosity reduction . Also single-walled CNTs determine a nucleation eﬀect in cement-based composites . Moreover, the rheological behavior of cementitious materials with CNTs is diﬀerent from that of normal cement-based materials, showing a higher suspension viscosity .
126.96.36.199 Carbon nanofibers CNFs are 1D nanoﬁllers as CNTs but with greater dimensions and a diﬀerent internal structure. They are stacked according to three diﬀerent patterns: cups, cones, or plates. They can be produced by low heat treatment with temperatures up to 1500◦ C, which partially chemically graphitize the vapor-deposited carbon on the surface and allow us to obtain ordered structures. Their average diameter and length vary from 70 to 200 nm and 50 to 200 μm, respectively (Fig. 1.4b). They have a tensile strength slightly less than that of CNTs, but their cost is about 50 times lower, making them particularly appropriate for scalable applications . Their mechanical and conductive properties make them suitable for realizing cementitious materials with high mechanical resistance  and electrical capabilities for applications in de-icing , self-sensing , and electromagnetic shielding .
188.8.131.52 Graphene nanoplatelets GNPs generally are chemically exfoliated from natural graphite. They consist of small layers of graphene with an overall thickness of about 3–10 nm (Fig. 1.4c). In the scientiﬁc literature, these elements are often named “graphite nanoplatelets” . GNPs are excellent electrical and thermal conductors as a result of their pure
10 Nanoinclusions for Cementitious Materials
graphitic composition. Unlike other nanoﬁllers presented before, they are 2D, resulting in the achievement of isotropic nanomodiﬁed composites . Graphene is one of the strongest materials: its tensile strength is approximately 100–300 times higher than that of steel. So, its possible applications are an interesting topic in the ﬁeld of engineering. Added to cement matrices, graphene nanomaterials provide enhanced mechanical  and smart capabilities, resulting in multifunctional composites . Graphene is an expensive material with respect to other carbon-based nanoparticles, and it is highly hydrophobic, so a dispersion procedure is needed to obtain homogeneous composites. Cementitious materials doped with hybrid GNPs show enhanced strength, fracture resistance, and higher durability than high-performance concrete (HPC) . Also, such nanomaterials signiﬁcantly contribute to arrest crack generation.
184.108.40.206 Carbon black CB is composed of pure elemental carbon in the form of colloidal spherical particles in an amorphous molecular structure (Fig. 1.4d). The row material is produced by incomplete combustion of organic materials such as petroleum or coal. CB particles are able to provide electrical conductivity both in water and in solvent-borne systems. Electron tunneling is one of the factors inﬂuencing the electrical conductivity of such nanoparticles, a property that comes from the capacity of electrons to jump the gaps between the closed CB pigments. This amorphous carbon allotrope represents a cheaper alternative to provide electrical properties to cement-based materials. The reduced size of CB and its electrical conductivity make it an economical method for protecting steel rebars from corrosion . Despite being less eﬀective than carbon ﬁbers, the literature [30, 31] reports a good self-sensing behavior of cement matrices containing CB: an increase in the compressive stress leads to a linear decrease in the fractional change of the electrical resistance . Other researchers  have measured both the mechanical and the piezoresistive performances of mortar specimens doped with CB. They found that the addition of CB with a content of approximately 4% w/b (weight-to-binder ratio) is
Nanoinclusions for Cement-Based Materials
Figure 1.4 Micrographs obtained by scanning electron microscopy of diﬀerent ﬁllers: (a) multiwalled CNTs, (b) CNFs, (c) GNPs, (d) CB, (e) titania, and (f) nanonickel particles.
favorable for improving the compressive and tensile strengths of the composites.
220.127.116.11 Graphene oxide GO consists of graphite oxidized with oxygen molecules that separate the carbon layers . Carboxyl, hydroxyl, and epoxy functional groups confer high water solubility to GO but, on the other hand, degrade its electrical properties . GO can compete economically with CNTs because of its ease of production and its higher solubility in aqueous solutions. It acts as a nucleation area for C–S–H gel, promoting cement hydration . A 0.05 wt% of GO increases the compressive strength of cement paste by 15%–33% and the ﬂexural strength by 41%–59% . Also, the presence of GO enhances the ductility of cementitious materials.
12 Nanoinclusions for Cementitious Materials
1.3.2 Metallic Nanoinclusions 18.104.22.168 Nano-TiO2 Titanium dioxide nanoparticles (titania, TiO2 ) are white pigments with reﬂective properties. Nano-TiO2 is the most widely used photocatalyst ﬁller in construction materials and the second most used nano-oxide particle . It has been successfully applied in the production of self-cleaning concrete, as in the construction of the Dives in Misericordia Church in Rome. This nanoparticle is able to break down organic pollutants, volatile organic compounds, and bacterial membranes through a photocatalytic reaction. Its hydrophilic capability provides self-cleaning properties to materials where it is dispersed or applied. The resulting concrete surfaces remain with a white color . Nano-TiO2 possesses a high density (about 3.9 g/cm3 ) , which determines a higher hardness and has a direct inﬂuence on the properties and durability of cement-based materials where it is dispersed. Literature studies show that compressive strength gains about 10% and 20% for ﬁller contents of 0, 5, and 10 wt% . The packing eﬀect of nano-TiO2 in cementitious materials reduces permeability and the chloride diﬀusion coeﬃcient . Also, nano-TiO2 accelerates cement hydration and increases the reaction total heat, indicating a nucleation eﬀect of nano-TiO2 [38, 40].
22.214.171.124 Nano-Fe2 O3 An enhancement of compressive strength of composites with these nano-oxides is observed in cement-based materials containing 0.5%, 1.25%, and 2.5% of these nanoparticles . The capillary permeability decreases for concrete with nano-Fe2 O3 . Literature studies also show that it is able to confer self-sensing properties to cementitious materials where it is dispersed .
126.96.36.199 Silver nanoparticles Nanosilver particles are able to inhibit the growth of bacteria, with a disinfection eﬀect toward infection, odor, itchiness, and sores. The strength of such particles is their capability to be distributed
Nanoinclusions for Cement-Based Materials
uniformly due to their very small size. Their application results in the realization of smart surfaces and coatings .
188.8.131.52 Nano-Al2 O3 Aluminum oxide nanoparticles react with calcium hydroxide in the hydration of calcium silicates. This pozzolanic reaction is related to the amount of available surface area. So, the addition of alumina improves the mechanical properties of concretes, such as tensile and ﬂexural strength. The alumina could also substitute cement up to 2.0% as a binder of cementitious materials, with an optimal replacement amount of 1.0% [7, 9], even if good results have been obtained for higher amounts . Nano-Al2 O3 , or nanoalumina, is also identiﬁed as a retarder of cement hardening . The capillary permeability decreases for concrete with nano-Al2 O3 . It is also able to determine a signiﬁcant increase in the elastic modulus (up to 143% with an addition of 5%) but with a limited eﬀect on compressive strength .
184.108.40.206 Nano-ZnO Nano-ZnO possesses semiconducting and piezoelectric dual prop erties, which can confer to materials, such as cement-based ones, enhanced electrical properties. Used for concrete manufacturing, it also improves the processing time and the resistance of concrete against water .
220.127.116.11 Nano-ZrO2 Zirconium oxide nanoparticles, or zirconia nanopowder, have dimensions between 5 and 100 nm. They are white and pos sess high-surface-area particles (speciﬁc surface area of 25–50 m2 /g). Nano-ZrO2 , or nanozirconia, shows good properties with regard to aesthetics (translucency), mechanical strength (hardness, ﬂexibility, durability), and chemical resistance (basically inert) and is a notable insulator . Small amounts of nano-ZrO2 , up to 2.5%, enhance the compressive strength of nanocementitious composites .
14 Nanoinclusions for Cementitious Materials
18.104.22.168 Nano-MgO Nano-MgO is a newly explored chemical nanoﬁller for cementitious materials. It possesses properties as a shrinkage compensator, and it is more eﬀective than other expansion agents .
1.3.3 Noncarbon Nanoinclusions 22.214.171.124 Nano-SiO2 Nano-SiO2 , or nanosilica, is the main studied oxide nanoﬁller for cement-based materials that could be delivered in powdered or liquid suspensions. Its real density is about 2.25–2.54 g/cm3 [6, 7], and it leads to the cheapest cost–volume relationship for oxide nanoparticles. A pozzolanic reaction is directly related to its high surface area. The use of nano-SiO2 in concretes signiﬁcantly increases the compressive strength by ﬁlling the pores between large ﬂy ash and cement particles. Compressive strength could increase by about 18% due to the reaction of nanomaterials with calcium hydroxide crystals of the interfacial zone between cement paste and aggregates, producing C–S–H gel. Flexural strength could increase up to 8%. Also the ﬁlling action of nano-SiO2 enhances the strength of the composites through the resulting denser microstructure . The optimal percentage of addiction is around 3% because greater amounts may reﬂect negatively to the performance of the composite due to the agglomeration of the ﬁllers. Other studies  have indicated that the optimum nano-SiO2 volume content is about 2%, and the compressive strength decreases after this ﬁller quantity. Permeability shows a reduction of about 45% for concrete with 3 wt% of nano-SiO2 , with a decrease of carbonation velocity and chloride diﬀusion coeﬃcient [49, 39]. These properties and the durability enhancement could be related with two important microstructural aspects of cementitious nanomaterials: the packing eﬀect and the pozzolanic reaction of the nano-SiO2 ﬁller . Moreover, nano-SiO2 is able to decrease the setting time of cementitious materials when compared to silica fume (microsize), can reduce bleeding water and avoid segregation, and is helpful in facilitating the use of recycled materials in the cement. The
Nanoinclusions for Cement-Based Materials
addition of nano-SiO2 to cement-based materials can also decrease the degradation of the calcium-silicatehydrate reaction caused by calcium leaching into water, preventing water penetration and so enhancing the durability. Nano-SiO2 is a cement-hardening acceler ator; it improves workability and resistance to water penetration . Furthermore, nano-SiO2 is one of the most economical, the most studied, and, also, the most consumed nanoﬁller in cement worldwide .
126.96.36.199 Nano-CaCO2 Nano-CaCO3 accelerates the hardening process of concrete and reduces the shrinkage, although high humidity of the environment is needed during curing of the samples to improve their durability . Small amounts of such a nanoﬁller, up to 2.5%, enhance the compressive strength of nanocementitious composites . Higher percentages improve microhardness and the elastic modulus , which produce also a nucleation eﬀect.
188.8.131.52 Nanoclay Another pozzolanic material used in the cement matrix is nanomontmorillonite, commonly called nanoclay. It consists of a three-layered 2D structure of aluminum inserted between two layers of silicon. It seems promising in enhancing mechanical properties, resistance to chloride penetration, and self-compacting ability and in reducing the permeability and shrinkage  of cementitious materials. Nanoclay also acts as a plasticizer and reduces permeability . Compressive strength of cementitious materials could increase by about 11% due to the reactions in the interfacial zone between cement paste and aggregates, producing C– S–H gel. Flexural strength could increase by 4% .
184.108.40.206 Cement nanoparticles Cement nanoparticles are binder nanoparticles of C2 S, C3 S, C3 A, and C4 AF obtained by sol-gel processing and heating treated by a ﬂame spray reactor and oven heating. They possess a high surface area, which determines a notable water demand, and consequently,
16 Nanoinclusions for Cementitious Materials
the nanocomposites they create generally have higher water/binder ratios and so greater porosity. Also, ultrasonic treatment induces a positive impact on compressive strength .
1.4 Safety of Nanomaterials The risks related to the use of nanomaterials essentially occur by exposures during the preparation of nanoparticles and their possible accidental release. The toxicity of nanocomposites depends on a number of factors such as particle size, surface area, crystallinity, surface chemistry, and particle agglomeration tendency [57, 58]. The main risks of nanoparticles can be summarized as follows: • Aggregation: Leads to poor corrosion resistance, high solubil ity, and deterioration with consequent issues in the structure maintenance [59, 60]. • Reactivity or charge: Chemical structure and charge-related critical functional groups could be critical for speciﬁc func tionality and for bioavailability of nanomaterials . • Impurity: Nanoparticles can interact with impurities due to their high reactivity and generate undesirable features. • Contaminant dissociation: This refers to contamination of residual impurities in the nanoparticles. • Size: It aﬀects the reactivity and agglomeration of nanoparti cles. • Recycling and disposal: There aren’t deﬁnitive experimental results about nanoparticles’ exposure and their potential toxicity. The available data about the toxicity of nanomaterials concerns: • Dose and exposure time eﬀect, which is related to the penetration in cells and depends on the molar concentration of the nanoparticles . • Aggregation and concentration eﬀect, with contradictory points of view. Indeed, some researches assert that the
Discussion and Conclusion
increase of nanoparticles enhances agglomeration features unable to penetrate the cells, with loss of toxicity. • Particle size eﬀect: Studies show size-dependent toxicity . • Particle shape eﬀect: Nanoparticles possess diﬀerent toxicity levels at diﬀerent aspect ratios . • Surface area eﬀect: Generally the toxicological eﬀect of nanoparticles increases with a decrease in the particle size and an in the surface area. • Crystal structure eﬀect: Diﬀerent structures may exhibit dif ferent cellular uptake, oxidative mechanisms, and subcellular localizations . • Surface functionalization eﬀect: Diﬀerent particles’ function alization is related to diﬀerent oxidation processes [66, 67]. • Pre-exposure eﬀect: Pre-exposure to nanoparticles results in the adaptability of the human body . Protective measures and actions against nanoparticles’ risks are available. Mainly they consist in (i) engineering control (use of ventilated/ﬁltered environment and boxes), (ii) administrative controls (appropriate information, clear and exhaustive procedures, good hygiene practices), (iii) personal protective equipment (PPE; respiratory protection devices, dermal protection, and eye protec tion), and (iv) medical screening and surveillance (proper medical continuous screening). It is also important to note that nanoparticles are widely used in bioapplications, but evidence about potential adverse health and environmental eﬀects due to protracted exposure to them has not yet been established. However, the environmental impact of such nanomaterials and of their residual waste is expected to increase in the future . Moreover, many factors can inﬂuence their ecotoxicity, such as pH, salinity, and organic residues .
1.5 Discussion and Conclusion Nowadays, novel nanoparticles are always available in the market, due to the progress of nanotechnology. There are diﬀerent types of nanomaterials suitable to be added to cementitious mixtures,
18 Nanoinclusions for Cementitious Materials
providing enhanced properties or new ones. Among other nano ﬁllers, carbon-based ones appear particularly promising for the realization of multifunctional concretes. Also nanotitania and nanosilica are increasingly adopted for their eﬀectiveness and low cost. Issues related to the preparation of composites with nanoﬁllers are associated with the dispersion procedures and the choice of the optimal amount. The homogeneity of nanocomposites is essential to realize feasible materials, and higher additions may determine a deterioration of peculiar properties. A delicate task also concerns the health and environmental eﬀects related to an increasing use of nanoparticles, because in-depth epidemiology studies with univocal and clear results are not completely available.
Acknowledgments The support of the European Union’s Framework Programme for Research and Innovation HORIZON 2020 under Grant Agreement No. 765057 and of the Italian Ministry of Education, University and Research (MIUR) through the funded Project of Relevant National Interest “SMART-BRICK: Novel Strain-Sensing Nanocomposite Clay Brick Enabling Self-Monitoring Masonry Structures” is gratefully acknowledged.
References 1. Horszczaruk, E., Sikora, P., Lukowski, P. (2016). Application of nanomaterials in production of self-sensing concretes: contemporary developments and prospects, Arch. Civ. Eng., LXII(3), pp. 61–73. 2. Han, B., Ding, S., Yu, X. (2015). Intrinsic self-sensing concrete and structures: a review, Measurement, 59, pp. 110–128. 3. Kawashima, S., Houa, P., Corr, D. J., Shah, S. P. (2015). Modiﬁcation of cement-based materials with nanoparticles, Cem. Concr. Compos., 36, pp. 8–15. 4. Han, B., Yu, X., Ou, J. (2011). Multifunctional and smart carbon nanotube reinforced cement-based materials, in Gopalakrishnan, K., Birgisson, B., Taylor, P., Attoh-Okine, N. O. (eds.) Nanotechnology in Civil Infrastructure: A Paradigm Shift, Springer.
5. Cwirzen, A., Habermehl-Cwirzen, K., Nasibulina, L. I., Shandakov, S.
D., Nasibulin, A. G., Kauppinen, E. I., Mudimela, P. R., Penttala, V.
(2009). CHH cement composite, in Nanotechnology in Construction 3,
˜ ˜ 6. Bastos, G, Patino-Barbeito, F., Patino-Cambeiro, F., Armesto, J. (2016).
Nano-inclusions applied in cement-matrix composites: a review, Mate
rials, 9(12), p. 30.
7. Mendes, T., Hotza, D., Repette, W. (2015). Nanoparticles in cement based
materials: a review. Rev. Adv. Master. Sci., 40, pp. 89–96.
8. Yonathan Reches, Y. (2018). Nanoparticles as concrete additives: review
and perspectives, Constr. Build. Mater., 175, pp. 483–495.
9. Konsta-Gdoutos, M. S., Metaxa, Z. S., Shah, S. P. (2010). Highly dispersed
carbon nanotube reinforced cement based materials, Cem. Concr. Res.,
40(7), pp. 1052–1059.
10. Collins, F., Lambert, J., Duan, W. H. (2012). The inﬂuences of admixtures on the dispersion, workability, and strength of carbon nanotube-OPC paste mixtures, Cem. Concr. Compos., 34(2), pp. 201–207. 11. Coppola, L., Buoso, A., Corazza, F. (2011). Electrical properties of carbon nanotubes cement composites for monitoring stress conditions in concrete structures, Appl. Mech. Mater., 82, pp. 118–123. ´ 12. D’Alessandro, A., Ubertini, F., Garc´ıa-Macıas, E., Castro-Triguero, R., Downey, A., Laﬂamme, S., Meoni, A., Materazzi, A. L. (2017). Static and dynamic strain monitoring of reinforced concrete components through embedded carbon nanotube cement-based sensors, Shock Vib., 2017, 3648403 (11 pp). 13. Han, B., Yu, X., Ou, J. (2011). Multifunctional and smart nanotube reinforced cement-based materials, in Gipalakrishnan, K., Birgisson, B., Taylor P., Attoh-Okine, N. (eds.) Nanotechnology in Civil Infrastructure: A Paradigm Shift, Springer, pp. 1–48. 14. Olar, R. (2011). Nanomaterials and nanotechnologies for civil engi neering, Buletinul institutului politehnic din ias¸i, LIV(LVIII), 4, pp. 109– 118. 15. Cwirzen, A., Cwirzen K., Pentalla, V. (2008). Surface decoration of carbon nanotubes and mechanical properties of cement/carbon nanotube composites, Adv. Cem. Res., 20(2), pp. 65–73. 16. Konsta-Gdoutos, M. S., Metaxa Z., Shah, S. (2010). Multi-scale mechanical and fracture characteristics and early-age strain capacity of high performance carbon nanotube/cement nanocomposites, Cem. Concr. Compos., 32(2), pp. 110–115.
20 Nanoinclusions for Cementitious Materials
17. Nochaiya T., Chaipanich, A. (2011). Behavior of multi-walled carbon nanotubes on the porosity and microstructure of cement-based materials, Appl. Surf. Sci., 257(6), pp. 1941–1945. 18. Makar, J. M., Chan, G. W. (2009). Growth of cement hydration products on single-walled carbon nanotubes, J. Am. Ceram. Soc., 92(6), pp. 1303– 1310. 19. Yazdani, N., Brown, E. (2016). Carbon nanoﬁbers in cement composites: mechanical reinforcement, in Loh, K., Nagarajaiah, S. (eds.) Innovative Developments of Advanced Multifunctional Nanocomposites in Civil and Structural Engineering, Woodhead Publishing, Sawston, UK, pp. 217– 246. 20. Metaxa, Z. S., Konsta-Gdoutos, M. S., Shah, S. P. (2010). Mechanical properties and nanostructure of cement-based materials reinforced with carbon nanoﬁbers and Polyvinyl Alcohol (PVA) microﬁbers, in Advances in the Material Science of Concrete, Proceedings of the Session at the ACI Spring 2010 Convention, Chicago, IL, USA, 21–25 March 2010, American Concrete Institute (ACI): Farmington Hills, MI, USA, pp. 115– 126. ˜ ´ L., Baeza, F. J., Carmona, J., Garces, ´ P. (2016). Highly 21. Galao, O., Banon, conductive carbon ﬁber reinforced concrete for icing prevention and curing, Materials, 9, p. 281. 22. Hanbay, S., lankson, M. A. (2017). Self-sensing damage assessment and image-based surface crack quantiﬁcation of carbon nanoﬁbre reinforced concrete, Constr. Build. Mater., 134, pp. 520–529. 23. Chung, D. D. L. (2012). Carbon materials for structural self-sensing, electromagnetic shielding and thermal interfacing, Carbon, 50(9), pp. 3342–3353. 24. Meng W., Khayat K. (2016). Mechanical properties of ultra-high performance concrete enhanced with graphite nanoplatelets and carbon nanoﬁbers, Composite Part B, 107, pp. 113–122. doi:10.1016/ j.compositesb.2016.09.069 25. Le, J.-L., Du, H., Pang, S. D. (2014). Use of 2D graphene nanoplatelets (GNP) in cement composites for structural health evaluation, Composite Part B, 67, pp. 555–563. 26. Wu Y., Yi N., Huang L., Zhang T., Fang S., Chang H., Li N., Oh J., Lee J., Kozlov M. (2015). Three-dimensionally bonded spongy graphene material with super compressive elasticity and near-zero Poisson’s ratio, Nat. Commun., 6, pp. 1–9. doi:10.1038/ncomms7141
27. Chuah, S., Pan, Z., Sanjayan, J. G., Wang, C. M., Duan, W. H. (2014). Nano reinforced cement and concrete composites and new perspective from graphene oxide, Constr. Build. Mater., 73, pp. 113–124. 28. Graybeal, B. (2011). Ultra-High Performance Concrete. Federal Highway Administration (FHWA), U.S. Department of Transportation; Washing ton, DC, USA. Publication Number FHWA-HRT-11-038. 29. Masadeh, S. (2015). The eﬀect of added carbon black to concrete mix on corrosion of steel in concrete, J. Miner. Mater. Charact. Eng., 3, pp. 271– 276. doi:10.4236/jmmce.2015.34029 30. Wen, S., Chung, D. D. L. (2007). Partial replacement of carbon ﬁber by carbon black in multifunctional cement-matrix composites, Carbon, 45, pp. 505–513. doi:10.1016/j.carbon.2006.10.024 31. Xiao, H., Lan, C., Ji, X., Li, H. (2003). Mechanical and sensing properties of structural materials with nanophase materials, Pac. Sci. Rev., 5, pp. 7–11. 32. Gao, D., Strum, M., Mo, Y. L. (2009). Electrical resistance of carbon nanoﬁber concrete, Smart Mater. Struct., 18, pp. 1–7. doi:10.1088/ 0964-1726/18/9/095039 33. Monteiro, A., Cachim, P., Costa, P. (2016). Carbon nanoparticles cement-based materials for service life monitoring, Proceedings of the International RILEM Conference on Materials, Systems and Structures in Civil Engineering, Lyngby, Denmark, 22–24 August 2016. 34. Paulchamy, B., Arthi, G., Lignesh, B. (2015). A simple approach to step wise synthesis of graphene oxide nanomaterial, J. Nanomed. Nanotechnol., 6, pp. 1–4. 35. Palermo, V., Kinloch, I., Ligi, S., Pugno, N. (2016). Nanoscale mechanics of graphene and graphene oxide in composites: a scientiﬁc and technological perspective, Adv. Mater., 28, pp. 6232–6238. 36. Babak, F., Abolfazl, H., Alimorad, R., Parviz, G. (2014), Preparation and mechanical properties of graphene oxide: cement nanocomposites, Sci. World J., 2014, pp. 1–10. 37. Pan, Z., Duan, W., Li, D., Collins, F. (2013). Graphene oxide reinforced cement and concrete. Patent Number: WO2013096990A1, 4 July 2013. 38. Chen, J., Kou, S., Poon, C. (2012). Hydration and properties of nano-TiO2 blended cement composites, Cem. Concr. Compos., 34(5), pp. 642–649. 39. Zhang, M., Liu, H. (2011). Pore structure and chloride permeability of concrete containing nano-particles for pavement, Constr. Build. Mater., 25, pp. 608–616.
22 Nanoinclusions for Cementitious Materials
40. Senﬀ, L., Hotza, D., Lucas, S., Ferreira, V., Labrincha, J. A. (2012). Eﬀect of nano-SiO2 and nano-TiO2 addition on the rheological behavior and the hardened properties of cement mortars, Mater. Sci. Eng., A, 532, pp. 354–361. 41. Oltulu, M., Sahim, R. (2011). Simple and combined eﬀects of nano SiO2 , nano-Al2 O3 and nano-Fe2 O3 powders on compressive strength and capillary permeability of cement mortar containing silica fume, Mater. Sci. Eng., 528, pp. 7012–7019. 42. Li, H., Xiao, H.-G., Yuan, J., Ou, J. (2004). Microstructure of cement mortar with nanoparticles, Composite Part B, 35(2), pp. 185–189. 43. Land, G., Stephan, D. (2014). Controlling cement hydration with nanoparticles, Cem. Concr. Compos., 57, pp. 64–67 44. Li, Z., Wang, H., He, S., Lu, Y., Wang, M. (2006). Investigation on the preparation and mechanical properties of the nano-allumina reinforced cement composite, Mater. Lett., 60(3), pp. 356–359. 45. Broekhuizen, F. A., Broekhuizen, J. C. (2009). Nanotehnologia ˆın industria europeana˘ a construct¸iilor – Stadiul actual al tehnologiei (transl. from English), pp. 7–30. www.efbww.org 46. Shah, S., Hou, P., Konsta-Gdoutos, M. (2015). Nano-modiﬁcation of cementitious material: toward a stronger and durable concrete, J. Sustainable Cem. Based Mater., 5, pp. 1–22. 47. Mohamed, A. M. (2016). Inﬂuence of nano materials on ﬂexural behaviour and compressive strength of concrete, HBRC J., 12, pp. 212– 225. 48. Ji, T. (2005). Preliminary study on the water permeability and microstructure of concrete incorporating nano-SiO2 , Cem. Concr. Res., 35(10), pp. 1943–1947. 49. Collepardi, M., Olagot, J. J. O., Skarp, U., Troli, R. (2002). Inﬂuence of amorphous colloidal silica on the properties of self-compacting concretes, in Challanges of Concrete Construction, p. 12. 50. Sanchez, F., Sobolev, K. (2010). Nanotechnology in concrete: a review, Constr. Build. Mater., 24, pp. 2060–2071. 51. Chithra, S., Senthil Kumar, S. R. R., Chinnaraju, K. (2016). The eﬀect of colloidal nano-silica on workability, mechanical and durability properties of high performance concrete with copper slag as partial ﬁne aggregate, Constr. Build. Mater., 15, pp. 794–804. 52. Cai, Y., Hou, P., Zhou, Z., Cheng, X. (2016). Eﬀects of nano-CaCO3 on the properties of cement paste: hardening process and shrinkage
at diﬀerent humidity levels, in Proceedings of the 5th International Conference on Durability of Concrete Structures, Shenzhen, China, 30 June–1 July 2016. 53. Liu, X., Chen, L., Liu, A., Wang, X. (2012). Eﬀect of nano-CaCO3 on properties of cement paste, Energy Procedia, 16, pp. 991–996. 54. Sato, T., Beaudoin, J. (2011). Eﬀect of nano-CaCO3 on hydration of cement containing supplementary cementitious materials, Adv. Cem. Res., 23(1), pp. 33–43. ¨ ¨ ¸, H., Oktay, B. M. (2016). Shielding behaviors 55. Mutuk, H., Mutuk, T., Gumus and analysis of mechanical treatment of cements containing nanosized powders, Acta Phys. Pol., 130, pp. 172–174. 56. Chang, T.-P., Shih, J.-Y., Yang, K., Hsiao, T.-C. (2007). Material properties of Portland cement paste with nano-montmorillonite, J. Mater. Sci., 42, pp. 7478–7487. 57. Jeevanandam, J., Barhoum, A., Yen, S., Chan, Y. S., Dufresne, A., Danquah, M. K. (2018). Review on nanoparticles and nanostructured materials: history, sources, toxicity and regulations, Beilstein J. Nanotechnol., 9, pp. 1050–1074. 58. Mathialagan Sumesh, M., Alengaram, U. J., Jumaat, M. Z., Mo, K. H., Alnahhal, M. F. (2017). Incorporation of nano-materials in cement composite and geopolymer based paste and mortar: a review, Constr. Build. Mater., 148, pp. 62–84. 59. Kennedy, A. J., Hull, M. S., Steevens, J. A., Dontsova, K. M., Chappell, M. A., Gunter, J. C., Weiss, C. A. (2008). Factors inﬂuencing the partitioning and toxicity of nanotubes in the aquatic environment, Jr. Environ. Toxicol. Chem., 27, pp. 1932–1941. doi:10.1897/07-624.1 60. Wang, Y., Li, Y., Pennell, K. D. (2008). Inﬂuence of electrolyte species and concentration on the aggregation and transport of fullerene nanoparticles in quartz sands, Environ. Toxicol. Chem., 27, pp. 1860– 1867. doi:10.1897/08-039.1 61. Tervonen, T., Linkov, I., Figueira, J. R., Steevens, J., Chappell, M., Merad, M. (2009). Risk-based classiﬁcation system of nanomaterials, J. Nanopart. Res., 11, pp. 757–766. doi:10.1007/s11051-008-9546-1 62. Buzea, C., Pacheco, I. I., Robbie, K. (2007). Nanomaterials and nanoparticles: sources and toxicity, Biointerphases, 2, MR17–MR71. doi:10.1116/1.2815690 63. Ivask, A., Kurvet, I., Kasemets, K., Blinova, I., Aruoja, V., Suppi, S., ¨ Vija, H., Kakinen, A., Titma, T., Heinlaan, M. (2014). Size-dependent
24 Nanoinclusions for Cementitious Materials
toxicity of silver nanoparticles to bacteria, yeast, algae, crustaceans and mammalian cells in vitro, PLoS One, 9, p. e102108. doi:10.1371/ journal.pone.0102108 64. Lippmann, M. (1990). Eﬀects of ﬁber characteristics on lung deposition, retention, and disease, Environ. Health Perspect., 88, pp. 311–317. doi:10.1289/ehp.9088311 65. Xia, T., Kovochich, M., Brant, J., Hotze, M., Sempf, J., Oberley, T., Sioutas, C., Yeh, J. I., Wiesner, M. R., Nel, A. E. (2006). Comparison of the abilities of ambient and manufactured nanoparticles to induce cellular toxicity according to an oxidative stress paradigm, Nano Lett., 6, pp. 1794–1807. doi:10.1021/nl061025k ¨ ¨ ¨ 66. Oberdorster, G., Oberdorster, E., Oberdorster, J. (2005). Nanotoxicology: an emerging discipline evolving from studies of ultraﬁne particles, J. Environ. Health Perspect., 113, pp. 823–839. doi:10.1289/ehp.7339 67. Sayes, C. M., Fortner, J. D., Guo, W., Lyon, D., Boyd, A. M., Ausman, K. D., Tao, Y. J., Sitharaman, B., Wilson, L. J., Hughes, J. B., West, J. L., Colvin, V. L. (2004). The diﬀerential cytotoxicity of water-soluble fullerenes, Nano Lett., 4, pp. 1881–1887. doi:10.1021/nl0489586 68. Johnston, C. J., Finkelstein, J. N., Mercer, P., Corson, N., Gelein, R., ¨ Oberdorster, G. (2000). Pulmonary eﬀects induced by ultraﬁne PTFE particles, Toxicol. Appl. Pharmacol., 168, pp. 208–215. doi:10.1006/ taap.2000.9037 69. Khana, I., Saeed, K., Khan, I. (2019). Nanoparticles: properties, applica tions and toxicities, Arabian J. Chem., 12(7), pp. 908–931. ¨ M., Owen, R., 70. Handy, R. D., von der Kammer, F., Lead, J. R., Hassellov, Crane M. (2008). The ecotoxicology and chemistry of manufactured nanoparticles, Ecotoxicology, 17, pp. 287–314.
Dispersion Techniques of Nanoinclusions in Cement Matrixes Matteo Tiecco Department of Chemistry, Biology and Biotechnology, University of Perugia, Via Elce di Sotto 8, 06124 Perugia, Italy [email protected]
2.1 Carbon Nanotubes: Chemical Structure and Properties Carbon nanotubes (CNTs) are nanoscaled hollow cylinders com posed of a hexagonal arrangement of sp2 -hybridized carbon atoms. The CNTs can be interpreted as sheets of graphene rolled up to form cylindrical nanostructures, with diameters ranging from one to tens of nanometers and with lengths up to micrometers [1, 2]. CNTs are generally classiﬁed into two main categories: they can be single-walled (SWCNTs, in the case of a single roll of graphene composing them) or multiwalled (MWCNTs, in the case of multiple layers of graphite superimposed) nanotubes [3, 4]. The van der Waals interactions occurring among the sheets determine the merge of the tubes of CNTs into self-aggregating ﬁbers or bundles [5, 6]. In Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
26 Dispersion Techniques of Nanoinclusions in Cement Matrixes
Figure 2.1 Representations of a single-walled carbon nanotube (SWCNT) as a rolled sheet of graphene, a multiwalled carbon nanotube (MWCNT), and the aggregation in bundles/ﬁbers of CNTs.
Fig. 2.1 the structures of SWCNTs, MWCNTs, and a scheme of their aggregations in ﬁbers are reported. There are many synthetic procedures that can be used to synthesize CNTs; their dimensions, their properties, and the yields of the procedure depend on the method used to realize them, and every method has either advantages or disadvantages. The arc discharge method is one of the most used, thanks to its ease; with this procedure both SWCNTs and MWCNTs can be created, using diﬀerent catalysts, in a low-pressure inert gas chamber through the arc vaporization of two graphite rods [7, 8]. The disadvantages of this procedure are represented by the by-products obtained and the purifying procedures needed to obtain pure CNTs. This is even more relevant in the case of MWCNT synthesis. The laser ablation method is based on the use of pulsed laser on a graphite target in a high temperature reactor [9, 10]. This method gives high-purity products, but high energy is required for the procedure. The applications of CNTs are wide and have been increasing in recent years as they represent unique nanostructured mate rials. Nanotechnology, nano-electronics, composite materials, and
Dispersion Techniques of Carbon Nanotubes 27
biomedical applications are some relevant examples of scientiﬁc ﬁelds where both SWCNTs and MWCNTs are ﬁnding advantageous roles [4, 11–13]. Moreover, recent studies on the low or absent toxicity of these nanomaterials, as well as their capability of membrane penetration, have opened the way for their application as biological carriers of drugs [14, 15]. Unfortunately, it is well known that both SWCNTs and MWCNTs are practically insoluble in water or in organic solvents; this is due to their chemical structures as well as their high dimensions and to their folding into ﬁbers that lead to even bigger aggregates even harder to solubilize in both polar and nonpolar solvents [5, 6, 16–19]. These facts limit the application of these nanostructured systems if the problem is not faced properly. In this chapter, the most used and eﬀective techniques used in the literature for the CNT dispersion are treated; the ultrason ication/surfactant method (as well as a description of surfactants structures and properties) will be treated in depth for its high relevance in the ﬁeld of cement-based sensor realization. The eﬃcacious dispersions of MWCNTs in water is, in fact, a key factor for the inclusion of these nanostructured materials in cement matrixes.
2.2 Dispersion Techniques of Carbon Nanotubes: Similia Similibus Solvuntur? The terms “solubilization” and “dispersion” of CNTs in water or in organic solvents are improperly used in the literature. Both these terms are almost equally reported and used ; however, they refer to two diﬀerent processes: a solution, therefore solubilization, is referred to as a stable solution, while a dispersion is the formation of a colloidal system. These two processes are related also to the dimensions of the solutes: in the case of small dimensions (lower than nanometer units), it is better to refer to a solution; with solutes of higher dimensions (higher than nanometer units), a colloidal dispersion is formed. In the literature of CNT dispersions, the stability times of suspensions are variable, and also the dimensions
28 Dispersion Techniques of Nanoinclusions in Cement Matrixes
of CNTs in solution ; therefore it is not possible to deﬁnitely deﬁne them as solutions or dispersions. In this chapter, the term “dispersion” will be considered as the most proper one except in speciﬁc cases of solubilization. There are many eﬃcacious methods reported in the literature for CNT dispersion in diﬀerent solvents, but they can be simply divided into diﬀerent categories, depending on the kind of technique used: • Physical methods (i.e., ultrasonication, plasma treatment, general mechanical methods) are based on the use of physical treatment on CNTs—solvent systems without any chemical modiﬁcation of the CNTs or without the use of other additives as dispersants. • Chemical methods (i.e., functionalization of the CNTs’ chem ical structures, additives) are based on the functionalization of the CNTs’ surface by adding hydrophilic/hydrophobic functional groups via covalent bonding to the CNTs or with weak interacting additives such as surfactants. • Biochemical methods (i.e., use of biochemical molecules as carriers) are based on the use of biological molecules as carriers, in a host–guest manner. They are biovariants of the chemical methods and are relevant in the biomedical application of CNTs. All these methods were also successfully implemented by using combinations of them: the use of ultrasonication and surfactants is the most interesting method and will be treated in depth in this chapter. Biochemical methods will not be discussed as they represent methods for use in biological systems of CNTs; therefore they are not pertinent to the topic of this chapter and of this book.
2.2.1 Physical Methods for CNT Dispersion There are many physical methods reported in the literature to facilitate the dispersion of CNTs in water or organic solvents; all of them are based on the disaggregation of the ﬁbers and
Dispersion Techniques of Carbon Nanotubes 29
bundles that the CNTs are able to form in the solvents. The energy applied by the external source is able to form isotropic CNT suspensions that are stable in diﬀerent times, depending on the technique used. Mechanical mill-based methods result in eﬀective rotating structures that can provoke an eﬀective CNT dispersion in water solutions due to the rotation of disks with ﬁxed pots on them . This method gave interesting results, and it was applied even with the use of low temperatures and with the addition of surfactants . The use of microwaves was found to decrease the density of CNTs in water, leading to the formation of a more isotropic system . The advantage of this method is the easy access to microwave systems for chemical synthesis in chemistry laboratories; this method was successfully employed also in a chemical method to functionalize the CNT surface . Diﬀerent types of plasma techniques were also successfully used with and without the addition of surfactant molecules [25–27].
220.127.116.11 Ultrasonication physical method The ultrasonication procedure is based on the application of sound energy to a sample at ultrasonic frequencies (over 20 kHz). In a CNT–solvent system, ultrasonication provokes an exfoliation of the ﬁbers and bundles of CNTs due to a process of cavitation, leading to a dispersion of the CNTs [28, 29]. There are mainly two kinds of ultrasonication that are based on the sonication energy of the procedure and therefore on the instrument used. In Fig. 2.2 the two diﬀerent procedures are schematically reported: the strong procedure is based on the use of a sonicating probe, while the weak procedure is based on the use of a simple water bath sonicator. Generally, the water bath sonicator is cheaper than the sonicating probe. To obtain an eﬃcacious dispersion, the power output of the sonicator is not relevant, as well as the sonication times, but is more important the sonication energy. Particular attention must be paid to the ultrasonication procedures, as, at high energies, this treatment can provoke damages on the CNTs and therefore lead to
30 Dispersion Techniques of Nanoinclusions in Cement Matrixes
Figure 2.2 Schematic representations of the two ultrasonication methods: strong with a probe immerged in the sample (left) and weak with the sample in a sonicating bath (right).
a loss and/or change of their properties. These damages can be the opening of the CNT rolls or cracks in the CNTs. There are two cavitation processes that an ultrasonication treatment can provoke on CNTs’ bundles or ﬁbers: stable and inertial. The stable process modiﬁes the chemical surface of the CNTs. and the inertial process is a simple exfoliation of the ﬁbers. A proper treatment of the CNT–solvent system (in terms of the sonication energy, times, and the CNTs used) must be applied in order to obtain the desired eﬀects. Many spectroscopic techniques can be used to evaluate the eﬀect of the ultrasonication on CNT suspensions, and particularly eventual damages on the CNT structures. Raman spectroscopy, atomic force microscopy (AFM), scanning electron microscopy (SEM), transmission electron microscopy (TEM), and ultraviolet-visible (UV-Vis) spectroscopy are successfully applied in the literature to evaluate the integrity of samples, and some of these techniques are also nondestructive [30–33]. The ultrasonication method is successfully applied also in combination with dispersing agents such as surfactants ; this is one of the cases of mixed physical-chemical techniques. This method has many advantages because the ﬁbers of CNTs can be opened or exfoliated by ultrasonication and the additive can eﬃcaciously interact with the CNT surfaces. This procedure will be better discussed later in this chapter, because it represents one of the most relevant techniques for CNT dispersion.
Dispersion Techniques of Carbon Nanotubes 31
2.2.2 Chemical Methods for CNT Dispersion The chemical methods are based on the use of synthetic molecules as additives or on the proper covalent functionalization of the CNTs’ surface in order to obtain an eﬀective dispersion of the CNTs in the solvent. These methods are often helped by the use of other physical methods that permit the exfoliation of the CNTs’ ﬁbers. The covalent methods are various, and they can be classiﬁed in terms of the class of the molecules used for the functionalization. Some examples of the most commonly used inorganic function alization methods are: • Ozone, peroxides, oxides, and strong acids. These are used to functionalize the CNTs’ surface to give oxygen derivatives. This functionalization prevents the folding of the CNTs into ﬁbers and increases the dispersion capabilities in diﬀerent solvents, depending on the hydrophobicity/hydrophilicity of the attached residue [35, 36]. • Decoration of the CNTs with quantum dots. This leads also to eﬃcient use as ﬂuorescent nanoprobes . • Metals, metal nanoparticles, and ions that prevent the folding into ﬁbers into ﬁbers and increase hydrophilicity . Some examples of the use of organic additives/functionalization are represented by: • Covalent functionalization with alkyl groups that leads to easy dispersion in organic media  • Binding/covalent binding of aromatic molecules that also possess optical properties for “smart functionalization”  • Surfactants
18.104.22.168 Surfactants: structure, properties, and solubilizing capabilities Surfactants are a class of organic molecules that are formed by two separate and diﬀerent portions: a hydrophobic one and a hydrophilic one. The smart properties of this class of molecules are due to these peculiar chemical structures [41, 42]. These molecules are also called “amphiphiles.” In Fig. 2.3 is reported a
32 Dispersion Techniques of Nanoinclusions in Cement Matrixes
Figure 2.3 (Top) Schematic representation of a surfactant with the hydrophobic portion (tail) and the hydrophilic portion (head). (Bottom) Cetyltrimethylammonium bromide (CTAB) chemical structure.
schematic representation of the chemical structure of a surfactant and an example of one of the most used molecule of this class, cetyltrimethylammonium bromide (CTAB). The presence in their structures of both polar and nonpolar portions leads to easy solubilization of these molecules both in polar (such as water) and nonpolar solvents. The increase of their concentration in solution leads to a self-aggregation process; this reduces the interactions between the solvent and the diﬀerently structured portions, leading to micelle formation [43, 44]. This phenomenon occurs at a concentration that is speciﬁc for every surfactant, which is called critical micellar concentration (CMC). This value depends on the structural features of the surfactant, particularly on its hydrophobicity. Micelles are nanoscaled spherical aggregates of molecules of surfactants that are spontaneously formed in order to reduce the contacts between the hydrophobic portions and water or between the hydrophilic portions with apolar solvents. In Fig. 2.4 are reported the structures of a micelle (surfactants in water) and of a reverse micelle (surfactants in apolar/hydrophobic solvents). The formation of these aggregates is spontaneous because they are energetically favored due to the high reduction of the repulsions between the solvent and the opposite-structured portions. The spherical structures, in fact, can “hide” from the solvent the portions of the molecules that are nonsimilar to it . The increase of the
Dispersion Techniques of Carbon Nanotubes 33
Figure 2.4 Schematic representations of micellar aggregate in water (left) and reverse micellar aggregate in organic/apolar solvents (right).
dimensions of hydrophobic portions in the surfactant molecules decreases the value of the CMC because the process is more favored. The name “surfactant” derives from a contraction of the terms SURFace ACTing AgeNTS: this is because these molecules have interfacial properties. In water they arrange on the surface, exposing the hydrophobic tail over it and the polar head in water, determining a decrease of surface tension . The amphiphilic properties of these compounds permit to solubilize organic compounds in water and/or polar compounds in organic solvents. This is because the solute can interact with a speciﬁc portion of these molecules, while the other portion can interact eﬃcaciously with the solvent, leading to a solubilization eﬀect. This process can be accomplished by the monomers of surfactants or by the micellar aggregates that can be interpreted as vectors for solubilization . The solubilization of greasy or organic materials by surfactants is responsible of the cleansing properties of the commonly used soaps, which can solubilize eﬃcaciously oil material in water . Surfactants can be classiﬁed into diﬀerent types, depending on the structure of the polar head (that can be negatively or positively charged with a counterion or that can be neutral or zwitterionic) or of the number of heads and hydrophobic portions (gemini or twin chain surfactants). The properties, and therefore the applications,
34 Dispersion Techniques of Nanoinclusions in Cement Matrixes
of these molecules can drastically change by small changes in their structures . Due to their structural features, and due to their properties that can be easily modulated by simple chemical changes, the surfactants ﬁnd a wide range of applications. They can act as gel supramolecular assemblies by the intercalation of organic molecules inside the micellar aggregates [48, 49]; they can act as biocides, or they can act as vector agents of water-insoluble drugs of for DNA, thanks to the structural similarity with the phospholipids of biological membranes [50–52]; they can act as general solubilizing agents to permit synthetic processes in a water solvent ; and they permit to obtain novel organic liquids with high solubilizing capabilities [54, 55]. Thanks to these properties, CNTs’ dispersion in water is successfully accomplished by surfactants.
2.3 Dispersion of Carbon Nanotubes in Water with Surfactants: Similia Similibus Solvuntur (with the Help of Ultrasonication) Widely used for “oil in water” and “water in oil” dispersions, surfactants are commonly used for CNT dispersions in water, both single-walled and multiwalled CNTs [56, 57]. The interactions between surfactant molecules and CNTs are based on the principle similia similibus solvuntur: a Latin phrase that means that similar substances will dissolve similar substances, or “like dissolves like.” In the case of surfactants, their two parts (in terms of their diﬀerent hydrophobicity/hydrophilicity) permit to solubilize/disperse hydrophobic solutes or molecules in polar solvents (such as water) and vice versa (Fig. 2.5). The interactions between surfactants and CNTs occur at the surfaces of the tubes: CNTs are hydrophobic; therefore the am phiphiles can interact with them with their hydrophobic tails. The polar (and often charged) headgroups of the surfactants therefore permit this CNT–surfactant aggregate to be easily dispersed in water for the favored ion–water interactions . The CNTs therefore
Dispersion of Carbon Nanotubes in Water with Surfactants 35
Figure 2.5 Aﬃnity of the two portions of a surfactant with hydrophobic CNTs (with the tail) and with water (with the headgroup).
Figure 2.6 Schematic representation of the coating of a CNT’s surface with monomers of surfactants.
result as functionalized with polar and/or charged groups on their surfaces. Even if the use of surfactants is a chemical method, these interactions are noncovalent. In Fig. 2.6 is reported a scheme of interaction between CNTs and monomers of surfactants. The experimental procedures developed in the literature for CNTs’ dispersion in water with surfactants are also based on
36 Dispersion Techniques of Nanoinclusions in Cement Matrixes
Figure 2.7 Schematic representation of the eﬀect of ultrasonication on CNT bundles (opening of the ﬁbers, reversible after variable times) and of surfactants on CNTs’ surfaces (coating, prevention of reaggregation in ﬁbers).
the use of ultrasonication processes; therefore the methods can be considered mixed physical/chemical ones [34, 59, 60]. This dual technique permits an eﬃcacious dispersion of CNTs: ﬁrst the ultrasonication opens the bundles to give isolated CNTs, and then the surfactants can interact with the surfaces of the dispersed CNTs. The charged surfaces avoid these functionalized nanostructures to spontaneously reaggregate in ﬁbers because of the equal charges’ repulsions . Single CNTs can in fact reaggregate because of the van der Waals forces between the tubes that provoke the ﬁber formation in water. These structures are also smaller than the aggregated structures, so they can be easily dispersed. In Fig. 2.7 the schematic representation of a CNT’s dispersion thanks to ultrasonication and surfactants is shown. This procedure is eﬃcaciously used applying ultrasonication on the samples of CNT– surfactants in water. The surfaces of the CNTs, coated by these charged species, can possess diﬀerent properties, and this could also help further functionalization of the CNTs, if needed [60, 62].
2.3.1 Optimization of CNT Dispersion with Surfactants A knowledge of the chemistry of surfactants is needed in order to obtain eﬃcacious and stable CNT dispersions in water and therefore their use in many applications where these dispersions are needed . The ﬁrst parameter that must be considered is the surfactants’ concentration. The surfactants can interact with the surface of CNTs as monomers, as micellar aggregates, or by forming aggregates on
Dispersion of Carbon Nanotubes in Water with Surfactants 37
Figure 2.8 Most common commercially available surfactants used in the literature for CNTs’ dispersion. Anionic: (a) sodium dodecyl sulfate (SDS) and (b) sodium dodecylbenzenesulfonate (SDBS). Cationic: (c) cetyltrimethylammonium bromide (CTAB) and (d) dodecyltrimethylammo nium bromide (DTAB). Non-ionic: (e) Brij, (f) Tween, and (g) Triton X.
their surfaces; these interactions can occur even simultaneously, and they can depend also on the molecular structure of the surfactant used. The concentration of surfactants needed to obtain eﬃcacious surfactant–CNT interactions is generally lower than their CMC. Moreover, the absence of micellar aggregates at concentrations higher than their CMC is evidence of interaction of the monomers with the CNTs: the molecules are involved in the interactions with the tubes’ surfaces and cannot form micellar aggregates. An excess of surfactants can also provoke a ﬂocculation of CNTs that favors their precipitation . The temperature also plays an important role in the eﬃcacious dispersions as lower temperatures can obviously decrease the dispersion capabilities of the technique . The most important parameter that must be considered in this topic is represented by the surfactant chemical structure.
22.214.171.124 Commercially available surfactants for CNT dispersions In the literature many commercially available surfactants are used for the dispersion of CNTs in water . In Fig. 2.8 are reported the structures of the most commonly used amphiphiles in this topic.
38 Dispersion Techniques of Nanoinclusions in Cement Matrixes
Cationic, anionic, and non-ionic amphiphiles are used in this topic for their ability to disperse CNTs in water with the help of ultrasonication processes. By tailoring the surfactant headgroup type or size or by enhancements in the hydrophobicity of the tails, it is possible to provoke diﬀerent capabilities of dispersion of the nanotubes; this is because the diﬀerent structures can give diﬀerent interactions, or more eﬃcacious ones, with the CNTs’ surface. The most used anionic surfactants in this ﬁeld are sodium dodecyl sulfate (SDS) and sodium dodecylbenzenesulfonate (SDBS) [66, 67]. SDBS has an aromatic ring in its hydrophobic portion that increases the interaction with the aromatic surfaces of CNTs and therefore increases the amount of dispersed CNTs . CTAB and dodecyltrimethylammonium bromide (DTAB) are commonly used cationic commercially available surfactants and they were successfully used in this topic [68, 69]. Their solubilizing properties are similar, even though they diﬀer in terms of their hydrophobic tail length. In the class of non-ionic surfactants, the molecular weight of the amphiphile is relevant in order to evaluate the eﬃcacy in CNTs’ dispersion [70, 71]. This could be explained for an eﬀect of steric stabilization of “bigger” surfactants on CNTs’ surfaces; this avoids the reorganization in ﬁbers of the CNTs . There are also many works reporting the eﬃcacy of mixtures of diﬀerent amphiphiles and water-soluble polymers for CNTs’ dispersions in water [72, 73]. The properties of the mixtures of surfactants (and the properties of these aggregates) are peculiar, and they do not correlate with the properties of the single amphiphiles composing them. In some cases (mixtures of cationic and anionic amphiphiles), charge neutralization phenomena of diﬀerently charged amphiphiles could occur, and this changes the amphiphile properties and the properties of the aggregates. Commercially available amphiphiles are eﬃcaciously used in the literature of this topic; however, due to the low number of commercially available amphiphiles and due to the small changes in their structures, it is not still possible to determine structure– activity relationships of the eﬃcacy of the surfactants in the CNTs’ dispersion with the use of commercially available molecules. The available molecules studied are in fact not properly structured in
Dispersion of Carbon Nanotubes in Water with Surfactants 39
Figure 2.9 Schematic representation of a two-headed and two-tailed gemini surfactant linked with a spacer (left). Chemical structure of 2,5 dimethoxy-1,4-bis[N-(n-dodecyl)-N,N-dimethylammoniomethyl]phenyl bromide [pXMo(DDA)2Br].
order to evaluate the most eﬀective portions of them involved in the CNTs’ dispersion.
126.96.36.199 Increasing CNT dispersion with the use of properly designed surfactants The use of speciﬁcally designed and synthesized surfactants can increase the advantages of the use of these molecules with very simple synthetic procedures. The synthesis of surfactants, in fact, is often very easy and involves few passages from the starting materials . Small changes in the chemical structures of surfac tants can lead to dramatic changes in their properties; therefore the design, the realization, and the structure–activity relationships that could be achieved are fundamental for the increase of the eﬀectiveness of these molecules and therefore of the entire process where amphiphiles are involved. A few papers have been up to now reported in the literature about the use of synthetic surfactants in the dispersion of CNTs in water, but the results are interesting and promising . Many papers are about the use of gemini synthetic surfactants: double headed and double-tailed structures with a linker between the headgroups (Fig. 2.9). Gemini surfactants have about twice the molecular weight of the correspondent single-chain amphiphiles, but their properties are often more than twice eﬀective than them . The use of a gemini surfactant in CNTs dispersions in water has eﬃcacious
40 Dispersion Techniques of Nanoinclusions in Cement Matrixes
results, as reported in many diﬀerent papers in the literature, and this is because of the increase of hydrophobicity of the amphiphiles (as well as the case of non-ionic surfactants) and because of speciﬁc interactions occurring between the amphiphile and the CNTs’ surface . The aromatic rings often present in these structures (in the spacers between the heads or on the hydrophobic tails) promote the interaction/association of the monomers on the aromatic surfaces of CNTs (similia similibus solvuntur). Here are some relevant examples of the use of gemini am phiphiles. Di Crescenzo and co-workers used synthetic gemini surfactants with aromatic portions in the spacers and obtained dispersions with a surfactant–CNT ratio four to seven times lower than commercially available CTAB, SDS, and SDBS amphiphiles . Liu and co-workers used imidazolium-based gemini surfac tants and increased the dispersions of CNTs using 0.1 mg/mL solutions of amphiphiles . Chen and co-workers revealed that only 0.6 wt% of a gemini surfactant can lead to 0.5 wt% of multiwalled CNT dispersions . In this ﬁeld of the dispersion of CNTs in water with surfactants, the use of synthetic amphiphiles could open for the realization of an optimal molecule for the purpose.
References 1. Iijima, S. (1991). Helical microtubules of graphitic carbon, Nature, 354, p. 56. 2. Iijima, S., Ichihashi, T. (1993). Single-shell carbon nanotubes of 1-nm diameter, Nature, 363, pp. 603–605. 3. Peng, X., Wong, S. S. (2009). Functional covalent chemistry of carbon nanotube surfaces, Adv. Mater., 21, pp. 625–642. 4. Pumera, M., Merkoc¸i, A., Alegret, S. (2007). Carbon nanotube detectors for microchip CE: comparative study of single-wall and multiwall carbon nanotube, and graphite powder ﬁlms on glassy carbon, gold, and platinum electrode surfaces, Electrophoresis, 28, pp. 1274–1280. 5. Bandyopadhyaya, R., Nativ-Roth, E., Regev, O., Yerushalmi-Rozen, R. (2002). Stabilization of individual carbon nanotubes in aqueous solutions, Nano Lett., 2, pp. 25–28.
6. Vigolo, B., Penicaud, A., Coulon, C., Sauder, C., Pailler, R., Journet, C.,
Bernier, P., Poulin, P. (2000). Macroscopic ﬁbers and ribbons of oriented
carbon nanotubes, Science (80-), 290, pp. 1331–1334.
7. Hutchison, J. L., Kiselev, N. A., Krinichnaya, E. P., Krestinin, A. V., Loutfy, R.
O., Morawsky, A. P., Muradyan, V. E., Obraztsova, E. D., Sloan, J., Terekhov,
S. V. (2001). Double-walled carbon nanotubes fabricated by a hydrogen
arc discharge method, Carbon N.Y ., 39, pp. 761–770.
8. Sugai, T., Yoshida, H., Shimada, T., Okazaki, T., Shinohara, H., Bandow, S.
(2003). New synthesis of high-quality double-walled carbon nanotubes
by high-temperature pulsed arc discharge, Nano Lett., 3, pp. 769–
773. 9. Sakakibara, Y., Tatsuura, S., Kataura, H., Tokumoto, M., Achiba, Y.
(2003). Near-infrared saturable absorption of single-wall carbon
nanotubes prepared by laser ablation method, Jpn. J. Appl. Phys., 42,
10. Yu, D. P., Sun, X. S., Lee, C. S., Bello, I., Lee, S. T., Gu, H. D., Leung, K. M., Zhou, G. W., Dong, Z. F., Zhang, Z. (1998). Synthesis of boron nitride nanotubes by means of excimer laser ablation at high temperature, Appl. Phys. Lett., 72, pp. 1966–1968. 11. Stankovich, S., Dikin, D. A., Dommett, G. H. B., Kohlhaas, K. M., Zimney, E. J., Stach, E. A., Piner, R. D., Nguyen, S. T., Ruoﬀ, R. S. (2006). Graphene based composite materials, Nature, 442, pp. 282–286. 12. Jiang, K., Li, Q., Fan, S. (2002). Nanotechnology: spinning continuous carbon nanotube yarns, Nature, 419, p. 801. 13. Zhang, Y., Bai, Y., Yan, B. (2010). Functionalized carbon nanotubes for potential medicinal applications, Drug Discov. Today, 15, pp. 428–435. 14. Cellot, G., Cilia, E., Cipollone, S., Rancic, V., Sucapane, A., Giordani, S., Gambazzi, L., Markram, H., Grandolfo, M., Scaini, D. (2009). Carbon nanotubes might improve neuronal performance by favouring electrical shortcuts, Nat. Nanotechnol., 4, pp. 126–133. 15. Movia, D., Prina-Mello, A., Bazou, D., Volkov, Y., Giordani, S. (2011). Screening the cytotoxicity of single-walled carbon nanotubes using novel 3D tissue-mimetic models, ACS Nano, 5, pp. 9278–9290. 16. Li, C., Chou, T.-W. (2003). Elastic moduli of multi-walled carbon nanotubes and the eﬀect of van der Waals forces, Compos. Sci. Technol., 63, pp. 1517–1524. 17. Bahr, J. L., Mickelson, E. T., Bronikowski, M. J., Smalley, R. E., Tour, J. M. (2001). Dissolution of small diameter single-wall carbon nanotubes in organic solvents? Chem. Commun., pp. 193–194.
42 Dispersion Techniques of Nanoinclusions in Cement Matrixes
18. Shimoda, H., Oh, S. J., Geng, H. Z., Walker, R. J., Bin Zhang, X., McNeil, L. E., Zhou, O. (2002). Self-assembly of carbon nanotubes, Adv. Mater., 14, p. 899. 19. Martel, R., Shea, H. R., Avouris, P. (1999). Rings of single-walled carbon nanotubes, Nature, 398, p. 299. http://dx.doi.org/10.1038/18589 20. Premkumar, T., Mezzenga, R., Geckeler, K. E. (2012). Carbon nanotubes in the liquid phase: addressing the issue of dispersion, Small, 8, pp. 1299– 1313. 21. Munkhbayar, B., Nine, M. J., Jeoun, J., Bat-Erdene, M., Chung, H., Jeong, H. (2013). Inﬂuence of dry and wet ball milling on dispersion characteristics of the multi-walled carbon nanotubes in aqueous solution with and without surfactant, Powder Technol., 234, pp. 132– 140. 22. Lee, J.-H., Rhee, K.-Y. (2010). A study on the dispersion characteristics of carbon nanotubes using cryogenic ball milling process, J. Korean Soc. Precis. Eng., 27, pp. 49–54. 23. Cho, S.-J., Shrestha, S. P., Lee, S.-B., Boo, J.-H. (2014). Electrical characteristics of carbon nanotubes by plasma and microwave surface treatments, Bull. Korean Chem. Soc., 35, pp. 905–907. 24. Wang, Y., Iqbal, Z., Mitra, S. (2005). Microwave-induced rapid chemical functionalization of single-walled carbon nanotubes, Carbon N. Y., 43, pp. 1015–1020. 25. Li, Y., Mann, D., Rolandi, M., Kim, W., Ural, A., Hung, S., Javey, A., Cao, J., Wang, D., Yenilmez, E. (2004). Preferential growth of semiconducting single-walled carbon nanotubes by a plasma enhanced CVD method, Nano Lett., 4, pp. 317–321. 26. Chen, W., Liu, X., Liu, Y., Kim, H.-I. (2010). Novel synthesis of self assembled CNT microcapsules by O/W Pickering emulsions, Mater. Lett., 64, pp. 2589–2592. 27. Choi, Y. C., Shin, Y. M., Lee, Y. H., Lee, B. S., Park, G.-S., Choi, W. B., Lee, N. S., Kim, J. M. (2000). Controlling the diameter, growth rate, and density of vertically aligned carbon nanotubes synthesized by microwave plasma enhanced chemical vapor deposition, Appl. Phys. Lett., 76, pp. 2367– 2369. 28. Caneba, G. T., Dutta, C., Agrawal, V., Rao, M. (2010). Novel ultrasonic dispersion of carbon nanotubes, J. Miner. Mater. Charact. Eng., 9, p. 165. 29. Tarasov, V. A., Komkov, M. A., Stepanishchev, N. A., Romanenkov, V. A., Boyarskaya, R. V. (2015). Modiﬁcation of polyester resin binder by
carbon nanotubes using ultrasonic dispersion, Polym. Sci. Ser.D, 8, pp. 9–16. 30. Osswald, S., Havel, M., Gogotsi, Y. (2007). Monitoring oxidation of multiwalled carbon nanotubes by Raman spectroscopy, J. Raman Spectrosc., 38, pp. 728–736. 31. Hafner, J. H., Cheung, C.-L., Woolley, A. T., Lieber, C. M. (2001). Structural and functional imaging with carbon nanotube AFM probes, Prog. Biophys. Mol. Biol., 77, pp. 73–110. 32. Yuzvinsky, T. D., Fennimore, A. M., Mickelson, W., Esquivias, C., Zettl, A. (2005). Precision cutting of nanotubes with a low-energy electron beam, Appl. Phys. Lett., 86, p. 53109. 33. Grossiord, N., Regev, O., Loos, J., Meuldijk, J., Koning, C. E. (2005). Time dependent study of the exfoliation process of carbon nanotubes in aqueous dispersions by using UV- visible spectroscopy, Anal. Chem., 77, pp. 5135–5139. 34. Strano, M. S., Moore, V. C., Miller, M. K., Allen, M. J., Haroz, E. H., Kittrell, C., Hauge, R. H., Smalley, R. E. (2003). The role of surfactant adsorption during ultrasonication in the dispersion of single-walled carbon nanotubes, J. Nanosci. Nanotechnol., 3, pp. 81–86. 35. Wiggins-Camacho, J. D., Stevenson, K. J. (2011). Mechanistic discussion of the oxygen reduction reaction at nitrogen-doped carbon nanotubes, J. Phys. Chem. C, 115, pp. 20002–20010. 36. Banerjee, S., Hemraj-Benny, T., Wong, S. S. (2005). Covalent surface chemistry of single-walled carbon nanotubes, Adv. Mater., 17, pp. 17– 29. 37. Bottini, M., Cerignoli, F., Dawson, M. I., Magrini, A., Rosato, N., Mustelin, T. (2006). Full-length single-walled carbon nanotubes decorated with streptavidin-conjugated quantum dots as multivalent intracellular ﬂuorescent nanoprobes, Biomacromolecules, 7, pp. 2259–2263. 38. Satishkumar, B. C., Vogl, E. M., Govindaraj, A., Rao, C. N. R. (2003). The decoration of carbon nanotubes by metal nanoparticles, in Adv. Chem. A Sel. CNR Rao’s Publ., World Scientiﬁc, pp. 292–295. 39. Chen, S., Shen, W., Wu, G., Chen, D., Jiang, M. (2005). A new approach to the functionalization of single-walled carbon nanotubes with both alkyl and carboxyl groups, Chem. Phys. Lett., 402, pp. 312–317. 40. Liu, A., Honma, I., Ichihara, M., Zhou, H. (2006). Poly (acrylic acid) wrapped multi-walled carbon nanotubes composite solubilization in water: deﬁnitive spectroscopic properties, Nanotechnology, 17, p. 2845.
44 Dispersion Techniques of Nanoinclusions in Cement Matrixes
¨ 41. Holmberg, K., Jonsson, B., Kronberg, B., Lindman, B. (2002). Surfactants and Polymers in Aqueous Solution, Wiley Online Library. 42. Rosen, M. J., Kunjappu, J. T. (2012). Surfactants and Interfacial Phenomena, John Wiley & Sons. ¨ H. (1980). Micelles, Micelles, pp. 1–83. 43. Lindman, B., Wennerstrom, 44. Hoﬀmann, H., Ebert, G. (1988). Surfactants, micelles and fascinating phenomena, Angew. Chemie Int. Ed., 27, pp. 902–912. 45. Ray, A. (1971). Solvophobic interactions and micelle formation in structure forming nonaqueous solvents, Nature, 231, pp. 313– 315. 46. Edwards, D. A., Luthy, R. G., Liu, Z. (1991). Solubilization of polycyclic aromatic hydrocarbons in micellar nonionic surfactant solutions, Environ. Sci. Technol., 25, pp. 127–133. 47. Menger, F. M., Keiper, J. S. (2000). Gemini surfactants, Angew. Chem. Int. Ed., 39, pp. 1906–1920. 48. Kumar, R., Ketner, A. M., Raghavan, S. R. (2009). Nonaqueous photorhe ological ﬂuids based on light-responsive reverse wormlike micelles, Langmuir, 26, pp. 5405–5411. 49. Baglioni, P., Braccalenti, E., Carretti, E., Germani, R., Goracci, L., Savelli, G., Tiecco, M. (2009). Surfactant-based photorheological ﬂuids: eﬀect of the surfactant structure, Langmuir, 25, pp. 5467–5475. 50. Shaban, S. M., Saied, A., Tawﬁk, S. M., Abd-Elaal, A., Aiad, I. (2013). Corrosion inhibition and biocidal eﬀect of some cationic surfactants based on Schiﬀ base, J. Ind. Eng. Chem., 19, pp. 2004–2009. 51. Far´ıas, T., De Menorval, L.-C., Zajac, J., Rivera, A. (2009). Solubilization of drugs by cationic surfactants micelles: conductivity and 1 H NMR experiments, Colloids Surf., A, 345, pp. 51–57. 52. Corte, L., Tiecco, M., Roscini, L., De Vincenzi, S., Colabella, C., Germani, R., Tascini, C., Cardinali, G. (2015). FTIR metabolomic ﬁngerprint reveals diﬀerent modes of action exerted by structural variants of N alkyltropinium bromide surfactants on Escherichia coli and Listeria innocua cells, PLoS One, 10(1), p. e0115275. 53. Antonietti, M., Wenz, E., Bronstein, L., Seregina, M. (1995). Synthesis and characterization of noble metal colloids in block copolymer micelles, Adv. Mater., 7, pp. 1000–1005. 54. Cardellini, F., Germani, R., Cardinali, G., Corte, L., Roscini, L., Spreti, N., Tiecco, M. (2015). Room temperature deep eutectic solvents of (1S) (+)-10-camphorsulfonic acid and sulfobetaines: hydrogen bond-based
mixtures with low ionicity and structure-dependent toxicity, RSC Adv., 5, pp. 31772–31786. 55. Bowers, J., Vergara-Gutierrez, M. C., Webster, J. R. P. (2004). Surface ordering of amphiphilic ionic liquids, Langmuir, 20, pp. 309–312. 56. Wang, H., Zhou, W., Ho, D. L., Winey, K. I., Fischer, J. E., Glinka, C. J., Hobbie, E. K. (2004). Dispersing single-walled carbon nanotubes with surfactants: a small angle neutron scattering study, Nano Lett., 4, pp. 1789–1793. 57. Matarredona, O., Rhoads, H., Li, Z., Harwell, J. H., Balzano, L., Resasco, D. E. (2003). Dispersion of single-walled carbon nanotubes in aqueous solutions of the anionic surfactant NaDDBS, J. Phys. Chem. B, 107, pp. 13357–13367. 58. Vaisman, L., Wagner, H. D., Marom, G. (2006). The role of surfactants in dispersion of carbon nanotubes, Adv. Colloid Interface Sci., 128, pp. 37– 46. 59. Li, J., Ma, P. C., Chow, W. S., To, C. K., Tang, B. Z., Kim, J. (2007). Correlations between percolation threshold, dispersion state, and aspect ratio of carbon nanotubes, Adv. Funct. Mater., 17, pp. 3207–3215. 60. Ma, P.-C., Siddiqui, N. A., Marom, G., Kim, J.-K. (2010). Dispersion and functionalization of carbon nanotubes for polymer-based nanocompo sites: a review, Composite Part A, 41, pp. 1345–1367. 61. Jiang, L., Gao, L., Sun, J. (2003). Production of aqueous colloidal dispersions of carbon nanotubes, J. Colloid Interface Sci., 260, pp. 89–94. 62. Sahoo, N. G., Cheng, H. K. F., Cai, J., Li, L., Chan, S. H., Zhao, J., Yu, S. (2009). Improvement of mechanical and thermal properties of carbon nanotube composites through nanotube functionalization and processing methods, Mater. Chem. Phys., 117, pp. 313–320. 63. Rastogi, R., Kaushal, R., Tripathi, S. K., Sharma, A. L., Kaur, I., Bharadwaj, L. M. (2008). Comparative study of carbon nanotube dispersion using surfactants, J. Colloid Interface Sci., 328, pp. 421–428. 64. Ham, H. T., Choi, Y. S., Chung, I. J. (2005). An explanation of dispersion states of single-walled carbon nanotubes in solvents and aqueous surfactant solutions using solubility parameters, J. Colloid Interface Sci., 286, pp. 216–223. 65. Moore, V. C., Strano, M. S., Haroz, E. H., Hauge, R. H., Smalley, R. E., Schmidt, J., Talmon, Y. (2003). Individually suspended single-walled carbon nanotubes in various surfactants, Nano Lett., 3, pp. 1379–1382.
46 Dispersion Techniques of Nanoinclusions in Cement Matrixes
66. Brege, J. J., Gallaway, C., Barron, A. R. (2007). Fluorescence quenching of single-walled carbon nanotubes in SDBS surfactant suspension by metal ions: quenching eﬃciency as a function of metal and nanotube identity, J. Phys. Chem. C, 111, pp. 17812–17820. 67. Tummala, N. R. (2009). SDS surfactants on carbon nanotubes: aggregate morphology, ACS Nano, 3, pp. 595–602. 68. Bai, Y., Park, I. S., Lee, S. J., Bae, T. S., Watari, F., Uo, M., Lee, M. H. (2011). Aqueous dispersion of surfactant-modiﬁed multiwalled carbon nanotubes and their application as an antibacterial agent, Carbon N. Y., 49, pp. 3663–3671. 69. Hu, C., Xu, Y., Duo, S., Zhang, R., Li, M. (2009). Non-covalent functionaliza tion of carbon nanotubes with surfactants and polymers, J. Chin. Chem. Soc., 56, pp. 234–239. 70. Chen, R. J., Bangsaruntip, S., Drouvalakis, K. A., Kam, N. W. S., Shim, M., Li, Y., Kim, W., Utz, P. J., Dai, H. (2003). Noncovalent functionalization of carbon nanotubes for highly speciﬁc electronic biosensors, Proc. Natl. Acad. Sci., 100, pp. 4984–4989. 71. Cui, S., Canet, R., Derre, A., Couzi, M., Delhaes, P. (2003). Characterization of multiwall carbon nanotubes and inﬂuence of surfactant in the nanocomposite processing, Carbon N. Y., 41, pp. 797–809. 72. Madni, I., Hwang, C.-Y., Park, S.-D., Choa, Y.-H., Kim, H.-T. (2010). Mixed surfactant system for stable suspension of multiwalled carbon nanotubes, Colloids Surf., A, 358, pp. 101–107. 73. O’Connell, M. J., Boul, P., Ericson, L. M., Huﬀman, C., Wang, Y., Haroz, E., Kuper, C., Tour, J., Ausman, K. D., Smalley, R. E. (2001). Reversible water solubilization of single-walled carbon nanotubes by polymer wrapping, Chem. Phys. Lett., 342, pp. 265–271. 74. Biermann, M., Lange, F., Piorr, R., Ploog, U., Rutzen, H., Schindler, J., Schmid, R. (1987). Synthesis of surfactants, in Falbe, J. (ed.) Surfactants in Consumer Products: Theory, Technology and Applications, SpringerVerlag, Berlin, pp. 23–132. 75. Wang, Q., Han, Y., Wang, Y., Qin, Y., Guo, Z.-X. (2008). Eﬀect of surfactant structure on the stability of carbon nanotubes in aqueous solution, J. Phys. Chem. B, 112, pp. 7227–7233. 76. Zhang, S., Lu, F., Zheng, L. (2011). Dispersion of multiwalled carbon nanotubes (MWCNTs) by ionic liquid-based Gemini pyrrolidinium surfactants in aqueous solution, Colloid Polym. Sci., 289, pp. 1815– 1819.
77. Di Crescenzo, A., Germani, R., Del Canto, E., Giordani, S., Savelli, G., Fontana, A. (2011). Eﬀect of surfactant structure on carbon nanotube sidewall adsorption, Eur. J. Org. Chem., 2011, pp. 5641–5648. 78. Liu, Y., Yu, L., Zhang, S., Yuan, J., Shi, L., Zheng, L. (2010). Dispersion of multiwalled carbon nanotubes by ionic liquid-type Gemini imidazolium surfactants in aqueous solution, Colloids Surf., A, 359, pp. 66–70. 79. Chen, L., Xie, H., Li, Y., Yu, W. (2008). Applications of cationic gemini surfactant in preparing multi-walled carbon nanotube contained nanoﬂuids, Colloids Surf., A, 330, pp. 176–179.
Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation in Composite Cement–Based Sensors Filled with Carbon Black Simon Laﬂammea and Filippo Ubertinib a Department of Civil, Construction, and Environmental Engineering,
Iowa State University, USA b Department of Civil and Environmental Engineering, University of Perugia, Italy laﬂ[email protected]
3.1 Introduction Recent advances in nanomaterials and synthetic metals have led to new possibilities in sensor development [3, 16], including new multifunctional materials that enable substantial improvements in the cost-eﬀectiveness of structural health management solutions for geometrically large systems [11, 22]. In particular, sensors fabricated from cementitious-based nanocomposites have been proposed to fabricate self-sensing mortar, concrete, and asphalt . These materials have great potential at improving structural Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
50 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
safety and resiliency by providing means to continuously monitor cementitious substrates in a non-intrusive manner. Examples of possible applications include self-sensing road pavements, which would signiﬁcantly improve the rapidity of road inspections, non intrusive weigh-in-motion sensors and smart slabs to improve traﬃc management, self-sensing concrete nuclear containment structures to monitor structural health on the internal layer, and smart mortar to monitor health of historic structures exposed to natural hazards . The sensing principle of cementitious sensors leverages their piezoresistive property, where a change in geometry provokes a measurable change in resistance. It is therefore possible to measure static or dynamic strain of cementitious structures, either through contact (e.g., through electrodes) or noncontact (e.g., eddy current) methods. These sensors are ideally fabricated with a level of conductive particles close to the percolation threshold in order to improve the sensor’s sensitivity . Percolation is here deﬁned as the material’s phase transition zone indicated by a signiﬁcant change in its electrical conductivity as a function of the ﬁller content. Several studies have analyzed multifunctional cementitious materials doped with carbon nanoinclusions, including carbon black (CB) [12, 15, 21, 24], carbon ﬁbers [7, 8, 21, 26], and carbon nanotubes (CNTs) [2, 5, 8, 9, 19]. Conductive cementitious materials have been studied and uti lized for a few decades, primarily for de-icing of road infrastructures [17, 23, 25]. Nevertheless, the development of multifunctional cementitious materials for sensing purposes is more complex. This is primarily because the nanocomposite must provide a linear and accurately measurable signal with respect to a change in the measured state. There are fundamental challenges that limit the cost-eﬀective fabrication of large volumes of conductive cementitious materials, namely: • There is a trade-oﬀ between the cost of the selected conductive ﬁller and its conductivity. Lower-conductivity nanoﬁllers such as CB require higher loading, which may signiﬁcantly aﬀect the strength of the nanocomposite. Con versely, higher-conductivity nanoﬁllers such as CNTs require
fewer particles but result in a much higher fabrication cost. • The majority of the proposed conductive cementitious mate rials necessitate a complex fabrication process to ensure ho mogeneous dispersion of nanoparticles , which impedes scalability. This is a problem particularly associated with CNTs that tend to spontaneously agglomerate in bundles due to van der Waals attraction forces . The authors have previously studied the problem of scalability of existing sensing solutions, and research led to CB-based strategies  due to their low cost and ease of dispersion . CB particles are therefore excellent candidates from economical and processing perspectives, although the amount of particle additives required to achieve electrical conductivity is prohibitive (see Wen & Chung  and Li et al.  for instance). Such a high doping content may have detrimental eﬀects on the materials’ strength. Thus, there is a need to develop techniques for assisting the formation of percolating CB networks within cementitious materials, which would decrease the requisite loading. Various studies have reported the interaction of CB with poly mers. For example,  showed that the use of styrene-butadiene styrene to disperse CB particles resulted in a 40% reduction in the percolation threshold.  studied the percolation in composites where polyethylene was mixed with polystyrene, and found that CB was selectively distributed on the polyethylene phase and thus led to reduced percolation thresholds compared to the utilization of monophase polymers as composites. Here, we study the utilization of a block copolymer, namely styrene-ethylene/butylene-styrene (SEBS), to accelerate percolation of CB-ﬁlled cementitious materials, therefore decreasing the requisite loading of ﬁller for the fabrication of cementitious sensors. SEBS is selected because of previous experience in successfully making conductive paint by adding a low amount of CB particles to SEBS. We termed such sensors “SEBS-CB sensors.” The study builds on the results of a preliminary investigation presented in conference proceedings . A more extensive study is presented here to support the hypothesis that SEBS can be used to accelerate percolation of cement paste
52 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
ﬁlled with CB. Also, the fabrication procedure has been updated and validated in order to improve on the dispersion of the SEBS-CB mix. This chapter is organized as follows. Section 3.2 gives details on materials and fabrication processes. Section 3.3 describes the research methodology. Section 3.4 presents and discusses results. Section 3.5 concludes the chapter.
3.2 SEBS-CB Sensors 3.2.1 Materials SEBS-type Mediprene was obtained from VTC Elastoteknik AB, Sweden (density = 930 kg/m3 ). It is a petroleum-based block copolymer widely used for medical applications because of its purity, softness, elasticity, and strength. CB-type Printex XE-2B (2% ash content and 500 ppm sieve residue 45 μm) was acquired from Orion Engineered Carbons (Kingswood, TX). It is characterized by a high structure (minimum oil absorption 380 cc/100g), which facilitates higher conductivity. Copper meshes to form the elec trodes were acquired from McMaster-Carr (Elmhurst, IL). Portland cement type I/II was locally purchased from Ash Grove Cement Company. All materials were utilized as received, except for CB. CB particles were ball-milled for 24 hours to break down agglomerated particles. Figure 3.1 is a magniﬁed picture of the CB particles before and after ball milling. Ball milling resulted in ﬁner particles of more homogeneous geometrical shapes. The average particle size decreased from approximately 900 μm to approximately 45 μm. Such procedure was used to improve on dispersion of CB.
3.2.2 Sensor Fabrication Both SEBS-CB and CB-only sensors were fabricated. CB-only samples were used for benchmark purposes. The fabrication process of CB only sensors is illustrated in Fig. 3.2. The desired levels of CB loadings were weighed and mixed in a high-shear mixer with the
Figure 3.1 milling.
CB particles: (a) before ball milling and (b) after 24 hours of ball
required amount of water needed for a 0.45 water/cement (w/c) ratio. CB particles were mixed in water for 5 minutes in a blender. Cement was then added to CB-water, and mixed for 2 minutes in a Hobart mixer at the highest speed. Samples were then cast in molds of dimensions 5.1 × 5.1 × 5.1 cm3 and vibrated/compacted to eliminate air voids. Two sets of copper mesh electrodes were inserted in each poured sample. The samples were covered with a damp cloth allowed to cure overnight before being demolded and allowed to cure in a curing room at 100% relative humidity at 22◦ C for 7 days. The samples were then air-cured dry for 4 days to let water evaporate. Figure 3.2, step 6 is a picture of a completed CB only sample.
Fabrication process of CB-only sensors.
54 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
Fabrication process of SEBS-CB sensors.
The fabrication process of SEBS-CB sensors is illustrated in Fig. 3.3. SEBS polymer obtained in granular form was ﬁrst dissolved in toluene in the ratio of 60 g of SEBS per 500 mL of toluene. The amount of SEBS used in the fabrication of SEBS-CB samples was governed by the quantity of CB to be added to ensure that the SEBS solution would not be saturated by CB particles. A mass of 3.41 g of SEBS in solution was used for CB loadings up to 0.71% volume, while a mass of 11.37 g of SEBS was used for CB loadings greater than 0.71% volume. CB was added to the SEBS solution in the desired loading amount before the mixture was mixed at high shear for 3 minutes. A neat cement paste mix was prepared by combining cement and water at a 0.45 w/c ratio and mixing for 2 minutes in a Hobart mixer at the highest speed. After, the SEBS-CB conductive paint was incorporated in the neat cement paste with 0.1 g of sodium lauryl sulfate (SLS) per 131 cm3 of materials (volume of one sample), a surfactant used to disperse the petroleum-based conductive paint with water, and mixed for additional 2 minutes in the Hobart mixer. The samples were then poured into molds of dimensions 5.1 × 5.1 × 5.1 cm3 and vibrated/compacted to eliminate air voids. Two sets of copper
mesh electrodes were inserted in each poured sample. The samples were covered with a damp cloth and allowed to cure overnight before being demolded and placed in a curing room at 100% relative humidity and 22◦ C for 48 hours. The samples were air cured for 4 days to develop a polymer microstructure and let water evaporate. Figure 3.3, step 7 is a picture of a completed SEBS-CB sample.
3.3 Methodology 3.3.1 Mix Proportions Cementitious mixes with CB-only and SEBS-only samples were prepared. For CB-only samples, a constant w/c ratio of 0.45 was selected, and mixes were designed for constant volumes of 164 cm3 to produce 25% extra material. The amount of water and cement varied as a function of the quantity of CB added. Table 3.1 lists all diﬀerent CB-only sample types. Three samples per type were fabricated and tested. SEBS-CB sample mixes were also designed to keep a constant w/c ratio of 0.45. For samples containing up to 0.71% CB loading, 15 mL of dissolved SEBS (3.41 g) was added to the mix, which corresponds to a concentration of 9% by volume. The quantity of SEBS was doubled for samples containing more than 0.71% to prevent saturation of CB within the SEBS solution. For SEBS-CB Table 3.1 CB-only samples Sample type (#)
1 2 3 4 5 6 7 8
293 292 291 290 289 286 286 286
0 1.65 3.30 5.00 6.65 9.00 12.0 15.0
651 649 647 645 643 630 630 630
6 6 6 6 6 6 6 6
0.45 0.45 0.45 0.45 0.45 0.45 0.45 0.45
0 0.18 0.36 0.54 0.71 0.96 1.25 1.60
56 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
Table 3.2 SEBS-CB samples Sample type (#)
sensors, only loadings up to 0.96% CB were considered because it was found that samples with 1.25% CB loadings and beyond were diﬃcult to fabricate due to the poor workability of the mix, resulting in heterogeneous dispersions. Table 3.2 lists all diﬀerent SEBS-CB sample types. Three samples per type were fabricated and tested.
3.3.2 Quality Control The quality of dispersion of CB particles was veriﬁed on each sample using thermography. The samples were connected to a 60 V AC current source and placed in an enclosed space. During the electrical loading, a FLIR A35 thermal camera was used to capture thermal images at a rate of approximately one image per second. These images were used to visually inspect the distribution of CB particles that revealed in the form of bright pigments. The thermal image of an electrically unloaded sample is shown in Fig. 3.4a, where the cementitious block shows as a black cube. Figures 3.4b and 3.4c are typical examples of well-dispersed samples containing high levels of CB particles. Both the CB-only sample with 1.60% CB (Fig. 3.4b) and the SEBS-CB sample with 0.71% CB reveal bright pigments that are well distributed over the observable area. Lastly, Fig. 3.4d shows the example of a badly dispersed sample for which the CB particles sank and agglomerated at the bottom. Samples that were judged as badly dispersed (e.g., Fig. 3.4d) were discarded and refabricated.
Figure 3.4 Thermal images of (a) electrically unloaded sample (typical), (b) electrically loaded sample (1.6% CB-only), (c) electrically loaded sample (0.71% SEBS-CB), and (d) electrically loaded sample with bad CB dispersion.
3.3.3 Measurements Tests were conducted to validate the hypothesis that SEBS can be utilized to accelerate percolation of the material and that the resulting conductive cementitious paste can be used as a sensor. First, the percolation curves were obtained by plotting the resistivity of each sample as a function of CB loadings. Three samples were used for each CB loading, and the resistance was measured using an LCR bridge at 100 kHz. Second, the strain-sensing capability and linearity of sensors were evaluated by applying strain on each samples and measuring
58 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
Figure 3.5 Experimental conﬁguration. (a) Cementitious sensor installed in the universal testing machine and (b) zoom on the cementitious sensors.
the change in resistance. The samples were placed in a universal testing machine of type Instron (50 kN capacity), loaded in steps of 40 μ at a rate of 0.0005 in/second up to 400 μ, and then unloaded using the same steps and rate.
3.3.4 Electromechanical Model To develop the electromechanical model, consider a cementitious sensor with two embedded electrodes of embedded width b and height h, spaced by a distance L, subjected to a uniaxial strain (perpendicular to the electrodes) provoking a change in the electrode distance L. The sensor can be modeled as a resistor of resistance R L (3.1) A where ρ is the resistivity of the material and A = b · w the cross section area of the embedded electrodes. Assuming small strain, taking the ﬁnite diﬀerence of Eq. 3.1 yields R=ρ
L A R ρ = + − R ρ L A ρ = + (1 + 2ν)ε ρ
Results and Discussion
with L (3.3) L where ν is the Poisson’s ratio of the material and ε the axial strain. Using Eq. 3.2, an expression for the gauge factor λ can be obtained: ε=
R λ= R ε
(3.4) ρ ρ = (1 + 2ν) + ε The ﬁrst term in Eq. 3.4 represents the change in resistance due to the change in the sensor’s geometry, while the second term represents the piezoresistive eﬀect.
3.4 Results and Discussion This section presents and discusses results on the percolation study, eﬀect of SEBS loading, and strain sensitivity of the cementitious sensors.
3.4.1 Percolation Thresholds Figure 3.6 shows a plot of the resistivity of the sensors as a function of CB loading for both CB-only and SEBS-CB samples. It can be observed that the percolation threshold for CB-only samples is located between 0.71% and 1.25%, while the percolation threshold appears to be located between 0.36% and 0.71% for SEBS-CB samples. This initial comparison of thresholds shows that the utilization of SEBS results in reducing the percolation threshold by approximately 50%. However, samples with SEBS initially have a higher value of resistivity because of the insulating nature of the polymer, and SEBS-CB samples after percolation have a value of resistivity that compares with that of CB-only samples before percolation.
60 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
Resistivity versus CB% for CB-only and SEBS-CB samples.
3.4.2 Strain Sensitivity The relative changes in the sensors’ resistance as a function of strain was studied for samples located around the percolation threshold found in the percolation study. Results are plotted in Figs. 3.7 (CB only samples) and 3.8 (SEBS-CB samples). The slope of the linear ﬁt is the gauge factor λ (or sensitivity) of the sensor to strain. The gauge factor for each sample type is listed in Table 3.3. Results for CB-only samples (Fig. 3.7) show a higher gauge factor for CB-only samples at 0.96% CB, while results for SEBS-CB samples exhibit a higher gauge factor at 0.54%CB loading. Thus, the inclusion of SEBS Table 3.3
Experimental gauge factors λ
0.18% 0.36% 0.54% 0.71% 0.96% 1.25%
25.8 30.8 38 17.7 − −
− − 47.3 82.5 178 17
Results and Discussion
Figure 3.7 Percentage change in resistance vs. CB loading for CB-only samples.
Figure 3.8 samples.
Percentage change in resistance vs. CB loading for CB with SEBS
in the cementitious matrix allows to reach the optimal sensitivity with a lower CB loading, but this optimal gauge factor is signiﬁcantly lower than one obtained through CB-only samples. A comparison of the optimal gauge factors shows that CB-only samples yield a gauge factor (λ = 178) that is 4.7 times higher.
62 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
Also, a closer inspection of the results shows that the CB-only samples exhibit a good linearity, except for the 0.96% loading at low levels of strain, which nonlinearity could be attributed to the piezoresistive eﬀect being more important at low strain levels around the percolation threshold. The SEBS-CB samples show higher nonlinearities. While the piezoresistive eﬀect may also explain the nonlinearity at low strain levels, it is possible that the capacitance of the material is also aﬀected by strain. Lastly, the presence of the polymer may create a signiﬁcant hysteresis, which can also be observed in Fig. 3.8. The modeling of the nonlinearities in the SEBS-CB samples is left to future work. While the SEBS-CB samples underperform the CB-only samples in terms of gauge factor and linearity, results from this section demonstrate that the inclusion of SEBS in the cementitious mix results in reducing the location of the percolation threshold.
3.5 Conclusion This chapter investigated the use of SEBS to accelerate percolation of cementitious composites ﬁlled with CB particles. While CB is an inexpensive conductive ﬁller, it is less conductive compared to the more expensive counterparts such as CNTs. It results that a larger amount of CB particles is necessary to reach the percolation threshold, which provides a sensor with high level of sensitivity. However, using a large amount of conductive ﬁllers may result in a signiﬁcant loss in the material’s mechanical properties such as strength. The motivation of the research was to create optimally sensitive cementitious sensors with a smaller amount of conductive particles, therefore maintaining good mechanical properties. Conductive cement paste sensors were fabricated with SEBS mixed with various concentrations of CB particles (SEBS-CB). The resistivity of each sample was measured for each concentration, which was used to ﬁnd the percolation threshold. Results were compared with conductive cement paste sensors fabricated without SEBS (CB-only). It was found that the utilization of SEBS reduced the
percolation threshold by approximately 50%. However, percolated SEBS-CB samples yielded a resistivity similar to the CB-only samples before percolation, attributed to the insulating nature of SEBS. The sensitivity or gauge factor of specimens around the percolation threshold was investigated by measuring the change in electrical resistance as a function of applied strain. Results show that a concentration of 0.54% of CB resulted in an optimal gauge factor of 38 for SEBS-CB samples, while this concentration was 0.86% for CB-only samples, yet yielding a gauge factor of 178. This result conﬁrmed that SEBS could be used to accelerate the percolation of the material. However, the optimal gauge factor of SEBS-CB sensors is signiﬁcantly smaller than the optimal gauge factor of CB-only sensors. In addition, an investigation of the linearity of the sensors showed that SEBS-CB samples were signiﬁcantly nonlinear compared to CB-only samples. Several factors were listed to explain the nonlinearity, including the piezoresistive eﬀect at low levels of strain, the nonnegligible participation of the material’s capacitance, and the hysteresis generated by the use of a polymer. This study demonstrated the promise of SEBS for fabricating cementitious sensors with smaller amounts of CB particles. While the overall electromechanical properties of SEBS-CB samples were found inferior to those of CB-only samples, the utilization of smaller amount of CB could lead to signiﬁcantly enhanced mechanical properties. Future work includes the study of such mechanical properties, as well as alternative fabrication procedures of SEBS-CB samples (e.g., concentration of SEBS, use of diﬀerent surfactant, etc.) to improve on the electromechanical properties.
Acknowledgments The authors acknowledge Dr. Joseph Schaefer from the Department of Aerospace Engineering at Iowa State University for his assistance with the electromechanical tests. The authors are also grateful to Dr. Steve Holland from Center for Non-Destructive Evaluation at Iowa State University for his help with thermography.
64 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
References 1. (a) Laﬂamme, S., Eisenmann, D., Wang, K., Ubertini, F., Pinto, I., DeMoss, A. (2018). Smart concrete for enhanced nondestructive evaluation, Mater. Eval., 76(10), pp. 1395–1404. (b) Al-Saleh, M. H., Sundararaj, U. (2008). An innovative method to reduce percolation threshold of carbon black ﬁlled immiscible polymer blends, Composites Part A, 39(2), pp. 284–293. 2. Arshak, K., Morris, D., Arshak, A., Korostynska, O. (2008). Sensitivity of polyvinyl butyral/carbon-black sensors to pressure, Thin Solid Films, 516(10), pp. 3298–3304. 3. Chiacchiarelli, L., Rallini, M., Monti, M., Puglia, D., Kenny, J., Torre, L. (2013). The role of irreversible and reversible phenomena in the piezoresistive behavior of graphene epoxy nanocomposites applied to structural health monitoring, Compos. Sci. Technol., 80, pp. 73–79. 4. Cochrane, C., Koncar, V., Lewandowski, M., Dufour, C. (2007). Design and development of a ﬂexible strain sensor for textile structures based on a conductive polymer composite, Sensors, 7(4), pp. 473–492. 5. D’Alessandro, A., Rallini, M., Ubertini, F., Materazzi, A., Kenny, J., Laﬂamme, S. (2015). A comparative study between carbon nanotubes and carbon nanoﬁbers as nanoinclusions in self-sensing concrete, in 2015 IEEE 15th International Conference on Nanotechnology (IEEE NANO), Rome, pp. 698–701. 6. D’Alessandro, A., Ubertini, F., Laﬂamme, S., Materazzi, A. L. (2016). Towards smart concrete for smart cities: recent results and future application of strain-sensing nanocomposites, J. Smart Cities, 1, p. 1. ´ P. (2014). Strain and damage 7. Galao, O., Baeza, F., Zornoza, E., Garces, sensing properties on multifunctional cement composites with cnf admixture, Cem. Concr. Compos., 46, pp. 90–98. ´ ome, ˆ R., Teyssie, P., Vanlathem, E., Deltour, R., Calderone, 8. Gubbels, F., Jer ´
A., Parente, V., Bredas, J.-L. (1994). Selective localization of car bon black in immiscible polymer blends: a useful tool to design electrical conductive composites, Macromolecules, 27(7), pp. 1972– 1974. 9. Han, B., Yu, X., Kwon, E. (2009). A self-sensing carbon nanotube/cement composite for traﬃc monitoring, Nanotechnology, 20(44), p. 445501. 10. Huang, J.-C. (2002). Carbon black ﬁlled conducting polymers and polymer blends, Adv. Polym. Technol., 21(4), pp. 299–313.
11. Laﬂamme, S., Cao, L., Chatzi, E., Ubertini, F. (2015). Damage detection and localization from dense network of strain sensors, Shock Vib., 2016, p. 2562949. 12. Laﬂamme, S., Pinto, I., Elkashef, M., Wang, K., Cochran, E. W., Ubertini, F. (2015). Conductive paint-ﬁlled cement paste sensor for accelerated percolation, Proc. SPIE, 9437, p. 943722. 13. Laﬂamme, S., Saleem, H. S., Vasan, B. K., Geiger, R. L., Chen, D., Kessler, M. R., Rajan, K. (2013). Soft elastomeric capacitor network for strain sensing over large surfaces, IEEE/ASME Trans. Mechatron., 18(6), pp. 1647–1654. 14. Lourie, O., Cox, D., Wagner, H. (1998). Buckling and collapse of embedded carbon nanotubes, Phys. Rev. Lett., 81(8), p. 1638. 15. McCarter, W., Starrs, G., Chrisp, T. (2000). Electrical conductivity, diﬀusion, and permeability of portland cement-based mortars, Cem. Concr. Res., 30(9), pp. 1395–1400. 16. Monti, M., Natali, M., Petrucci, R., Kenny, J., Torre, L. (2011). Impact damage sensing in glass ﬁber reinforced composites based on carbon nanotubes by electrical resistance measurements, J. Appl. Polym. Sci., 122, pp. 2829–2836. 17. Tumidajski, P., Xie, P., Arnott, M., Beaudoin, J. (2003). Overlay current in a conductive concrete snow melting system, Cem. Concr. Res., 33(11), pp. 1807–1809. 18. Ubertini, F., Laﬂamme, S., D’Alessandro, A. (2016). Smart cement paste with carbon nanotubes, in Loh, K. J., Nagarajaiah, S. (eds.) Innovative Developments of Advanced Multifunctional Nanocomposites in Civil and Structural Engineering, Woodhead Publishing, pp. 97–120. 19. Ubertini, F., Materazzi, A. L., D’Alessandro, A., Laﬂamme, S. (2014). Natural frequencies identiﬁcation of a reinforced concrete beam using carbon nanotube cement-based sensors, Eng. Struct., 60, pp. 265– 275. 20. Wen, S., Chung, D. (1999). Piezoresistivity in continuous carbon ﬁber cement-matrix composite, Cem. Concr. Res., 29(3), pp. 445–449. 21. Wen, S., Chung, D. (2007). Partial replacement of carbon ﬁber by carbon black in multifunctional cement–matrix composites, Carbon, 45(3), pp. 505–513. 22. Wu, J., Song, C., Saleem, H. S., Downey, A., Laﬂamme, S. (2015). Network of ﬂexible capacitive strain gauges for the reconstruction of surface strain, Meas. Sci. Technol., 26(5), p. 055103.
66 Use of Styrene Ethylene Butylene Styrene for Accelerated Percolation
23. Wu, S., Mo, L., Shui, Z., Chen, Z. (2005). Investigation of the conductivity of asphalt concrete containing conductive ﬁllers, Carbon, 43(7), pp. 1358–1363. 24. Xiao, H., Li, H., Ou, J. (2010). Modeling of piezoresistivity of carbon black ﬁlled cement-based composites under multi-axial strain, Sens. Actuators, A, 160(1), pp. 87–93. 25. Yehia, S. A., Tuan, C. Y. (2000). Thin conductive concrete overlay for bridge deck deicing and anti-icing, Transp. Res. Rec., 1698(1), pp. 45– 53. 26. Zhang, W., Dehghani-Sanij, A. A., Blackburn, R. S. (2007). Carbon based conductive polymer composites, J. Mater. Sci., 42(10), pp. 3408–3418.
Advancements in Silica Aerogel–Based Mortars ´ ˆ Flores-Colen, and Jorge de Brito Antonio Soares, Ines CERIS, Department of Civil Engineering, Architecture and Georresources, Instituto Superior T´ecnico, Universidade de Lisboa, Portugal [email protected]; ines.ﬂ[email protected]; [email protected]
Thermal mortars are thermal insulation solutions for the opaque envelope of buildings. However, the solutions with greater weight in the market still possess thermal conductivity values higher than those obtained by current thermal insulation materials, which reach at least 0.04 W/m · K. One way of overcoming this threshold is through the incorporation of superinsulating materials, such as silica aerogel. Silica aerogel is a nanostructured material with high porosity (75% to 98%) and pores of small sizes (between 10 and 100 nm), which allows it to have thermal conductivities between 0.012 and 0.021 W/m · K, lower than the air thermal conductivity at ambient pressure (0.026 W/m · K). It is produced through a sol-gel process, and it comes as monoliths or small-size (grain) aerogels with diﬀerent characteristics regarding mechanical strength, thermal behavior, density, degree of hydrophobicity, and opacity.
Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
68 Advancements in Silica Aerogel–Based Mortars
There are already applications of aerogel in insulation solutions in buildings, from thermal insulation of glazed siding to aerogel applied in blankets. The incorporation of silica aerogel has only recently begun to be exploited, and there are still only a few mortars with aerogel incorporation in the European market and some patented mortars. Mortars with aerogel incorporation may reach thermal conductivity values lower than 0.03 W/m · K. However, most studies on these mortars are focused mostly on their thermal behavior, and there is still lack of information on the remaining relevant properties to the overall performance of a thermal mortar. This chapter presents a summary of the studies on thermal mortars with aerogel and some of the main diﬃculties concerning the incorporation of this superinsulating material in mortars.
4.1 Introduction There has been a long-standing concern about thermal comfort inside buildings, with the ﬁrst thermal insulation panels emerging in the 19th century through the processing of organic materials (Bozsaky, 2010). On the other hand, the growth of the world population, associated with an increase in the consumption habits of society, has made human impact increasingly signiﬁcant on the environment (Wenzel et al., 1997; Milutiene˙ et al., 2012). But in the recent past scientists around the world have recognized that climate change and global warming are the result of human action (Gupta, 2016), and therefore it is important to take measures to reduce energy consumption and gaseous pollutant emission. In this sense, with the Kyoto Protocol, which Portugal signed, a set of policies and measures has been created to counter this tendency (United Nations, 1998; Parliament et al., 2003). Since buildings embody 40% of the total energy consumption in the European Union (EU), there is a signiﬁcant potential for reducing energy consumption by improving the performance of buildings (EU, 2010). This improvement can be achieved through the use of thermal insulation systems, focusing mainly on reducing the thermal conductivity of materials and on the thermal transmission of the elements of the building envelope (Jelle et al., 2010).
One of the ways to improve the thermal performance of buildings is to minimize losses and thermal gains through the opaque envelope (Gonc¸alves and Grac¸a, 2004), and this can be achieved through the use of thermal insulation systems such as mortars with thermal performance improvement, which have the same procedure application as those traditionally applied on buildings (Leopolder, 2010, cited by Barbero-Barrera et al., 2014). For a mortar to be classiﬁed as thermal, it needs to comply with certain levels of performance present in the EN 998-1 (CEN, 2010) standard, as shown in Table 4.1. The thermal conductivity coeﬃcient (λ), expressed in W/m · K or W/m · ◦ C, characterizes thermally homogeneous products by the amount of heat (expressed in W per unit area [m2 ]) that crosses a unit thickness (m), when a unit temperature diﬀerence (1◦ C or 1 K) is established between two ﬂat and parallel faces (Pina dos Santos and Matias, 2006). To achieve thermal conductivity values compatible with the requirements of EN 998-1 (2010), the incorporation of lightweight aggregates has been seen as a way of reducing the bulk density of mortars and consequently their thermal conductivity. In Fig. 4.1 several scientiﬁc publications and technical data sheets are presented, where it is possible to observe a trend of reduction of the thermal conductivity of diﬀerent products with the reduction of bulk density. It is also possible to observe that the variation of the thermal conductivity with the bulk density is not linear, reaching a level from which it is diﬃcult to reduce the thermal conductivity at the expense of the density, and the same tendency can be observed in commercial mortars (Barbero-Barrera et al., 2014). It is also observed that industrial mortars reach values of thermal conductivity (indicated in datasheets) lower than those obtained in research papers. However, the lower values of thermal conductivity presented are approximately 0.04 W/m · K for mortars with bulk density less than 250 kg/m3 . Nevertheless, regardless of the density of the material, the ther mal conductivity of the gas (air) remains constant (∼0.026 W/m · K), which causes a barrier (lower limit of thermal conductivity) of 0.03 W/m · K to the performance of current thermal insulation materials
Cc ≤ 0.4 (W1)
EN 1015-18 (CEN, 2002b)
Testing method EN 1015-11 (CEN, 1999b)
EN 1015-19 (CEN, 2004)
μ ≤ 15
EN 1745 (CEN, 2002a)
λ ≤ 0.1 (T1) λ ≤ 0.2 (T2)
Properties with requirements to fulﬁll Compressive Water Water vapor Thermal strength absorption permeability conductivity (N/mm2 ) due to coeﬃcient coeﬃcient capillary (W/m · K) (kg/m2 · min0.5 )
Classes/limits 0.4 a 2.5 (CS I) 1.5 a 5.0 (CS II)
EN 1015-10 (CEN, 1999a)
EN 1015-12 EN (CEN, 13501-1 2000) (CEN, 2007)
≥ declared value and rupture type
Properties with declared values Adhesion Reaction Durability Dry bulk (N/mm2 ) to ﬁre density (kg/m3 )
Table 4.1 Characteristics and requirements for a thermal mortar, in accordance with EN 998-1 (data from CEN, 2010)
70 Advancements in Silica Aerogel–Based Mortars
Figure 4.1 Thermal conductivity versus mortar’s density. Sources: (Fu and Chung, 1997; Xu and Chung, 2000b; Xu and Chung, 2000a; Demirboga, 2003; Uysal et al., 2004; Demirboga et al., 2007; Benazzouk et al., 2008; Azichem, 2009; Ashour et al., 2010; Sengul et al., 2011; FassaBortolo, 2011; Panesar ´ ´ ´ ´ and Shindman, 2012; Gutierrez-Gonzalez et al., 2012b; Gutierrez-Gonzalez et al., 2012a; Taoukil et al., 2012; Barreca and Fichera, 2013; Herrero et al., 2013; Thermowall, 2013; Barbero-Barrera et al., 2014; Tecresa, 2015; ¨ ARDEX, 2016; EDILTECO, 2016; Secil, 2016; Weber, 2016; ROFIX, 2016; Chiraema, 2017; Diasen, 2017; CVR, 2017; LATERLITE, 2017; Kimia, 2017).
(Simmler et al., 2005, cited by Cuce et al., 2014), so it is necessary to use innovative materials to exceed this limit.
4.1.1 Nanomaterials Nanotechnology allows the manipulation of materials with sizes and precision between 0.1 and 100 nm. At the nanoscale, surface eﬀects are more important than bulk properties, which can lead to materials with enhanced properties (Drexler, 1981, cited by Pacheco-Torgal and Jalali, 2011; Holister, 2002; Zhu et al., 2004; SCENIHR, 2010). According to the International Organization for Standardization (ISO, 2010, cited by Potoˇcnik, 2011), a “nanomaterial” describes any
72 Advancements in Silica Aerogel–Based Mortars
material with external sizes to the nanoscale or with the internal structure or surface structure at the nanoscale. Nanomaterials, according to their unconﬁned sizes at the nanoscale, can still be classiﬁed into 0D (nanoparticles), 1D (nanotubes, nanoﬁlaments, and nanoﬁbers), 2D (nanoﬁlms and nanocoatings), and 3D (mono liths) (Gonc¸alves, 2012). However, what makes these sizes so interesting is the high ratio between surface area and volume. Thus, there is a greater exposure of atoms/molecules of the material to the surrounding environment and a greater amount of possible connections available to the surface, which makes the particle chemically more active. For example, in a particle with the approximate diameter of 10 nm, about 20% to 25% of the atoms are exposed to the surrounding medium, whereas in a particle with 3 nm this percentage increases from 45% to 60% (Sengupta and Sarkar, 2015). There are two types of approaches to nanomaterial synthesis: top down or bottom up. With the top-down approach, the size of the structure is reduced to the nanoscale, while retaining the original properties. Thus, nanomaterials are obtained by methods such as high-energy milling, mechanochemical processing, pickling, electric blasting, ultrasonic agitation, cathodic spraying, and laser ablation. Immediately after the process of obtaining the nanoparticles, they are highly reactive and can easily form agglomerates. Thus, these methods have to be carried out under vacuum or in an inert atmosphere, because if the procedure is performed in the presence of some reactive gas, additional reactions may occur (Taylor, 2002; Nass et al., 2004; Zhu et al., 2004; Al-Jabri and Shoukry, 2014). In turn, the bottom-up approach involves the manipulation of atoms and molecules with synthesis of materials to create nanostructures, through chemical reactions, chemical processes based on the transformation of solutions, such as the sol-gel process, vapor deposition by chemical process, plasma or ﬂame spray synthesis, and atomic or molecular condensation. Of these methods, the sol-gel process is highlighted, which diﬀers from the rest because it occurs at low temperatures, which makes it a versatile and cost eﬀective process (Taylor, 2002; Nass et al., 2004; Zhu et al., 2004; Al-Jabri and Shoukry, 2014).
Nanomaterials can improve some characteristics of the construc tion products (like strength and durability) and add new functions such as photocatalytic (self-cleaning, pollution reduction, and anti microbial ability), antifogging, and self-sensing abilities (Jayapalan et al., 2013). Therefore, the introduction of nanomaterials in con ventional construction products can lead to construction materials with excellent properties and make buildings with a more eﬃcient performance (Li et al., 2004; Senﬀ et al., 2013). Even though nanotechnology is not a new science or technology, only in the past two decades has there been an increase in research in this ﬁeld (Ge and Gao, 2008). Recently some studies have emerged regarding the incorporation of nanomaterials in mortars, leading to mortars with enhanced and innovative properties to be applied on building facades (nanorenders). Due to their nanosize, nanomaterials generally aﬀect the strength, shrinkage, and durability properties of Portland cement paste and help to improve the quality and longevity of structures (Ltiﬁ et al., 2011; Hanus and Harris, 2013). With nanomaterials it is also possible to prevent the initiation of microcracks through the control of nanocracks with nanosized ﬁbers (Konsta-Gdoutos et al., 2010a), to enhance the thermal performance (Stahl et al., 2012), and to give photocatalytic and self-cleaning properties to the renders (Jayapalan et al., 2013). To achieve these improvements, good dispersion of the nanopar ticles in a cement mortar matrix is important, which is diﬃcult to reach due to their high surface energy and strong interparticle forces, which can lead to poor dispersion, resulting in weak zones or potential areas with concentrated stresses (Guskos et al., 2010; Nazari and Riahi, 2011; Givi et al., 2011, cited by Hanus and Harris, 2013). The possible risks that nanomaterials could pose on health are also a concern, among them being lung inﬂammation or cancer, and because of that, they should be handled like a material with unknown toxicity (Grassian et al., 2007; Hallock et al., 2009, cited by Pacheco-Torgal and Jalali, 2011), especially powder nanomaterials (nanoparticles). Multiwalled carbon nanotubes (CNTs) have a tensile strength and Young’s modulus that are hundreds and tens of times, respectively, those of steel. Their incorporation in small amounts, associated with
74 Advancements in Silica Aerogel–Based Mortars
a higher aspect ratio, leads to an eﬀective arrest of the nanocracks (Konsta-Gdoutos et al., 2010a; 2010b; Hanus and Harris, 2013). Multiwalled CNTs can also improve the durability of the cement matrix because they reduce the ﬁne pores, which results in a decrease of the capillary stresses. Therefore, it is possible to obtain a mortar with good properties for protection against chemical attack (Konsta-Gdoutos et al., 2010b). However, it is very important to get a uniform dispersion of CNTs in the cement matrix (Xie et al., 2005), which is diﬃcult to accomplish because of their poor interaction with cement, resulting from their intrinsically hydrophobic nature and because of the tightly bound formation of agglomerates or bundles resulting from their production (Grobert, 2007, cited by Konsta-Gdoutos et al., ´ de Ibarra et al., 2006, cited by Hanus and Harris, 2013). 2010a; Saez Several studies have emerged regarding the incorporation of nanosilica (nano-SiO2 ), with good results in improving the com pressive and splitting tensile strengths of cement-based materials (Shekari and Razzaghi, 2011) and reducing the permeability of cement mortar (Sadrmomtazi et al., 2009). However, the adverse eﬀect on cement-based materials’ workability due to the high speciﬁc surface area of nano-SiO2 and the dispersion of these nanoparticles can cause lower strength of mortars in later ages (Kawashima et al., 2013). To counteract the diﬃculties in achieving a good distribution of nano-SiO2 , some authors suggest a low percentage of particles (1–5 wt%), while others propose contents of 10 wt% by weight of cement (Senﬀ et al., 2009, cited by Ltiﬁ et al., 2011). Nano–titanium dioxide (nano-TiO2 ), with photocatalytic and self cleaning properties, can enable mortars with new functionalities that contribute to the reduction of air pollutants, like biocide properties and self-cleaning eﬀects, leading to the maintenance of aesthetic characteristics, such as color, and decrease the environ ´ mental impact of construction materials (Cardenas et al., 2012; Hanus and Harris, 2013; Jayapalan et al., 2013). Once these particles need light stimulation for catalytic action, nano-TiO2 particles are normally applied on external renders or paints (Senﬀ et al., 2013). However, some studies (Hanus and Harris, 2013) found that the self cleaning and photocatalytic eﬀects of TiO2 may form harmful side
products, which indicates the need for more research on their side eﬀects. The use of ﬁne particles may also has a negative eﬀect on the rheological properties, which results in higher water demand and ¨ shorter setting time (Husken et al., 2009; Chen et al., 2012; Senﬀ et al., 2012, cited by Senﬀ et al., 2013). Summing up, with the incorporation of nanomaterials in mortars it is possible to improve several characteristics, as shown in Table 4.2. In general, an increase of mortars’ compacity was observed due to the nanosize of the particles that ﬁll their voids. However, in some cases, a decrease of mortars’ workability was noticed due to the high speciﬁc surface area of the nanomaterials, and some diﬃculties in achieving good dispersion of nanoparticles in the mortar matrix were reported. Although there are materials that do not have a nanoscale size that allows them to react or ﬁll certain spaces, they can present a nanostructure that gives the material exceptional properties, as is the case of silica aerogel. The advantages and disadvantages of this nanomaterial are also found in Table 4.2, with a more detailed description of its inﬂuence on mortars in the following section. To sum up, an environmental concern has been noticed with the use of nanomaterials in mortars. Nevertheless, despite their high initial impact, nanomaterials can contribute positively in the long term to more sustainable buildings. However, there is still a lack of research on their health impact. Nowadays, despite the eﬀorts to reduce the production cost of some nanomaterials, their production cost is still high and there is a considerable lack of information regarding the real costs of renders with nanomaterials. Therefore, it is important to research the eﬀects of nanomaterials in mortars to identify the aspects to be improved and, in the future, achieve products to apply in renders with advanced properties at a low or competitive cost.
4.2 Silica-Based Aerogel Silica aerogel is a nanostructured material, produced by the sol gel process, consisting of a large number of pores of small size (Aspen, 2014; citados por Thapliyal and Singh, 2014; Kyushu, 2014).
Workability and mixing
Initial increase Decrease at 28 days
Compressive strength Reduction of capillary stresses Reduction of water permeability Reduction of thermal conductivity Photocatalytic and self-cleaning properties (new properties)
%, percentage of incorporation; (–), low; (+) high; e e e , very expensive; e e, expensive; n.s., not speciﬁed.
Table 4.2 Eﬀect of various nanomaterials on mortars (data from Soares et al., 2014a)
Initial increase Final decrease Initial increase Final decrease
76 Advancements in Silica Aerogel–Based Mortars
The structure of the aerogel is composed of small spherical silica agglomerates (SiO2 particles), generally 2 to 5 nm in size, which are connected together in chain, resulting in a “pearl necklace,” forming a porous space grid, in which the pores have an average size of 20 to 40 nm, generally ranging between 10 and 100 nm. Thus, aerogels with diﬀerent particle and pore sizes can be obtained, as well as diﬀerent porosity values, which in general range from 75% to 98% (Rubin and Lampert, 1983; Zeng et al., 1994; Pajonk, 1998; Schmidt and Schwertfeger, 1998; Wagh et al., 1999; Akimov, 2003; Ilharco et al., 2007; Soleimani Dorcheh and Abbasi, 2008). These characteristics confer unique properties to the aerogel, as a very low density, and in some cases can reach values very close to the density of air (1.2 kg/m3 ). This is the case of a silica aerogel synthesized by Dr. Steven Jones of NASA’s Jet Propulsion Laboratory, which in 2002 was considered by the Guinness World Records book as the lightest solid material in the world with density 3 kg/m3 (NASA, 2002; Akimov, 2003). This milestone was already surpassed in 2004 by another silica aerogel with density 1.9 kg/m3 (S and TR, 2003) and recently (2012) by graphene aerogel (0.18 kg/m3 ) (Mecklenburg et al., 2012), with a graphene aerogel with density 0.16 kg/m3 being the current holder of the Guinness World Record for the lightest solid in the world (since 2013) (Guinness, 2013). Although aerogel is classiﬁed as a nanomaterial due to its nanostructure, it is composed of a continuous pore network, which allows obtaining aerogels of small size, such as aerogel in granules ¨ (Fig. 4.2a) or monoliths of considerable size (Fig. 4.2b) (Husing and Schubert, 1998; Pajonk, 1998; Bhagat et al., 2007; Zhu et al., 2007; Roy and Hossain, 2008). The high thermal insulation capacity of aerogel can be justiﬁed by its high total porosity and small particle size that make up the structure, resulting in a solid structure occupying a small part of the aerogel. In addition, it has an open structure that has a high amount of loose ends, that is, dead ends for heat transfer by conduction through the structure, resulting in a path with high tortuosity and ineﬃciency for the heat transfer through the solid part of the aerogel (Zeng et al., 1994; Akimov, 2003; Wei et al., 2011; Baetens et al., 2011; Thapliyal and Singh, 2014).
78 Advancements in Silica Aerogel–Based Mortars
Figure 4.2 Example of silica-based aerogels: (a) grain and (b) monolith.
The heat transfer component associated with the solid structure depends on the density of the aerogel and can be evaluated using vacuum. For example, the thermal conductivity component associated only with the solid structure has values in the order of 0.01 W/m · K for aerogels with density 270 kg/m3 and can reach 0.001 W/m · K for aerogels with density 80 kg/m3 (Heinemann et al., ¨ 1996; Husing and Schubert, 1998; Zhu et al., 2007; Baetens et al., 2011). Because the average pore size (about 20 nm) is less than the space required for air to move (about 70 nm) at ambient temperature and pressure, the movement of the gas molecules within the silica aerogel porous network is strongly suppressed, thus reducing gas conduction (Wei et al., 2011), resulting in a marked decrease of thermal conductivity in pores from 1 μm to 10 nm (Jelle et al., 2010). Thus, it is possible to assume that the air molecules become entrapped in the porous structure, whereby the heat transfer by air convection inside the pores is negligible. Therefore, the contribution of the air inside the aerogel to the thermal conductivity is 0.005 to 0.01 W/m · K, considerably lower than the air conductivity without air convection (0.026 W/m · K) (Rubin and Lampert, 1983; Kuhn et al., 1995; Zhu et al., 2007). Silica aerogel can absorb radiation with wavelengths greater than 5 μm (infrared radiation), so it is eﬃcient to block the radiation emitted by walls and windows at an environment temperature and
can be considered a translucent thermal insulator, which eﬃciently conducts sunlight but blocks infrared radiation. However, at wavelengths between 3 μm and 5 μm, its absorption is reduced, which results in a deterioration of the thermal insulation capacity with the temperature increase (Fricke and Tillotson, 1997; Fricke, 1988; Ebert, 2011). The radiation conduction component has values between 0.0015 and 0.003 W/m · K for aerogels with density ¨ et al., 1993). 100 kg/m3 , at a temperature of 26.85◦ C (Hummer In this way, the aerogel is presented as a material with high potential for thermal insulation. In fact, this material, synthesized for the ﬁrst time in 1931 by Steven S. Kistler, has considerably reduced thermal conductivities ranging from 0.012 to 0.021 W/m · K. Even the highest values of thermal conductivity recorded in silica aerogels are lower than the thermal conductivity of air ¨ at ambient pressure (0.026 W/m · K) (Husing and Schubert, 1998; Schmidt and Schwertfeger, 1998; Zhu et al., 2007; Baetens et al., 2011; Buratti and Moretti, 2012; Jelle et al., 2014). Despite their remarkable properties of thermal insulation and good acoustic properties, the characteristics that make aerogels good insulators are also responsible for making aerogel a weak material, which is a disadvantage for its use in building insulation materials (Parmenter and Milstein, 1998; Wei et al., 2011). Silica aerogels are cellular solid with a “pearl necklace”-type skeleton net. The fragility of silica aerogel is attributed to the “necks” (weak points of this structure that are in the regions between particles) that form the structural network of the aerogel (Woignier and Phalippou, 1988; Ma et al., 2000; Tan et al., 2001; Zhang et al., 2004; She and Ohji, 2002, cited by Lu et al., 2011). It is possible to improve the strength of the aerogel monoliths by increasing the width of these link points between particles (Leventis et al., 2002). Another reason for the aerogel’s fragility is that the solid structure presents a disordered morphology, which causes an irregular distribution of pores with zones of greater porosity and others of dense agglomeration of particles (with little deﬁned connections), which results in a low-organized material with density gradients (Obrey et al., 2011). Because of the fragility of the aerogels and the complexity involved in handling the preparation of specimens for mechanical
80 Advancements in Silica Aerogel–Based Mortars
testing, it is diﬃcult to carry out tests of pure traction, torsion, or multiaxial stresses, so usually only compression and bending tests are carried out (Woignier and Phalippou, 1988, cited by Lu et al., 2011). The lower values of the compressive strength of aerogels of greater density may also be related to the “neck” region. In fact, unlike low-porosity materials in which the materials are treated as a whole and the connection between the particles of the solid is not taken into account, in materials of high porosity the way the particles are linked together is an important parameter (Woignier and Phalippou, 1988). The most common process for preparing silica aerogels is the sol gel process, which includes three main steps: hydrolysis reactions, condensation (gelling) reactions, and aging and drying (Brinker and Scherer, 1990). The sol-gel process consists of obtaining a solid 3D network of an oxide, by chemical reaction in solution, at low temperatures. To this end, starting from suitable precursors, a colloid (sol) is produced that can generate, by polymerization reactions, a rigid 3D structure (gel) from which it is possible to obtain ceramic materials. A “sol” may be deﬁned as a stable dispersion of colloidal particles or polymers in a solvent, wherein “colloidal” represents a dispersion of suspended solids of such a small size (1 to 1000 nm) that the gravitational forces are negligible and the interactions may be called short-range forces, such as van der Waals forces and surface charges, with no agglomeration or sedimentation occurring. In turn, a “gel” consists of a continuous 3D network involving the liquid phase (Brinker and Scherer, 1990; Ghosh, 2015). Hydrolysis of precursors (generally metal alkoxides) and con densation between hydrolyzed oligomers are catalyzed, in a co solvent, with controlled stirring and temperature. The synthesis and process parameters determine the aerogel structure, aﬀecting its properties and applications (Menaa et al., 2010; Pierre and Rigacci, 2011). For example, adequate aging of the wet gel, during which the condensation reactions proceed, strengthening the network, leads to aerogels with higher mechanical strength (Ma et al., 2000). Thus, the sol-gel process can be described as a two-step process to form a structural network (hydrolysis and condensation
Aerogel-Based Mortars 81
reactions). In the ﬁrst stage of the reaction, polymers or rings are established, subsequently resulting in colloids deﬁning the “sol.” In the second step, due to condensation reactions, the polymer network grows with the union of the molecules, establishing macromolecules that extend throughout the solution, obtaining the transition from “sol” to “gel” (De Souza et al., 2011; Pandey and Mishra, 2011). In this manner, the sol-gel process can be performed with diﬀer ent precursors and/or solvents and with diﬀerent drying methods, which allows obtaining materials of diﬀerent sizes (small grains to monoliths of considerable sizes) and diﬀerent characteristics with regard to mechanical resistance, thermal behavior, density, degree ´ and Ilharco, 2017). of hydrophobicity, and opacity (Julio Since silica aerogel was discovered, many potential applications have been described (Schmidt and Schwertfeger, 1998) and can be used from pharmacy or agriculture (as carrier material), electronics, kinetic energy absorbers (to collect dust particles suspended in the atmosphere), and thermal insulation (mostly for cryogenic ambient conditions or high temperature) (Tsou, 1995; Schmidt and Schwertfeger, 1998; Pajonk, 2003; Jones, 2006). With regard to the application of silica aerogel in construction, there has been a high interest in the thermal insulation of glazed siding of buildings in order to reduce energy costs with domestic and industrial heating (Schmidt and Schwertfeger, 1998; Pajonk, 2003). Aerogels are also applied in blankets for insulation of the opaque building envelope (Baetens et al., 2011; Ibrahim et al., 2015). Their high thermal insulation and good acoustic behavior make them a potential material to be used in buildings (Schmidt and Schwertfeger, 1998; Acharya et al., 2013).
4.3 Aerogel-Based Mortars The incorporation of silica aerogel in coating materials has been studied only recently, with the ﬁrst research paper on the subject emerging in 2012 (Stahl et al., 2012). Since mortars are produced using water, it is important to understand the behavior of aerogels in the presence of mixing
82 Advancements in Silica Aerogel–Based Mortars
Figure 4.3 Collapsed particles of hydrophilic aerogel in mortar under (a) a binocular microscope and (b) scanning electronic microscopy (SEM).
water. These may exhibit diﬀerent degrees of hydrophobicity, from hydrophilic to superhydrophobic, resulting in diﬀerent behaviors of the mortars at the fresh and hardened states (Soares et al., 2014b; ´ et al., 2016b; Julio ´ and Ilharco, 2017; Soares et al., 2018). Julio Hydrophilic aerogels have high structural sensitivity to the presence of water. When incorporated in mortars, internal fractures appear in the aerogel that lead to its collapse, with poor adhesion between the aerogel and the remaining mortar paste, resulting in a mortar with poor cohesion at the hardened state (Fig. 4.3). This property makes hydrophilic aerogels unsuitable for aerogel incorporation into mortars, especially for high incorporation rates. On the other hand, hydrophobic aerogels are presented as a possible solution of insulating aggregates for incorporation in high-performance thermal mortars, because they do not allow the entrance of water into their interior and consequent collapse. Stahl et al. (2012) prepared a hydrophobic mineral cement-free mortar of high thermal performance (0.025 W/m · K) and a density of 200 kg/m3 , incorporating an aerogel in 60% to 90% of the total volume, and some additions to improve the workability, which are not identiﬁed. However, the study does not refer to mechanical strength, water behavior, or other fundamental properties that allow the complete performance characterization of the mortars. Buratti et al. (2014) presented a study on the thermal and acoustic performance of a mineral-based render with incorporation of an aerogel, between 80% and 99% of the total volume,
Aerogel-Based Mortars 83
with thermal conductivities between 0.014 and 0.05 W/m · K and densities between 125 and 300 kg/m3 . The renders produced by the authors showed an increase in the sound absorption coeﬃcient in relation to the reference material (laminated gypsum plaster). Ibrahim et al. (2014; 2015) studied the hygrothermal behavior of a patented mortar based on mineral and/or hydraulic binder, an insulating ﬁller composed of hydrophobic silica xerogel powder or grains. The studied mortar had a low thermal conductivity and density (0.0268 W/m · K and 156 kg/m3 , respectively), good water behavior with a coeﬃcient of resistance to water vapor of 4.25% ±6%, and a coeﬃcient of water absorption of 0.184% ±15% (kg/m2 s1/2 ) in which they evaluated the change in thermal conductivity with relative humidity. The same authors found that the coeﬃcient of thermal conductivity changes only for relative humidity values higher than 60% and also presents a good thermal insulation behavior (∼0.041 W/m · K) for relative humidity higher than 90%. However, no indication is given regarding the mechanical behavior of this mortar. Ng et al. (2015) carried out a study of cement-based mortars incorporating aerogel at between 20% and 80% of the total volume, where they analyzed the thermal and mechanical performance of the mortars with an increase in the aerogel content. A mortar with aerogel in the amount of 80% of the total volume reached the thermal conductivity value of 0.31 W/m · K and a density of 690 kg/m3 , with negligible resistance values (very close to zero). The same authors also studied the aerogel interface with the binder matrix, where they found a gap (spaces) between the two materials. These aspects were also analyzed by Gao et al. (2014) for concrete, which shows the diﬃculty of incorporating hydrophobic aerogels into mortars or concrete, due to problems of connection at the interface between the aerogel and the cement matrix. ´ Julio et al. (2016b) bypassed this situation through the incor poration of surfactants, resulting in a better connection between the hydrophobic aerogel and the remaining mortar mix. The same authors indicate that the content of surfactants should be adjusted to the hydrophobicity of the aerogel, since to a certain extent its incorporation is positive for the connection between the aerogel and the remaining matrix, but overcoming a limit, gaps (spaces)
84 Advancements in Silica Aerogel–Based Mortars
Figure 4.4 Aerogel-based mortar: (a) production, (b) application on a brick substrate, (c) application on a wall, and (d) the ﬁnal aspect.
occur again around the aerogel. Thus, with correct adjustment of the content of surfactants as a function of the hydrophobicity of aerogel, it is possible to produce mortars with a good workability for application to the spoon (Fig. 4.4).
4.4 Performance of Aerogel-Based Mortars There are already a few mortars with aerogel on the market; one of them is FIXIT222 with claimed thermal conductivity (λ10 ) of 0.0261 W/m · K (EMPA, 2016). Several studies have been developed with this mortar (Koebel et al., 2012; Ibrahim et al., 2014; Wakili et al., 2015). This mortar should have a reinforced ﬁnishing, similar to the ETICS-type system, and these studies are mainly focused on thermal conductivity. Table 4.3 synthesizes the relevant properties for a thermal mortar according to EN 998-1 (CEN, 2010), which are available for aerogel-based mortars from various authors, as well as industrial mortars and patents (presented in the previous sections). As shown in this table, the values of thermal conductivity are between 0.014 and 0.076 W/m · K, clearly proving the potential of these materials as aggregates. However, the lack of information on
Lime, gypsum, cement Alumina cement, Portland cement, lime, calcium sulfate
144 to 318 450 to 630 –
Mineral binder and/or organic hydraulic binder Hydraulic lime NHL 5, calcium hydroxide, white cement Cement
Portland cement, silica fume Cement
4 to 5
4.25 ± 6%
0.184 ± 15% –
0.015 to 0.066 0.15 to 0.25 0.034
0.027 ± 3%
0.025 0.014 to 0.016 0.31
(Doshi et al., 2011) (Frank et al., 2000) (Achard et al., 2011)
(Khamidi et al., 2014) (Ibrahim et al., 2014)
(Stahl et al., 2012) (Buratti et al., 2014) (Ng et al., 2015)
Properties with declared values Properties with requirements to fulﬁll Reference ρ fu RF D CS W μ λ 3 2 2 2 0.5 (kg/m ) (N/mm ) (N/mm ) (kg/m s ) (W/m · K) 200 115 to 125 0 (8.76) Ro Ro The variation of the gauge factor as a function of the ﬁller concentration is plotted in Fig. 8.20. Note that the gauge factor is slightly higher in the case of tensile stresses. Moreover, it is also important to note that maximum values of both gauge factors, λ− and λ+ , are found around the percolation threshold fc . The sensitivity of the composites rapidly decreases as the ﬁller content moves away from this critical threshold, especially for ﬁller contents below the percolation threshold.
8.4 Summary In this chapter we introduced the micromechanics modeling of nanomodiﬁed composites, in particular for CNT-reinforced compos ites. First, after a concise overview of the fundamentals of mean-ﬁeld homogenization theory, the main approaches on the mechanical
210 Micromechanics Modeling of Nanomodified Cement-Based Composites
homogenization of CNT-reinforced composites were introduced. We discussed the suitability of mean-ﬁeld homogenization theory for incorporating physically meaningful variables of the microstructure, such as ﬁller topology, ﬁller distribution, waviness, and agglomera tion eﬀects. Second, we used the basis of mechanical homogenization for modeling of the electric transport properties of CNT-reinforced composites. By virtue of the analytical framework of mean-ﬁeld homogenization theory, the electrical mechanisms governing the electrical conductivity of these composites were incorporated, including electron hopping and conductive networking. Afterward, the piezoresistive properties of the composites were analyzed by characterizing the strain-induced variations in the microstructure. Finally, a discussion of the strain-sensing capabilities of CNT reinforced composites was made by analysis of strain sensitivity, as well as characterization of gauge factors.
References 1. Yakobson, B. I., Avouris, P. (2001). Mechanical properties of carbon nanotubes, in Carbon Nanotubes, Springer, pp. 287–327. 2. Demczyk, B., Wang, Y., Cumings, J., Hetman, M., Han, W., Zettl, A., Ritchie, R. (2002). Direct mechanical measurement of the tensile strength and elastic modulus of multiwalled carbon nanotubes, Mater. Sci. Eng. A, 334, pp. 173–178. 3. Ebbesen, T., Lezec, H., Hiura, H., Bennett, J., Ghaemi, H., Thio, T. (1996). Electrical conductivity of individual carbon nanotubes, Nature 382, pp. 54–56. ´ P. (2014). Strain and damage 4. Galao, O., Baeza, F., Zornoza, E., Garces, sensing properties on multifunctional cement composites with CNF admixture, Cem. Concr. Compos., 46, pp. 90–98. 5. Han, B., Han, B., Ou, J. (2009). Experimental study on use of nickel powder-ﬁlled Portland cement-based composite for fabrication of piezoresistive sensors with high sensitivity, Sens. Actuators, A, 149, pp. 51–55. 6. Ubertini, F., Materazzi, A. L., D’Alessandro, A., Laﬂamme, S. (2014). Natural frequencies identiﬁcation of a reinforced concrete beam using
carbon nanotube cement-based sensors, Eng. Struct., 60, pp. 265– 275. ´ 7. Ferreira, A. D. B., Novoa, P. R., Marques, A. T. (2016). Multifunctional material systems: a state-of-the-art review, Compos. Struct., 151, pp. 3– 35. 8. Eshelby, J. D. (1957). The determination of the elastic ﬁeld of an
ellipsoidal inclusion, and related problems, Proc. R. Soc. London, Ser. A,
241, pp. 376–396.
9. Mura, T. (1987). Micromechanics of Defects in Solids, Vol. 3, Springer
Science & Business Media.
10. Mori, T., Tanaka, K. (1973). Average stress in matrix and average elastic energy of materials with misﬁtting inclusions, Acta Metall., 21, pp. 571– 574. 11. Benveniste, Y. (1987). A new approach to the application of MoriTanaka’s theory in composite materials, Mech. Mater., 6, pp. 147–157. 12. Hill, R. (1965). A self-consistent mechanics of composite materials, J. Mech. Phys. Solids, 13, pp. 213–222. 13. Qiu, Y., Weng, G. (1990). On the application of Mori-Tanaka’s theory involving transversely isotropic spheroidal inclusions, Int. J. Eng. Sci., 28, pp. 1121–1137. 14. Ferrari, M. (1991). Asymmetry and the high concentration limit of the Mori-Tanaka eﬀective medium theory, Mech. Mater., 11, pp. 251–256. 15. Dvorak, G. J., Bahei-El-Din, A. (1997). Inelastic composite materials: transformation analysis and experiments, in Continuum Micromechan ics, Springer Nature, pp. 1–59. 16. Ferrari, M. (1994). Composite homogenization via the equivalent poly inclusion approach, Compos. Eng., 4, pp. 37–45. 17. Dunn, M. L., Ledbetter, H., Heyliger, P. R., Choi, C. S. (1996). Elastic constants of textured short-ﬁber composites, J. Mech. Phys. Solids, 44, pp. 1509–1541. 18. Schjødt-Thomsen, J., Pyrz, R. (2001). The Mori-Tanaka stiﬀness tensor: diagonal symmetry, complex ﬁbre orientations and non-dilute volume fractions, Mech. Mater., 33, pp. 531–544. 19. Vigolo, B. (2000). Macroscopic ﬁbers and ribbons of oriented carbon nanotubes, Science, 290, pp. 1331–1334. 20. Poelma, R. H., Fan, X., Hu, Z. Y., Van Tendeloo, G., van Zeijl, H. W., Zhang, G. Q. (2016). Eﬀects of nanostructure and coating on the mechanics of carbon nanotube arrays, Adv. Funct. Mater., 26, pp. 1233–1242.
212 Micromechanics Modeling of Nanomodified Cement-Based Composites
21. Hsiao, H., Daniel, I. (1996). Elastic properties of composites with ﬁber waviness, Composites Part A, 27, pp. 931–941. 22. Shi, D., Feng, X., Huang, Y. Y., Hwang, K., Gao, H. (2004). The eﬀect of nanotubewaviness and agglomeration on the elastic property of carbon nanotube-reinforced composites, J. Eng. Mater. Technol., 126, pp. 250– 257. ´ 23. Garc´ıa-Mac´ıas, E., D’Alessandro, A., Castro-Triguero, R., Perez-Mira, D., Ubertini, F. (2017). Micromechanics modeling of the electrical conductivity of carbon nanotube cement-matrix composites, Composites Part B, 108, pp. 451–469. 24. Dong, S., Zhou, J., Liu, H., Qi, D. (2015). Computational prediction of waviness and orientation eﬀects in carbon nanotube reinforced metal matrix composites, Comput. Mater. Sci., 101, pp. 8–15. 25. Yanase, K., Moriyama, S., Ju, J. W. (2013). Eﬀects of CNT waviness on the eﬀective elastic responses of CNT–reinforced polymer composites, Acta Mech., 224, pp. 1351–1364. 26. Wernik, J. M., Meguid, S. A. (2010). Recent developments in multifunc tional nanocomposites using carbon nanotubes, Appl. Mech. Rev., 63, p. 050801. 27. Li, H., Xiao, H., Ou, J. (2006). Eﬀect of compressive strain on electrical resistivity of carbon black-ﬁlled cement-based composites, Cem. Concr. Compos., 28, pp. 824–828. 28. Chang, L., Friedrich, K., Ye, L., Toro, P. (2009). Evaluation and visualiza tion of the percolating networks in multi-wall carbon nanotube/epoxy composites, J. Mater. Sci., 44, pp. 4003–4012. 29. Xu, J., Zhong, W., Yao, W. (2010). Modeling of conductivity in carbon ﬁber-reinforced cement-based composite, J. Mater. Sci., 45, pp. 3538– 3546. 30. Takeda, T., Shindo, Y., Kuronuma, Y., Narita, F. (2011). Modeling and characterization of the electrical conductivity of carbon nanotube-based polymer composites, Polymer, 52, pp. 3852–3856. 31. Feng, C., Jiang, L. (2013). Micromechanics modeling of the electrical conductivity of carbon nanotube (CNT)–polymer nanocomposites, Composites Part A, 47, pp. 143–149. 32. Simmons, J. G. (1963). Generalized formula for the electric tunnel eﬀect between similar electrodes separated by a thin insulating ﬁlm, J. Appl. Phys., 34, pp. 1793–1803.
33. Li, C., Thostenson, E. T., Chou, T. W. (2007). Dominant role of tunneling resistance in the electrical conductivity of carbon nanotube–based composites, Appl. Phys. Lett., 91, p. 223114. 34. Wen, S., Chung, D. (2001). Eﬀect of carbon ﬁber grade on the electrical behavior of carbon ﬁber reinforced cement, Carbon, 39, pp. 369–373. 35. Yan, K., Xue, Q., Zheng, Q., Hao, L. (2007). The interface eﬀect of the eﬀective electrical conductivity of carbon nanotube composites, Nanotechnology, 18, p. 255705. 36. Komori, T., Makishima, K. (1977). Numbers of ﬁber-to-ﬁber contacts in general ﬁber assemblies, Text. Res. J., 47, pp. 13–17. 37. Pan, N. (1993). A modiﬁed analysis of the microstructural characteris tics of general ﬁber assemblies, Text. Res. J., 63, pp. 336–345. 38. Shim, W., Kwon, Y., Jeon, S., Yu, W. (2015). Optimally conductive networks in randomly dispersed CNT: graphene hybrids, Sci. Rep., 5, p. 16568. 39. Kumar, V., Rawal, A. (2016). Tuning the electrical percolation threshold of polymer nanocomposites with rod-like nanoﬁllers, Polymer, 97, pp. 295–299. 40. Toll, S. (1998). Packing mechanics of ﬁber reinforcements, Polym. Eng. Sci., 38, pp. 1337–1350. 41. Zheng, X., Forest, M. G., Vaia, R., Arlen, M., Zhou, R. (2007). A strategy for dimensional percolation in sheared nanorod dispersions, Adv. Mater., 19, pp. 4038–4043. 42. Deng, F., Zheng, Q. S. (2008). An analytical model of eﬀective electrical conductivity of carbon nanotube composites, Appl. Phys. Lett., 92, p. 071902. 43. Taya, M. (2005). Electronic composites: modeling, characterization, processing, and MEMS applications, Cambridge University Press. 44. Seidel, G. D., Lagoudas, D. C. (2009). A micromechanics model for the electrical conductivity of nanotube-polymer nanocomposites, J. Compos. Mater., 43, pp. 917–941. 45. Feng, C. (2014). Micromechanics modeling of the electrical conductivity of carbon nanotude (CNT)-polymer nanocomposites, Ph.D. thesis, University of Western Ontario. 46. Feng, C., Jiang, L. (2014). Investigation of uniaxial stretching eﬀects on the electrical conductivity of CNT-polymer nanocomposites, J. Phys. D: Appl. Phys., 47, p. 405103.
214 Micromechanics Modeling of Nanomodified Cement-Based Composites
47. Hu, N., Fukunaga, H., Atobe, S., Liu, Y., Li, J. (2011). Piezoresistive strain sensors made from carbon nanotubes based polymer nanocomposites, Sensors, 11, pp. 10691–10723. ´ 48. Garc´ıa-Mac´ıas, E., D’Alessandro, A., Castro-Triguero, R., Perez-Mira, D., Ubertini, F. (2017). Micromechanics modeling of the uniaxial strain sensing property of carbon nanotube cement-matrix composites for SHM applications, Compos. Struct., 163, pp. 195–215. 49. Sobha, A., Narayanankutty, S. K. (2015). Improved strain sensing property of functionalised multiwalled carbon nanotube/polyaniline composites in TPU matrix, Sens. Actuators, A, 233, pp. 98–107.
Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures Andrea Meoni, Antonella D’Alessandro, Filippo Ubertini, and Annibale Luigi Materazzi Department of Civil and Environmental Engineering, University of Perugia, Via G. Duranti 93, 06125 Perugia, Italy [email protected]
9.1 Introduction Carbon cement–based sensors represent a promising technology for the structural health monitoring (SHM) of concrete buildings. The novel technology is capable to overcome the known problems related to the use of oﬀ-the-shelf sensing technologies such as strain gauges, accelerometers, optical sensors, etc., which ﬁnd limitations in their small size in comparison to the structure being monitored, durability against environmental actions, cost, and diﬃculty in applying and maintenance. Nanomodiﬁed cementitious materials can be used to manufacture sensors to be embedded at critical locations of reinforced concrete (RC) frames or to produce entire structural elements, enabling in both cases automated SHM. Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
216 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
The chapter is organized as follows. Section 9.2 reports a summary about the state of the art of nanomodiﬁed structures. Section 9.3 describes an example focused on the characterization of electrical and electromechanical properties of nanomodiﬁed sensors. In Section 9.4, smart cement paste sensors were used for the dynamic strain monitoring of a full-scale structural element. Section 9.5 describes results obtained performing tests on small scale structural elements entirely made with nanomodiﬁed cemen titious material, subjected to diﬀerent load cases. Sections 9.6 and 9.7 conclude the work with remarks and comments.
9.2 State of the Art of Nanomodified Structures Carbon nanotubes (CNTs), in particular multiwalled carbon nano tubes (MWCNTs), thanks to their particular aspect ratio and excellent electrical and mechanical properties, are the most promising conductive nanoinclusions for cementitious material [1–7]. One important ﬁeld of research regarding the developing of this nanotechnology is represented by the study of the dispersion of nanoinclusions into cement-based materials, as concrete or cement paste [8, 9], and of the fabrication process of the composite materials [10–12]. The addition of CNTs to the base material enhances its electrical and piezoresistive properties, so a nanomodiﬁed cement based sensor can be deﬁned as a strain-sensing sensor where measurable changes in its electrical resistance, under static or dynamic compressive load, can be associated to the applied strain [13–21]. This attractive capability has encouraged the embedding of nanocomposite sensors inside structural elements, allowing their SHM [22, 24]. Moreover, an interesting research task with regard to the possibility of use cementitious materials doped with CNTs to detect, localize, and quantify damage [25–28] occurred at crit ical structural components, transforming the monitored structure into a self-sensing system enabling real-time condition assess ment, reducing overall maintenance expenditures, and increasing safety.
Cement-Based Sensors for Structural Health Monitoring 217
9.3 Cement-Based Sensors for Structural Health Monitoring The section reports the results of an investigation presented in Ref. , where a set of MWCNT cement-based sensors were manufactured and tested in the laboratory in order to analyze the repeatability of electrical outputs and of strain-sensing capabilities of composite nanomodiﬁed specimens using two diﬀerent measure ment methods. Ten cube specimens of 5 cm sides, characterized by a cement paste matrix, were doped with 1% of MWCNTs type Arkema Graphistrength C100 , with respect to the weight of cement (Fig. 9.1). The dispersion of the nanoinclusions (Fig. 9.2) was achieved by performing a preliminary mechanical mixing, with a physical dispersant, followed by a sonication procedure. The obtained stable water suspension was mixed with the cement matrix and a plasticizer. The used cement was 42.5 pozzolanic, with a water/cement ratio of 0.45. Specimens were poured into oiled molds
Figure 9.1 Geometry of the samples and electrodes (dimension in cm) (a) and picture of the fabricated samples with strain gauges installed onto lateral surfaces (b)  (open access).
218 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
(i) Preparation of nanosuspension
(ii) Preliminary mixing
(iv) Mixing of paste
(v) Forming of samples with electrodes
(vi) Curing of the samples
Figure 9.2 Preparation process of the cement paste samples with 1% of MWCNTs  (open access).
and four stainless steel meshes, used as electrodes, were embedded into each sample before solidiﬁcation. The internal meshes were placed at a mutual distance of 2 cm, while the outer ones were at a distance of 4 cm. Samples were unmolded, after solidiﬁcation, for a curing phase of 28 days at laboratory conditions. Two electrical strain gauges, 2 cm long, with a gauge factor of 2.1, were placed onto the center of the opposite lateral sides of each specimen. Electrical tests in DC current were performed with both two probe and four-probe setups in order to investigate the electrical properties of the cement-based sensors, using a NI PXIe-1073, a data acquisition system (DAQ) composed of a chassis with dedicated modules. Electric power was supplied through an NI PXI-4130 module capable of providing a four-quadrant ±20V and ±2A output in a single isolated channel, while electrical measurements were conducted using a high-speed digital multimeter, type NI PXI-4071, which acquired current in the two-probe measurement setup and voltage in the four-probe measurement setup. To reduce the signal drift due to the dielectric nature of the cementitious matrix, a polarization of 6000 s was performed. The electrical resistance was computed at the end of this phase using the ﬁrst Ohm’s law adapted at both measurement methods. The following equations refer to two-probe (1.0) and four-probe (2.0) methods: V , (9.1) R2P (t) |t=tp = I (t) |t=tp V (t) |t=tp , (9.2) I where V and I are the applied constant voltage and current, respec tively; V (t) ad I (t) are the measured voltage variations and current intensity over time, respectively; and tp is the polarization time. R4P (t) |t=tp =
Cement-Based Sensors for Structural Health Monitoring 219
Times (s) Cyclical load
Figure 9.3 Applied cyclical (a) and dynamic (b) uniaxial loads for electromechanical tests  (open access).
Using the two-probe method, where the inner stainless steel meshes were used as active electrodes, the specimens were subjected to an electrical voltage of 5 V with a current measurement range of 1.0 mA. Otherwise, using the four-probe method, samples were subjected to 15 mA with a voltage measurement range of 10 V, where the current was applied to the external stainless steel meshes and the voltage drop was measured at the internal electrodes. Electromechanical tests were performed to evaluate the strain– sensing capability of each specimen. Electrical measurements were performed with the setup used during electrical tests. An additional module PXIe-4330, with 8 channels, 24-bit resolution, 25 kHz maximum sampling rate, and anti-aliasing ﬁlters, was added to the chassis NI PXIe-1073 to acquire data from strain gauges. Two types of compression loads were applied on each sample: a cyclic load, varying from 0.5 to 2.0 kN with 1 kN/s constant speed, and a dynamic load, varying from 0.5 to 1.5 kN characterized by an increasing application frequency from 0.25 to 8.0 Hz (Fig. 9.3). Loads were applied using a servocontrolled pneumatic universal dynamic testing machine, model IPC Global UTM 14P, with a controlled temperature chamber (Fig. 9.4). A polarization phase of 10 min was performed before the application of each load history. A voltage equal to 5 V with a current measurement range of 1.0 mA was applied in the two-probe conﬁguration, while a current of 15 mA was applied with a voltage measurement range of 10 V using the
220 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.4 Sketch and pictures of the setup for the electromechanical tests on cement-based samples with carbon nanotubes: power source and device for acquisition of strain gauges and electrical measurements (a), a sample during test (b), and data acquisition system of the hydraulic actuator (c)  (open access).
four-probe method. The sampling rate was 1000 Hz. Electrical resistance was computed considering the ﬁrst Ohm’s law, while the gauge factor of each sensor was computed applying the following relation: R = −λε, (9.3) R0 where R is the variation in electrical resistance, R 0 is the value of the resistance without applied load, λ is the gauge factor, and ε is the axial strain, positive in compression. Both electrical and electromechanical tests were carried out under a controlled temperature of 20◦ C. Figure 9.5 presents results obtained from electrical tests. The average value of the electrical resistance obtained using the two probe method is 609 , while the four-probe approach has provided a lower average value of 215 due to the electrical conﬁguration, which is able to remove the electrical contact resistance from the measured value . The corresponding coeﬃcients of variation, 0.16 and 0.24, demonstrate that the repeatability of the sensors’ electrical resis tance is satisfying, especially considering the two-probe method for
Cement-Based Sensors for Structural Health Monitoring 221
Figure 9.5 Results of the electrical measurements conducted on all of the carbon nanotube cement-based sensors (COV denotes the coeﬃcient of variation) using two-probe (a) and four-probe (b) methods  (open access).
which the obtained coeﬃcient of variation is very similar to the coeﬃcient of variation of other properties of cementitious materials, such as their compressive strength . Scattered values of the electrical resistance have been obtained owing to the non-uniform dispersion of the nanoﬁllers during the manufacturing process. Figures 9.6 and 9.7 show examples of time histories of the average strain, ε(t), measured using strain gauges and of the normalized change in electrical resistance, R, obtained from electromechanical tests performed on a sensor for both static and dynamic loads using the four-probe method. As expected,
222 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.6 Results of electromechanical tests: measured average strain (a) and normalized variation of electrical resistance (b) on sample number 6 (typical) using the four-probe method under cyclical loads. (a)
Figure 9.7 Results of electromechanical tests: measured average strain (a) and normalized variation of electrical resistance (b) on sample number 6 (typical) using the four-probe method under dynamic loads  (open access).
Figure 9.8 Plots of gauge factors (a) and of normalized resistance variation (b) with increasing frequency of applied load using the two-probe method.
Cement-Based Sensors for Structural Health Monitoring 223
Figure 9.9 Plots of gauge factors (a) and of normalized resistance variation (b) with increasing frequency of applied load using the four-probe method.
224 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Structures with Embedded Cement-Based Sensors 225
the application of a compression load provides negative changes in electrical resistance, R(t), acquired through the sensor. This behavior is due to an average reduction in the distance between nanotubes and the enhancement of the tunneling eﬀect. As shown in the ﬁgures, this change in electrical resistance is reversible when the value of applied compression load decreases. Electrical signals are characterized by very low noise and a clear strain sensitivity can be noted in all the graphs. Figures 9.8 and 9.9 present the variations in gauge factor and normalized change in electrical resistance, varying the application load frequency, carried out for the two- and the four probe method, respectively. These curves are useful to assess the strain-sensing capability of the sensors at diﬀerent frequencies, considering that an ideally dynamic sensor would have a horizontal frequency response func tion. Results show good strain-sensing capability of the sensors with more scattered values of gauge factors, which are characterized by variation coeﬃcients of 1.72 and 1.79 computed for the two-probe and four-probe methods, respectively. This behavior is probably due to the proximity of the 1% MWCNT mix to the percolation threshold. As demonstrated in Ref.  the gauge factor reached the maximum value close to the percolation threshold, but it is also very sensitive to small changes in the nanoﬁller dispersion. Reported results demonstrated the potential of the nanocompos ite cement paste sensors for the SHM of RC buildings, thanks to their strain-sensing capability. The scattered values of the sensors’ gauge factor can be solved through the calibration of each sensor before its embedding into a structural element.
9.4 Structures with Embedded Cement-Based Sensors To investigate the behavior of nanocomposite cement-based sensors when they are embedded in a concrete structural element, seven specimens, previously calibrated, were inserted into a full-scale RC beam during its molding.
226 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.10 Sketch of the full-scale beam test setup (a), picture of the beam with the embedded sensors (b), and detailed view of the sensors at the midspan (c)  (open access).
The beam, simply supported by two steel supports installed at a distance of 200 cm, had a square cross section of 25 × 25 cm2 and a length of 220 cm. Concrete was reinforced with 8-mm-diameter longitudinal steel rebars and stirrups. The sensors were instrumented in order to acquire elec trical output and strain gauges measurements, as shown in Fig. 9.10. The electrical measurements were carried out using the two probe method. Data acquisition was performed with the chassis NI PXIe-1073 characterized by the same setup used during the elec tromechanical tests on the sensors described in the previous section. The RC beam was involved in two diﬀerent electromechanical tests, which consisted of the application of a distributed static load of 1 kN/m and in the application of random hits in time and space
Structures with Embedded Cement-Based Sensors 227
Figure 9.11 Time histories of average strain (a) and measured electrical current (b) during static loading and unloading of the full-scale RC beam  (open access).
using an instrumented hammer. A polarization phase of 30 min was performed before each test. The instrumented sensor was subjected to a voltage of 2.5 V with a current measurement range of 1.0 mA. The sampling rate was 1000 Hz. Figure 9.11 shows the results obtained from the application of the static load on the RC beam. The plots report the time histories of the average strain, measured by the strain gauges placed on the sensor embedded in the middle of the beam, and of the electrical current output provided by the sensor itself. Loading and unloading phases are clearly visible in both signals, demonstrating that the sensor detects changes in strain occurring in the beam’s compression zone during the test. Figure 9.12 reports results obtained from the vibration test in which the RC beam was hit with a hammer. To eliminate the residual eﬀect of the polarization, a high-pass ﬁlter, with a cut-oﬀ frequency of 5 Hz, was applied to the signal. Random hammer hits are clearly visible in the time history of the electrical current reported in Fig. 9.12a. Furthermore, a detailed view of a single hammer hit is shown in Fig. 9.12b in order to point out the waveform of the damped vibration of the RC beam. Afterward, an in-depth study of the strain-sensing capability
228 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.12 Section of the time history of the current during vibration tests (a) and detailed view of the output of a single hammer hit (b)  (open access).
of the sensor was performed. Figure 9.13a reports the overlapped ﬁltered signals of the measured strain, computed considering the average value obtained from the outputs of the two strain gauges applied on the sensor and of the estimated strain, computed using Eq. 9.3 from the electrical output provided by the sensor itself. Results reported in Fig. 9.13 show a clear correspondence between measured and computed strain, as conﬁrmed by the signal magniﬁcations shown in Figs. 9.13b and 9.13c. Moreover, a spectral analysis of the strain and of the electrical current outputs, respectively, provided by strain gauges and by the sensor, was performed in order to understand whether the sensors, embedded in the RC beam, can be used for output-only modal identiﬁcation and vibration-based SHM of the structural element. The power spectral density (PSD) functions of the strain signal, measured by the strain gauges, and of the electrical current, obtained from the sensor, have been reported in Fig. 9.14 applying a high-pass ﬁlter with a cut-oﬀ frequency of 5 Hz. Both PSD functions are characterized by the same leading peak at a frequency of 64.45 Hz that can be associated with the ﬁrst vertical vibration mode of the RC beam.
Structures with Embedded Cement-Based Sensors 229
Figure 9.13 Time histories of measured average strain from strain gauges and estimated strain from electrical measurements (a). Enlarged view of measurements number 1 (b) and number 2 (c)  (open access).
Figure 9.14 PSD of strain gauges measurements (a) and of electrical measurements (b) from the embedded sample placed at midspan  (open access).
230 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Results have demonstrated that embedded MWCNTs sensors are suitable to monitor the strain conditions of a full-scale structural element subjected to a static or a dynamic load. In addition, it has been demonstrated that embedded sensors can be used for output-only modal identiﬁcation and vibration-based SHM of a structural element.
9.5 Structures Made of Nanomodified Cement-Based Materials A very attractive solution in the ﬁeld of the SHM of RC buildings con cerns the possibility of manufacturing speciﬁc structural elements with nanomodiﬁed materials, which, placed at key points of the structure, are able to achieve smart diﬀuse monitoring. An interesting investigation on this topic is reported in Ref. , where a steel-reinforced cement-based beam, made with cement paste doped with 1% of MWCNTs with respect the weight of the cement, was subjected to a four-point loading test up to failure. Furthermore, the paper presents a resistor mesh model developed in order to anticipate the electrical response of smart concrete structural elements with the purpose to allow their real time monitoring. Nanoﬁllers were dispersed into deionized water with a sur factant (lignosulfonic acid sodium salt) using mechanical mixing followed by a sonication procedure. The obtained solution was mixed with type IV Portland cement. Following, the smart cement paste was cast in a prismatic mold with dimensions of 100 × 100 × 500 mm3 and 16 steel electrodes were embedded in the bottom rectangular side. The electrical tests were conducted with a DC biphasic method , in which a function generator was used to provide a 2 Hz square wave, ranging from −2.5 to 2.5 V, characterized by a duty cycle of 50%, to the electrodes of the specimen. This approach allows the simultaneous measurements of the voltage drop of every section of the reinforced MWCNT cement paste beam between two electrodes, eliminating also the drift eﬀect that aﬄicts electrical outputs of dielectric materials, through cycles
Structures Made of Nanomodified Cement-Based Materials 231
of charging and discharging. Resistance, R, was computed through the following equation: Vsense , (9.4) R= i where Vsense is the measured voltage drop and i is the ﬂowing current between two electrodes computed considering the relation Vdrop , (9.5) i= Rin-line where Vdrop is the voltage drop across a resistor characterized by an electrical resistance of Rin-line . The aim of the work was to propose and validate a procedure, based on a resistor mesh model, to detect, localize, and quantify cracks in self-sensing concrete structures, considering permanent local changes in electrical resistance induced by cracks. In fact,
Figure 9.15 A resistor mesh model with a 10 × 5 resistor mesh for crack detection, localization, and quantiﬁcation in cement composite structures with key components highlighted. Reprinted from Ref. , Copyright (2017), with permission from Elsevier.
232 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
when a crack opens, a greater voltage drop occurs in the element. The developed 2D resistor mesh model, fully explained in Ref. , is composed by strain-sensitive, contact, and damage resistors, as shown in Fig. 9.15, where an example of a resistor mesh model is illustrated. Changing in strain and damage can be detected by a resistor model through the variation of the resistive value of individual resistors. To this purpose, a ﬁnite element analysis (FEA) model of the reinforced MWCNTs cement paste beam was built to validate the behavior of the strain-sensitive resistors present in the resistor mesh model, which was solved using SPICE , an open source analog electronic circuit simulator. The results of the FEA model were compared with those obtained from six strain gauges placed on both the lateral surfaces of the beam. A four-point loading test was performed applying 24 loading steps with an increment of 0.1 kN. An audible crack was heard during the application of 1.8 and 1.9 kN loads. Figure 9.16 shows the experimental setup for the reinforced MWCNT cement paste beam. A damage, localized on the intrados of the left-most monitored section and developed during the four-point loading test, has been reported in Fig. 9.16a. Minor multiple cracks, developed on the surface of the beam, were photographed to allow crack monitoring during the conduction of the test. Figure 9.17 presents a comparison between the results obtained from experimental tests and from the analytical model for the healthy state of the beam. The experimental trend denotes a large voltage drop occurred in sections 6, 7, and 8 due to the presence of cracks and a slight cavity localized on the top of the beam. Electrical outputs, obtained for reference sections of the beam, performing the four-point loading test are illustrated in Fig. 9.18a. In the center section 8, it is possible to note that the voltage drop increases with the increase of the applied load until reaching 1.4 kN when the value of the electric output starts to decrease. This behavior is due to the formation of several microcracks, starting at the loading step 1.4 kN, which implies a loss in the strain-sensing capability of the material. Due to the symmetric loading condition applied on the beam, each pair of sections, localized externally respect the center section, demonstrated a constant change in voltage drop, as expected. In the plot, outputs of sections 4 and 12
Structures Made of Nanomodified Cement-Based Materials 233
Figure 9.16 Experimental setup for the self-sensing reinforced cement paste beam: (a) annotated diagram labeling key components of the test setup and (b) experimental setup as tested (with the load-bearing clamp removed for clarity). Reprinted from Ref. , Copyright (2017), with permission from Elsevier.
and sections 6 and 10 conﬁrm such behavior. The trend of the change in voltage drop outputted by the section 1 conﬁrms the development of a crack, occurring during the loading test, at the left-adjacent section (Figs. 9.18b and 9.18d). On the other side, in section 15, the decrease of the voltage drop is a consequence of the increment that occurred in section 1. Figure 9.18c shows the strong agreement between the experimental and analytical results found in sections 1 and 15. Both results show an increment in the change of the voltage drop due to the developed of the crack at the left-most side of section 1. Damage resistors were added to the resistor mesh model in order to reproduce the observed experimental behavior. To take
234 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.17 Experimental analytical model results for the healthy state of specimen III. Reprinted from Ref. , Copyright (2017), with permission from Elsevier.
into account the presence of a pre-existing crack of 4 mm on the outside of the left-most contact, a ﬁrst resistor was added to the model. Then, another resistor was inserted to consider the 4 mm crack that occurred applying a load of 1.8 kN. A last resistor was introduced to consider the damage associated at 1.9 kN. The total simulated crack has a length of 10 mm. Results obtained from experimental electrical measurements have demonstrated that concrete structural elements with CNTs can provide a measurable change in electrical outputs that can be related to the damage states that occur at diﬀerent sections of the element. Moreover, analytical results obtained from the developed resistor mesh model, proposed and validated in Ref. , have demonstrated a reliable matching with the experimental results. Another relevant example of a structural element made with nanomodiﬁed cementitious material is presented in Ref. . In this work, a cement paste plate 500 × 500 × 50 mm3 , doped with 1% of MWCNTs with respect to the weight of the cement, was subjected to progressive damage developed performing repetitive impact tests. The aim of the paper was to analyze a 2D resistor mesh model developed from the resistors’ system, proposed and validated in Ref. , adding a procedure for the automated placement of resistors using a sequential Monte Carlo method. The analytical model was validated comparing its results with those obtained from the experimental tests. During the manufacturing of the specimen, Arkema C100 MWC NTs  were ﬁrst mechanically mixed with water and a surfactant
Structures Made of Nanomodified Cement-Based Materials 235
Figure 9.18 Experimental data and analytical model results for specimen III, showing: (a) measured change in voltage drop as a function of the applied load, (b) crack detected outside section 1, (c) analytical model versus experimental results for voltage drop measured at section 1, and (d) bottom view of the surface crack on the outside of section 1. Reprinted from Ref. , Copyright (2017), with permission from Elsevier.
and then dispersed using a sonication procedure. The obtained nanomodiﬁed suspension was mixed with cement powder to obtain a smart cement paste. The doped material was cast into a mold, adding steel nets with wires of 1.2 mm diameter, as reinforcement, arranged in a 60 × 60 mm2 grid. During the curing of the plate, ﬁfty-six 1.2 mm copper wires were embedded into the smart concrete material in a grid of 80 × 80 mm2 , as shown in Fig. 9.19. Electrical measurements were carried out using a DC biphasic method  where a constant 20 V pp square wave, with a frequency
236 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.19 Key components and dimensions of the 500 × 500 × 50 mm3 c IOP smart cement paste specimen used in this study. From Ref. . � Publishing. Reproduced with permission. All rights reserved.
of 1 Hz and a duty cycle of 50%, was applied by a function generator, model Rigol DG1022a, to the active copper electrodes embedded in the plate. To avoid the inﬂuence of the contact resistance between copper contacts and MWCNT cement paste, voltage measurements were directly acquired at each embedded electrode using dedicated modules, model PXIe-4302 and PXIe-6361, arranged in a chassis, type PXIe-1071. Simultaneous acquisition of the electrodes was allowed through a wire connecting them. The voltage values were taken at 80% of the constant part of the acquired voltage signal and were used as input to the resistor mesh model. Testing validation was performed acquiring the biphasic signal with an oscilloscope, model Rigol DS-1054. Diﬀerent conﬁgurations of the resistor mesh model were investigated in order to establish a suitable setup capable to mimic the conductive paths of the MWCNT cement paste plate. Figure 9.20 shows the applied model where 110 resistors were implemented to connect the electrodes of the plate. Diagonal resistors are independent and do not form a conductive path. The procedure used to place damaged resistors in the resistor
Structures Made of Nanomodified Cement-Based Materials 237
Figure 9.20 The resistor mesh model used for electrical modeling of the c IOP Publishing. Reproduced with permission. All plate. From Ref. . � rights reserved.
Figure 9.21 Experimental test setup showing (a) key components used in the impact testing of the smart cement paste plate with an embedded copper contact shown in the inset and (b) electrical test schematic showing the connection of the data acquisition system to the test specimen with c IOP Publishing. key system components annotated. From Ref. . � Reproduced with permission. All rights reserved.
238 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.22 A purely data-driven damage detection analysis (no resistor mesh model) for the test plate showing (a) damage and the location of inspection points and (b) the change in the plate’s total resistance and the change in voltage data taken at the three inspection points of interest, selected to show damage forming during diﬀerent portions of the test. c IOP Publishing. Reproduced with permission. All rights From Ref. . � reserved.
mesh model is based on a bi-optimization objective function that is capable, ﬁrst, to recognize points where the highest error between experimental and analytical measurements occurs, and then in a second step, to minimize the value of the mean error at the considered points. A sequential Monte Carlo algorithm is used to estimate a resistor set that best reproduces the spatial resistance distribution in the conductive nanomodiﬁed cement paste plate. More details of the used resistor mesh model and of the procedure can be found in Ref. . Experimental tests were performed on an extruded aluminum frame equipped with a 3 kg hammer, as reported in Fig. 9.21, where the experimental setup is full shown. The impact of the hammer on the plate produced a 1.5 J of energy and it was carried out rotating back 20◦ the hammer from the initial position. The test was conducted hitting 100 times the center of the plate. The damage state of the plate is reported in Fig. 9.22a, while Fig. 9.22b presents electrical outputs obtained from the embedded copper contacts. Plate global health was monitored assessing the total resistance value of the specimen obtained through electrical measurements with a two-probe method. The trend of the solid red line indicates that the majority of the damage occurred during the
Structures Made of Nanomodified Cement-Based Materials 239
Figure 9.23 Final damage detection results showing (a) spatial distribution of high-value resistors for the healthy state, (b) healthy test specimen, (c) spatial distribution of high-value resistors for the damaged state with crack distribution overlaid to show relationship between damage and points of high resistance, and (d) damaged (100 impacts) test specimen. c IOP Publishing. Reproduced with permission. All rights From Ref. . � reserved.
ﬁrst 25 hammer impacts, producing an increase in the value of the electrical resistance. Then, such a feature continued to increase with a lower rate. The damage localization was investigated monitoring the voltage at three plate electrodes placed in diﬀerent positions respect to the developed crack path clearly visible in Fig. 9.22a. The dashed blue line, reported in Fig. 9.22b, corresponds to a copper contact located in an undamaged area of the plate. It can be noted that the measured voltage increases during the test probably to balance voltage drops that occur at other electrodes located in damaged areas. The orange dot-dashed line refers to the measured
240 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
Figure 9.24 Final results for the plate showing the relative resistance change in resistance for the damaged condition when compared to the c IOP Publishing. Reproduced with healthy condition. From Ref. . � permission. All rights reserved.
voltage at an electrode placed where a crack visually occurs after a few hits of the hammer, as conﬁrmed by the marked voltage drop presented at the beginning of the output. The dotted green line refers to a copper contact placed near a crack formed around hammer impact 60. Its voltage trend varies during the test in relation to the developing of the neighboring cracks. Analytical results obtained from the resistor mesh model are presented in Fig. 9.23, compared to the healthy and damaged states of the plate. Moreover, Fig. 9.24 reports the change in electrical resistance computed at the end of the test. The resistor mesh model, built with the sequential Monte Carlo algorithm, detects three prominent damage areas on the plate: the hammer impact point, located in the center of the specimen; a damaged area located on the bottom center (front and back) of the plate, where a loss of material occurred after a few hammer hits; and an area above the center right, where a piece of cement paste, on the back of the plate, was lost around hammer hit 80. Results from experimental tests have demonstrated how a structural element made with nanomodiﬁed cement paste is able
to provide electrical output useful to monitor its health state. The assessment of the plate’s global health can be performed from the evaluation of the total electrical resistance, while outputs of voltage can detect and localize crack paths that occur on the structural element. Furthermore, analytical results obtained from the resistor mesh model demonstrated the possibility to enable the real-time detection, localization, and quantiﬁcation of a crack path.
9.6 Comments Several applications of carbon cement–based sensors have been presented in this chapter. Ten cube MWCNT cement paste sensors were subjected to electrical and electromechanical tests where electrical measure ments were conducted using both two-probe and four-probe methods. Results from electrical tests have demonstrated that the dispersion of MWCNTs in the cement-based material results in a key point for the repeatability and feasibility of the electrical measurement. However, even if some scattered values occur, a good repeatability of the electrical outputs has been found, especially performing measurements with the two-probe setup. Results from electromechanical tests demonstrated the strain-sensing capability of the cube sensors for both static and dynamic load cases. Scattered values of the gauge factor (GF) were due to the proximity of the ﬁller content to the percolation threshold. This occurrence suggests the individual calibration of each sensor before its embedding in a structural element should be monitored. Results obtained from electromechanical tests have conﬁrmed that smart sensors are capable of detecting static loads and dynamic inputs. Embedded sensors can be also used for output-only modal identiﬁcation and vibration-based SHM. Experimental tests also demonstrated that cement-based nanomodiﬁed materials can be utilized as constituent materials for structural smart elements. Performed tests have demonstrated that the nanomodiﬁed material can provide a measurable change in electrical voltage that can be related to the developing of cracks in the material. Also, analytical results obtained
242 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
from the model showed satisfactory agreement with those obtained from experimental tests. Impact tests performed on a MWCNT cement paste plate produced relevant results useful to improve the interpretation of electrical outputs obtained from a smart structural element and to assess its health state. The evaluation of the electrical resistance allowed assessment of the global health state of the plate, while detecting, localizing, and quantifying the damage occurred in the structural element. An automated procedure, based on a sequential Monte Carlo algorithm, allowed the automated updating of the damage resistors in the model. The analytical results have conﬁrmed the potential of this approach.
9.7 Conclusion The discussed examples have demonstrated some promising ap plications of nanocomposite cement-based materials for civil engi neering application, especially for smart SHM of concrete buildings. Nanomodiﬁed sensors can be embedded at critical positions of a concrete frame, or entire structural elements can be manufactured with such a material. Moreover, the results demonstrated that this technology can be fruitfully used to monitor changes in load and crack paths due to the application of static and dynamic loads.
References 1. Makar, J., Beaudoin, J. (2003). Carbon nanotubes and their application in the construction industry, in Bartos, P. (ed.) Proceedings of the 1st International Symposium on Nanotechnology in Construction (NICOM 2003), Springer Verlag, Berlin Heidelberg, pp. 331–341. 2. Mondal, P., Shah, S. P., Marks, L. D. (2008). Nanoscale characterization of cementitious materials, ACI Mater. J., 105, pp. 174–179. 3. Yu, X., Kwon, E. (2009). Acarbon nanotube/cement composite with piezoresistive properties, Smart Mater. Struct., 18(5), p. 055010. 4. Materazzi, A. L., Ubertini, F., D’Alessandro, A. (2013). Carbon nanotube cement-based transducers for dynamic sensing of strain, Cem. Concr. Compos., 37(1), pp. 2–11.
5. Han, B., Zhang, K., Yu, X., Kwon, E., Ou, J. (2012). Electrical charac teristics and pressure-sensitive response measurements of carboxyl MWNT/cement composites, Cem. Concr. Compos., 34(6), pp. 794–800. 6. Gdoutos, E. E., Konsta-Gdoutos, M. S., Danoglidis, P. A., Shah, S. P. (2016). Advanced cement based nanocomposites reinforced with MWCNTs and CNFs, Front. Struct. Civ. Eng., 10(2), pp. 142–149. 7. D’Alessandro, A., Ubertini, F., Materazzi, A. L., Laﬂamme, S., Porﬁri, M. (2014). Electromechanical modelling of a new class of nanocomposite cement-based sensors for structural health monitoring, Struct. Health Monit., 14(2), pp. 137–147. 8. D’Alessandro, A., Rallini, M., Ubertini, F., Materazzi, A. L., Kenny, J. M. (2016). Investigations on scalable fabrication procedures for self-sensing carbon nanotube cement-matrix composites for SHM applications, Cem. Concr. Compos., 65, pp. 200–213. 9. Hilding, J., Grulke, E. A., Zhang, Z. G., Lockwood, F. (2003). Dispersion of carbon nanotubes in liquids, J. Dispersion Sci. Technol., 24(1), pp. 1–41. 10. Han, B., Ding, S., Yu, X. (2015). Intrinsic self-sensing concrete and structures: a review, Measurements, 59, pp. 110–128. 11. Nadiv, R., Vasilyev, G., Shtein, M., Peled, A., Zussman, E., Regev, O. (2016). The multiple roles of a dispersant in nanocomposite systems, Compos. Sci. Technol., 133, pp. 192–199. 12. Ubertini, F., Laﬂamme, S., Ceylan, H., Materazzi, A. L., Cerni, G., Saleem, H., D’Alessandro, A., Corradini, A. (2014). Novel nanocomposite tech nologies for dynamic monitoring of structures: a comparison between cement-based embeddable and soft elastomeric surface sensors, Smart Mater. Struct., 23, p. 12. 13. Han, B., Ou, J. (2007). Embedded piezoresistive cement-based stress/ strain sensor, Sens. Actuators, A, 138(2), pp. 294–298. 14. Hou, T.-C., Lynch, J. P. (2005). Conductivity-based strain monitoring and damage characterization of ﬁber reinforced cementitious structural components, in Proceedings of the Smart Structures and Materials 2005: Sensors and Smart Structures Technologies for Civil, Mechanical, and Aerospace Systems, pp. 419–429. 15. Cao, J., Chung, D. D. L. (2004). Electric polarization and depolarization in cement-based materials, studied by apparent electrical resistance measurement, Cem. Concr. Res., 34, pp. 481–485. 16. Wen, S., Chung, D. D. L. (2000). Damage monitoring of cement paste by electrical resistance measurement, Cem. Concr. Res., 30, pp. 1979–1982.
244 Use of Carbon Cement–Based Sensors for Dynamic Monitoring of Structures
17. Loh, K. J., Gonzalez, J. (2015). Cementitious composites engineered with embedded carbon nanotube thin ﬁlms for enhanced sensing performance, J. Phys. Conf. Ser., 628, p. 012042. 18. Xie, P., Gu, P., Beaudoin, J. J. (1996). Electrical percolation phenomena in cement composites containing conductive ﬁbers, J. Mater. Sci., 31, pp. 4093–4097. 19. Wen, S., Chung, D. D. L. (2007). Double percolation in the electrical conduction in carbon ﬁber reinforced cement-based materials, Carbon, 45, pp. 263–267. 20. Azhari, F., Banthia, N. (2012). Cement-based sensors with carbon-ﬁbers and carbon nanotubes for piezoresistive sensing, Cem. Concr. Compos., 34(7), pp. 866–873. 21. Han, B., Zhang, K., Yu, X., Kwon, E., Ou, J. (2012). Electrical charac teristics and pressure-sensitive response measurements of carboxyl MWNT/cement composites, Cem. Concr. Compos., 34(6), pp. 794–800. 22. Han, B., Yu, X., Kwon, E. (2009). A self-sensing carbon nanotube/cement composite for traﬃc monitoring, Nanotechnology, 20, p. 445501. 23. Saaﬁ, M. (2009). Wireless and embedded carbon nanotube networks for damage detection in concrete structures, Nanotechnology, 20, p. 395502. 24. Ubertini, F., Materazzi, A. L., D’Alessandro, A., Laﬂamme, S. (2014). Natural frequencies identiﬁcation of a reinforced concrete beam using carbon nanotube cement-based sensors, Eng. Struct., 60, pp. 265–275. 25. Chen, B., Liu, J. (2008). Damage in carbon ﬁber-reinforced concrete, monitored by both electrical resistance measurement and acoustic emission analysis, Constr. Build. Mater., 22(11), pp. 2196–2201. 26. Vertuccio, L., Vittoria, V., Guadagno, L., De Santis, F. (2015). Strain and damage monitoring in carbon-nanotube-based composite under cyclic strain, Composites Part A, 71, pp. 9–16. 27. Wang, S., Chung, D. D. L. (2006). Self-sensing of ﬂexural strain and damage in carbon ﬁber polymer-matrix composite by electrical resistance measurement, Carbon, 44(13), pp. 2739–2751. 28. Downey, A., Garcia-Macias, E., D’Alessandro, A., Laamme, S., CastroTriguero, R., Ubertini, F. (2017). Continuous and embedded solutions for SHM of concrete structures using changing electrical potential in self-sensing cement-based composites, in Felix Wu, H., Gyekenyesi, A. L., Shull, P. J., Yu, T.-Y. (eds.) Nondestructive Characterization and Monitoring of Advanced Materials, Aerospace, and Civil Infrastructure 2017, vol. 10169, Proc. SPIE.
29. D’Alessandro, A., Ubertini, F., Garc´ıa-Mac´ıas, E., et al. (2017). Static and dynamic strain monitoring of reinforced concrete components through embedded carbon nanotube cement-based sensors, Shock Vib., 2017, Article ID 3648403 (11 pp). 30. McAndrew, T. P., Laurent, P., Havel, M., Roger, C. (2008). Arkema R multi-walled carbon nanotubes, Technical Proceed Graphistrength� ings of the 2008 NSTI Nanotechnology Conference and Trade Show, NSTI-Nanotech, Nanotechnology, 1, pp. 47–50. 31. Wen, S., Chung, D. D. L. (2007). Piezoresistivity-based strain sensing in carbon ﬁber-reinforced cement, ACI Mater. J., 104(2), pp. 171–179. 32. NTC2008 Technical code for construction, DM 14 January 2008. 33. Downey, A., D’Alessandro, A., Baquera, M., Garc`ıa-Mac`ıas, E., Rolfes, D., Ubertini, F., Laamme, S., Castro-Triguero, R. (2017). Damage detection, localization and quantiﬁcation in conductive smart concrete structures using a resistor mesh model, Eng. Struct., 148, pp. 924–935. 34. Downey, A., D’Alessandro, A., Ubertini, F., Laamme, S., Geiger, R. (2017). Biphasic DC measurement approach for enhanced measurement stability and multi-channel sampling of self-sensing multi-functional structural materials doped with carbonbased additives, Smart Mater. Struct., 26(6), p. 065008. 35. Paolo Nenzi, H. V. (2014). Ngspice users manual - version 26, Paolo Nenzi, Holger Vogt, USA. 36. Downey, A., D’Alessandro, A., Ubertini, F., Laﬂamme, S. (2018). Auto mated crack detection in conductive smart-concrete structures using a resistor mesh model, Meas. Sci. Technol., 29(3).
INNOVATIVE APPLICATIONS OF ADVANCED
Cement-Based Piezoresistive Sensors for Structural Monitoring Ilhwan You,a Seung-Jung Lee,b and Doo-Yeol Yooc a School of Civil, Environmental and Architectural Engineering, Korea University,
145 Anam-ro, Seongbuk-gu, Seoul 02841, Republic of Korea
b Advanced Railroad Civil Engineering Division, Korea Railroad Research Institute,
176 Cheoldobangmulgwan-ro, Uiwang-si, Gyeonggi-do 16105, Republic of Korea
c Department of Architectural Engineering, Hanyang University, 222 Wangsimni-ro,
Seongdong-gu, Seoul 04763, Republic of Korea
[email protected]; [email protected]; [email protected]
10.1 Introduction Concrete has been the most widely used construction material for civil infrastructure and buildings for the past several decades. Be cause of its excellent mechanical strength, low cost, and durability, it has been eﬀectively applied to major structural elements, including columns, beams, slabs, etc., subjected to external loading. However, it has relatively poor tensile strength and toughness compared to those under compression, such that steel reinforcements, that is, reinforcing bars or prestressing strands, are generally incorporated, particularly where tensile stress occurs. This is because steel Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
250 Cement-Based Piezoresistive Sensors for Structural Monitoring
reinforcements show very ductile tensile behavior due to their yield ing plateaus, have a similar coeﬃcient of thermal expansion, and provide good bond performance with concrete. Thus, they have been broadly adopted for concrete structures. Such reinforced-concrete (RC) structures, however, deteriorate when steel reinforcements are corroded, mainly due to penetration of detrimental materials from outside concrete through cracks. In addition, concrete creep results in secondary stresses generated in RC structures, causing damage and structural integrity problems. Accordingly, structural health monitoring (SHM) techniques have attracted attention from engineers and researchers in order to monitor and investigate the structural integrity of existing large-scale structures . In most cases, SHM techniques are based on several types of attached and embedded sensors commercially available, including electric strain gauges (ESGs), ﬁber Bragg grating (FBG) sensors, and lead zirconate titanate (PZT)-based piezoelectric sensors , as shown in Fig. 10.1. Because of their advantages compared to conventional gauges—that is, high resistance to electromagnetic interference, long-term stability, light weight, and small size— numerous studies have been conducted by researchers since 1989 to measure mechanical strains and temperatures in structures. In the early 1990s, a study on PZT-based piezoelectric sensors was performed to detect damage in structures using impedance and intensive studies on the development of PZT-based piezoelectric sensors were conducted for practical applications to civil structures and buildings. Likewise, several types of sensors have been developed and intensively studied, but their practical applications have been very limited thus far. This is because, since the artiﬁcial sensors mentioned above are locally embedded and attached, only a local examination of the strain, temperature, and damage to RC
Figure 10.1 sensor.
Sensors commercially available: (a) strain gauge and (b) FBG
structures is feasible. The health monitoring of entire structures, therefore, is limited, and the artiﬁcial sensors must be applied after precise prediction of the weakest parts in structures. In addition, inaccurate estimation of the weakest parts of structures may lead the sensors to be useless for SHM . To overcome such drawbacks of the traditional sensors for SHM, numerous researchers [3–7] have developed a new type of self-sensing construction material, called cement-based sensors (CBS). To achieve electrical properties in a nonconductive cement composite, they have incorporated carbon-based nanomaterials, for example, carbon nanotubes (CNTs), graphene (G), carbon nanoﬁbers (CNFs), carbon ﬁbers (CFs), steel ﬁbers (SFs), carbon black (CB), and nickel powder. These novel self-sensing sensors oﬀer several advan tages over conventional sensors, such as low cost, high durability, and large sensing volume, and they don’t degrade the mechanical capacity of RC structures. In particular, most previous studies have focused on achieving piezoresistive properties in cement composites to monitor stress and strain variations based on changes in electrical resistivity. This special piezoresistive property could be obtained on the basis of the concept that the electrical resistivity of cement composites reinforced with conductive carbon materials varies with external force, since conductive pathways formed by connecting the carbon materials change due to deformation of the composites under force, as shown in Fig. 10.2. The electrical current can be transferred in cement composites as the conductive pathways are formed by direct connection with carbon materials. Furthermore, even though carbon materials are not in contact with each other, electrons move by the tunneling eﬀect (Fig. 10.2c) when the distance between carbon materials becomes closer under an
Figure 10.2 Schematic description of CNT links in composites: (a) without loading, (b) with loading, and (c) electrical tunneling eﬀect .
252 Cement-Based Piezoresistive Sensors for Structural Monitoring
external force. Xu et al.  proposed a cut-oﬀ distance between CNTs, one of the most widely used carbon nanomaterials, to achieve a tunneling eﬀect over 0.5 nm. Thus, to help the reader to broadly understand recent research trends on CBS for structural monitoring, we comprehensively examine the current state of knowledge. Our attention is focused on (1) conductive ﬁllers, such as carbon-based materials; (2) their dispersion, which can depend upon the quality of CBS; (3) the CBS state of the art; and ﬁnally (4) the practical applications of CBS with the carbon-based materials for SHM of civil infrastructure and buildings.
10.2 Various Types of Cement-Based Sensors 10.2.1 Piezoresistivity Piezoresistivity can be deﬁned as the change in resistance of a semiconductor due to applied mechanical stress. In detail, the sub jection of semiconductors to external forces can lead to deformation of their length or cross section; hence, the geometrical change in the electrical pathway results in semiconductor resistance. The change in resistance does not represent the characteristics of a speciﬁc object because resistance, having a unit , is deﬁned as the tendency of resisting the ﬂow of current. To evaluate the electrical properties of a semiconductor, the resistivity (ρ) should be adopted. The resistivity, also called speciﬁc resistance, is a characteristic value of the electrical property of the semiconductor under consideration of its geometry; its unit is · cm. The resistivity can be expressed as shown in Eq. 10.1: ρ=
where R, A, and L are the resistance, cross-sectional area, and length of the semiconductor, respectively. The evaluation of piezoresistive properties for semiconductors depends upon the change in resis tivity, ρ (ρ/ρ0 ) can be called the fractional change in resistivity
Various Types of Cement-Based Sensors
Figure 10.3 Example of cement-based sensors: (a, b) schematic diagrams and (c) true image.
(FCR) and is deﬁned as ρ (ρi − ρ0 ) = = FCR, ρ0 ρ0
where ρi is the changed resistivity of the semiconductor in the deformed state and ρ0 is the initial resistivity before application of the external load. The FCR can be transformed in a gauge factor (GF). The GF is one of the most important characteristics for evaluating semiconductor sensitivity. It can be calculated through comparison between change in resistivity and strain (ε), as in Eq. 10.3: GF =
FCR (ρ/ρ0 ) = ε ε
A representative CBS model based on the piezoresistive principle is introduced in Fig. 10.3. According to the measuring methods, two or four electrodes must be inserted into the CBS. In the case of a four-probe system, the inner and outer electrodes are linked with potential and voltage probes, respectively. The resistance of CBS will be measured in the section between the inner probes.
10.2.2 Cement-Based Composites Cement composites such as cement pastes, mortars, and concretes are typically heterogeneous and are produced by mixing cement and water, with or without aggregates (sand and gravel). According to the presence and type of aggregate, cement composites are divided into cement pastes and mortars (which have only sand)
254 Cement-Based Piezoresistive Sensors for Structural Monitoring
and concretes (which have both sand and gravel). Since cement composites are not electrically conductive materials on their own, a conductive ﬁller must be incorporated inside them to induce piezoresistivity. For mortars and concretes, the presence of aggregates can disturb the electrical pathway, thereby decreasing the self-sensing performance . Therefore, cement pastes are widely employed as matrices in these research ﬁelds.
10.2.3 Carbon-Based Materials (Conductive Fillers) To change cement composites into conductive materials, conductive ﬁllers should be incorporated at suﬃcient concentration. The suﬃcient amount is called the “percolation threshold.” If the ﬁllers are incorporated below the percolation threshold, the electrical conductivity will be governed by ionic conduction of cementitious materials and tunneling conduction, which takes place in electrical pathways with discontinuities no larger than 10 nm in length [8– 10]. However, at a similar or higher concentration compared to the percolation threshold, conductive ﬁllers are totally connected each other, meaning that continuous conductive ﬁllers can form electrical pathways. The percolation thresholds for carbon-based materials are given in Table 10.1. The carbon materials are frequently used as conductive ﬁllers and can be classiﬁed according to shape, ﬁber, and particle. Table 10.1 indicates the physical properties of carbon ﬁllers sorted by their shape, scale, and dimensions. Multiwalled carbon nanotubes Table 10.1 Physical properties of carbon-based materials and their percolation threshold
Type CNT CNF CF
Diameter (nm) [Ref.] 15  200  12,000– 18,000  120  2600 
Length (mm) [Ref.]
Aspect ratio (length/ diameter)
Percolation threshold (%) [Ref.]
0.01 0.01–0.03 5 
667 50–150 278–416 
1  0.5  0.5–1 
7.22–11.39  2.4 
Various Types of Cement-Based Sensors
Figure 10.4 Morphologies of carbon-based materials: (a) MWCNT , (b) CNF , (C) CF , (d) CB , and (e) G . (a, b, e) Reprinted from Ref. , Copyright (2019), with permission from Elsevier. (d) Reprinted from Ref. , Copyright (2017), with permission from Elsevier.
(MWCNTs), CNFs, and CFs are ﬁber types having an aspect ratio, CB and GP are powder types, and G and nanographite platelet (NGP) are laminar types. Figure 10.4 indicates images obtained from scanning electron microscopy on CNTs, CNFs, CFs, CB, and G. According to previous research [9, 17–20], the self-sensing properties of CBS can be aﬀected by the morphology of functional ﬁllers, such as shape and size. Fiber-type ﬁllers having high aspect ratios (i.e., ratio of length to diameter) can secure the sensing ability of concrete at lower concentrations than particle ﬁllers. The eﬀective concentration is not higher than 1% for ﬁbrous ﬁllers, whereas it is at least 5% for particle ﬁllers. However, the dispersion of ﬁber type ﬁllers in a cement matrix is diﬃcult since their aspect ratios can be entangled with one another. Hence, poor dispersion of carbon materials can induce mechanical defects and unbalance the self sensing quality. Moreover, nanoscale carbon-based ﬁllers such as CNTs, graphite nanoﬁbers, G, and graphene oxide (GO) lead easily to self-agglomeration due to the van der Waals force. Thus, the dis persion of nanoscale carbon-based ﬁllers is necessary in the ﬁeld of
256 Cement-Based Piezoresistive Sensors for Structural Monitoring
self-sensing. Details concerning the dispersion of nanoscale carbon based materials are discussed in Section 10.2.4.
10.2.4 Dispersion of Carbon-Based Nanomaterials in Cement-Based Composites As mentioned in the previous section, the dispersion of carbon based ﬁllers is the most important issue in the ﬁeld of CBS, as well as research areas where carbon nanomaterials are used. A great deal of research toward achieving uniform dispersion of carbon materials has been performed, and techniques can be classiﬁed as mechanical and chemical methods. Mechanical methods consist of separating each particle physi cally. Ultrasound is one such simple and eﬀective method that uses speciﬁc equipment (the sonicator; Fig. 10.5). The ultrasonic method requires a suspension in which carbon nanomaterials are dispersed to be produced. Furthermore, to achieve an eﬀective dispersion, surfactants are usually incorporated during the process of producing the suspension. Some studies have investigated the eﬀects of various surfactants upon the dispersion of CNTs [5, 21–23]. In the ultrasonic method, the surfactants lignosulfonate and polycarboxylate oﬀer good dispersion of CNTs in the suspension (Fig. 10.6). However, excessive dosages of surfactants are not recommended, since they can lead to delayed cement-setting times , generating entrapped pores . Konsta-Gdoutos et al.  successfully obtained a
(a) Figure 10.5 type.
Various models of sonicator : (a) bath type and (b) probe
Various Types of Cement-Based Sensors
Figure 10.6 Suspension of CNTs treated by various surfactants. Reprinted from Ref. , Copyright (2012), with permission from Elsevier.
homogeneous suspension with surfactant/CNT weight ratios of 4.0 and 6.25 under the ultrasonic method. Although ultrasound is useful, it suﬀers crucial drawbacks for making cement composites, making it unsuitable for mass production [5, 26]. To make suspensions, sonicators are necessary, and the suspension capacity is limited by the sonicator performance. According to previous studies [24, 27], incorporation of silica fumes (SFs) of similar size to CNTs can cause separate agglomerations of CNTs when only dry-mixing processes are used. Figure 10.7 shows a conceptual diagram of the dispersion processes of CNTs according to the SF contents reported Kim et al. . Chemical methods can be described as surface treatment of carbon nanomaterials. There is another reason for using chemical methods on carbon nanomaterials, besides dispersion. The carbon is typically hydrophobic due to nonpolar electrical properties; hence, carbon-based materials can induce weak bonds with the cement matrix [11, 28–32]. In this method, acids are frequently used to form functional groups; one example is carboxylic acid, which can induce covalent bonding with cement hydrates. The CNTs incorporated into the cement matrix are more tightly surrounded by cement hydrates such as C–S–H and Ca(OH)2 with increasing ages. Functional groups, formed on the basal plane by surface treatment carboxylic acid, form covalent bonds with C–S–H and Ca(OH)2 , as shown in Fig. 10.8. It can
258 Cement-Based Piezoresistive Sensors for Structural Monitoring
Figure 10.7 Schematics of dispersion of CNTs in a cement matrix: (a) without silica fumes, (b) with a low volume of silica fumes, and (c) with a high volume of silica fumes. Reprinted from Ref. , Copyright (2014), with permission from Elsevier.
Figure 10.8 Reaction scheme between carboxylic-acid groups and the hydration productions of cement. Reprinted from Ref. , Copyright (2015), with permission from Elsevier.
be followed by improving the hydrophilic and bonding properties with a cement matrix.
10.2.5 Preparation of Cement-Based Sensors and Test Configurations To measure the change of resistance in CBSs, the electrodes should take priority over the preparation of all other constituents. Electrode materials have to satisfy two basic features: low electrical resistance and stable electricity . Representative materials for use as electrodes include copper and silver, which have electrical resistivity of 1.7 × 10−8 and 1.59 × 10−8 · m, respectively . The widths
Various Types of Cement-Based Sensors
Figure 10.9 Schematic diagrams of measurement methods and principle: (a) four probes and (b) two probes .
and intervals of electrodes are decided according to the measuring section and dimensions of the CBS. It should be noted that improper electrode sizes can impair mechanical performance. Two or four probes are used to measure the electrical properties of semiconductors. Figure 10.9 indicates the typical conﬁgurations of two- and four-probe systems and shows their circuit schematics, demonstrating their respective measuring principles. The voltages in both two- and four-probe systems can be divided as coming from the electrodes (VE ), CBS (VS ), and contact resistance between the electrode and CBS (VC ), with VE being negligible. In four-probe systems, VC can also be eliminated, leaving only VS . Consequently, resistance measured by a two-probe system becomes higher than that for a four-probe system according to Ohm’s law (V = I R), where V and I are voltage and current, respectively. Chiarello et al.  (Fig. 10.10) discovered that with an increase in the ratio between the electrode spacing (L) and the electrode– contact area ( A) ratio, the resistance of CBS increases when measured by the two-probe system. On the other hand, in the case of the four-probe system, there was no signiﬁcant increase of
260 Cement-Based Piezoresistive Sensors for Structural Monitoring
Figure 10.10 Resistance according to length-to-contact-area ratio for diﬀerent probe methods. Reprinted from Ref. , Copyright (2005), with permission from Elsevier.
resistance. Thus, the four-probe system is preferred for electrical resistivity measurements of CBS . The CBS resistance is measured diﬀerently using direct current (DC) or alternating current (AC); in the latter, AC with diﬀerent frequencies can aﬀect the resistance value. Although DC is the simplest method to measure resistance, electrical polarization, which is the phenomenon by which resistance increases consis tently due to electrochemical reactions between negative ions of cement composites and the positively charged electrode, should be considered. Polarization is severe for DC because voltage is consistently supplied. To avoid polarization, the resistance of CBS should converge until complete polarization. However, because polarization depends upon specimen size, larger CBS need more time to reach complete polarization [34, 36]. Another method to reduce polarization is to employ AC signals. Polarization is also generated by AC, but it is very weak with high frequency and falls within acceptable ranges [9, 18, 34, 37, 38].
10.2.6 Self-Sensing Properties by Various Carbon-Based Materials Various factors inﬂuence the electrical resistivity of CBS. In general, it is well known that the electrical resistivity of CBS can aﬀect
Various Types of Cement-Based Sensors
their piezoresistive properties. Such sensors, having a relatively low electrical resistivity, will show good sensitivity since lower resistivity allows an enhanced signal-to-noise ratio . However, opposite results have been shown. Yoo et al.  investigated the inﬂuences of various carbon-based materials (MWCNTs, CFs, G, CNFs) upon electrical resistivity and the piezoresistive properties of CBS. This research showed that CBS incorporating 0.5% CFs by volume showed the lowest resistivity of about 100 · cm, as illustrated in Fig. 10.11a. At the same concentration as other carbon-based materials, the resistivity of CBS with MWCNTs was about 1000 · cm, whereas those of G and CNF composites were higher than 10,000 · cm, only slightly lower than the resistivity of plain paste. The trend of resistivity of carbon-based materials can be explained, as described in the previous section. Firstly, since CFs, MWCNTs, and CNFs were ﬁber-type nanomaterials, they could form electrical pathways more easily than G, which was laminar type. Therefore, CNFs oﬀered the closest particles among ﬁber type materials when only the aspect ratio was considered. Under cyclic compressive loads, CBS that incorporated MWCNTs showed the best response when subjected to loads for which the FCR-versus compressive-stress curve had a correlation coeﬃcient of 0.85, as shown in Fig. 10.11d. Fu et al.  found out that ozone treatment of CFs increased the surface oxygen concentration and changed the oxygen bond from C–O to C=O. Consequently, the incorporation of ozone-treated CFs into CBS improved the bond strength between cement paste and CFs. The sensing ability of CBS with ozone-treated CFs was improved in terms of increased GF and better repeatability, as shown in Fig. 10.12. Yu et al.  investigated the change in resistance of CBS with 0.1% carboxyl-functionalized MWCNTs corresponding to cyclic compression, as shown in Fig. 10.12a. This result was compared with CBS with ordinary MWCNTs. They found that CBS with 0.1% carboxyl-functionalized MWCNTs showed a higher signal-to-noise ratio of piezoresistive response. Numerous studies have focused on developing CBS incorporating various carbon-based materials. Table 10.2 compares the properties of such CBS. However, since the GFs depend on the loading rate 
262 Cement-Based Piezoresistive Sensors for Structural Monitoring
Figure 10.11 Self-sensing capacities of cement-based sensors with diﬀer ent carbon-based materials : (a) change in resistivity with increasing age, (b) FCR by load, (c–f) correlation between FCR and loads: (c) 0.5% CF, (d) 0.5% CNT, (e) 0.5% CNF, and (f) 0.5% G.
and compositions of CBS, it is hard to compare materials directly. Moreover, there is a little deviation in these results, because there remain unsolved problems, such as the dispersion of carbon-based materials. Although CNTs exhibit outstanding piezoresistive self-sensing properties, they are one of the most expensive carbon-based
Various Types of Cement-Based Sensors
Figure 10.12 Self-sensing capacities of cement-based sensors incorpo rating: (a) as-received carbon ﬁber and (b) ozone-treated carbon ﬁber. Reprinted from Ref. , Copyright (1998), with permission from Elsevier.
materials. Therefore, they are of limited use for large-scale and ﬁeld applications. Some researchers have investigated the feasibility of replacing CNTs with CBs  or CFs [11, 42, 46]. Luo et al.  conducted experiments for stress and strain sensing of CBS incorporating both CNTs and CBs and compared them to CBS with only CNTs under cyclic loading. CBS with both CNTs and CBs showed a more sensitive response to stress and strain than did those incorporating only CNTs. CNTs wrapped in cement hydrates were found to be able to increase the probability of contact with CB particles within cement hydrates with movement under the loading condition. Azhari et al.  found that CBS with a hybrid system of 15% CFs and 1%
264 Cement-Based Piezoresistive Sensors for Structural Monitoring
Table 10.2 Gauge factors of cement-based sensors with diﬀerent carbon-based materials at concentrations Materials
Loading rates [kN/s]
0.5 + 0.1
MWCNTs were superior to CBS incorporating only 15% CFs in terms of FCR against stress and strain. According to a recent study , the 0.5% concentration of MWCNTs could be replaced by a 0.1% concentration of CFs. The authors analyzed the cost of incorporating carbon-based materials (CFs, MWCNTs), as well as the self-sensing properties of CBS under compressive loading and strain. One of the main CBS in this research was a hybrid material with both 0.1% CFs and 0.5% MWCNTs, which was compared to CBS with only 1% MWCNTs (Fig. 10.13). The GFs of the two CBS were 160 and 166.6, respectively, under the same loading. The cost of carbon-based materials incorporated
Figure 10.13 Self-sensing capacities of cement-based sensors incorporat ing (a) only 0.5% MWCNTs and (b) both 0.1% CFs and 0.5% MWCNTs .
Practical Applications of Cement-Based Sensors
into the CBS with 0.1% CFs was about half that of CBS with 1% MWCNTs. Thus, the economic eﬃciency of CBS incorporating both 0.1% CFs and 0.5% MWCNTs was veriﬁed.
10.3 Practical Applications of Cement-Based Sensors The sensing properties of CBS can be generally calculated as the fractional change of the electrical resistivity of the composites. In order to use CBS for SHM, numerous researchers have compared fractional changes in electrical resistivity to changes in stress and strain under applied compressive loads to investigate CBS as strain sensors [5–7]. Thus, the use of CBS as crack sensors, self-heating elements, dynamic sensors, and damage sensors is explained in this chapter. Lim et al.  investigated the feasibility of using CBS with CNTs as crack sensors for concrete beams. The CBS was embedded in the reinforced mortar beam under three-point bending conditions, as shown in Fig. 10.14a. The crack’s width–conductivity relationship
Figure 10.14 Experimental setups for SHM using cement-based sensors: (a) crack monitoring under bending  and (b) self-heating element . (a) Reprinted from Ref. , Copyright (2017), with permission from Elsevier.
266 Cement-Based Piezoresistive Sensors for Structural Monitoring
was studied and a simpliﬁed theoretical conductivity model was developed to compare experimental results. According to their results, the reliability of CBS for detecting cracks depended upon both crack width and moisture content. Kim et al.  and Lee et al.  investigated the heat characteristics of CBS. Kim et al.  developed a CBS for use as a self-heating element for incorporation into a structural heating system. Although cement composites with 2.0 wt% CNTs can reach a temperature of 70◦ C within 30 min, the composite incorporating under 0.6 wt% CNTs was appropriate as a self-heating element on the basis of its heating characteristics. Lee et al.  analyzed the heating characteristics of cementitious composites with single walled carbon nanotubes (SWCNTs) and MWCNTs, as shown in Fig. 10.14b. They observed that SWCNTs were more eﬀective than MWCNTs for modifying the heat characteristics and that an applied voltage of 100 V or more yielded the desired results. Recently, some researchers have measured dynamic properties such as impulsive loading [48–50]. Materazzi et al.  developed a dynamic strain sensor using cement paste with MWCNTs. On the basis of their experimental results, cement paste with 2 wt% of MWCNTs could detect the dynamic responses to a load applied with a frequency of 0.1 Hz. The output of the CBS, namely its electrical resistance, was almost identical to the input over the entire investigated frequency range of 0.1–2.0 Hz, as shown in Fig. 10.15a. A close correlation between the measured electrical resistance, axial strain of the sensor and the frequency–response function was obtained as a quasi-linear relationship, as shown in Fig. 10.15b. On the basis of their results, they developed a CBS with CNTs mounted on the RC beam, as shown in Fig. 10.16a . Ubertini et al.  observed that the CBS could detect high frequencies with a very low level of noise and an excellent signal-to-noise ratio. Moreover, the output of the proposed sensor compared well to those of oﬀ-the-shelf strain gauges and accelerometers. Baeza et al.  investigated the performance of CBSs as damage sensors, as shown in Fig. 10.16b. They tested cement composites with CNFs and CFs under diﬀerent casting conditions (embedded or attached), and electrical resistance was compared to the bending
Practical Applications of Cement-Based Sensors
(b) Figure 10.15 Dynamic response of cement-based sensors: (a) comparison of normalized measured strain and electrical resistance with loading frequencies 0.1, 0.5, and 2.0 Hz and (b) measured frequency–response curve. Reprinted from Ref. , Copyright (2013), with permission from Elsevier.
268 Cement-Based Piezoresistive Sensors for Structural Monitoring
Figure 10.16 Experimental setups for SHM using two cement-based sensors: (a) dynamic sensor in the RC beam and (b) damage sensor in RC beam. (a) Reprinted from Ref. , Copyright (2014), with permission from Elsevier. (b) https://creativecommons.org/licenses/by/3.0/.
moment of the RC beam. The CBS could detect strain even during RC beam failure in this study. As shown in Fig. 10.17, Han et al.  investigated cement paste with nickel powder for a wireless stress/strain-sensing system. The wireless stress/strain measurement system can be used to achieve a sensitivity to stress/strain of a GF of 1336.5 and a stress/strain resolution of 150 Pa/0.02 με. The newly devel oped wireless stress/strain measurement system integrated with pressure-sensitive nickel powder-ﬁlled CBS has such advantages as high sensitivity to stress/strain, high stress/strain resolution, simple circuit, and low energy consumption. Saaﬁ et al.  also investigated cement paste with CNTs for damage sensing. The sensor could follow both monotonic and cyclic loading behavior and detect the initiation of damage at an early loading stage. The change in the electrical resistance CBS was measured by wireless networking. In the literature several attempts to monitor traﬃc on the road are reported [53–55]. Shi et al.  found by simple testing that cement paste with a 0.5 or 1.0 wt% concentration of CFs was eﬀective for traﬃc monitoring and weighing traﬃc in motion. Electrical resistance reversibly increased to 1 MPa stress and 55 mph speed. Han et al. [56, 57] tried to use a CBS embedded in pavement to detect vehicles. They constructed a self-sensing pavement embedded with nickel-particle-ﬁlled CBS, as shown in Fig. 10.18a. Since such CBS have high sensitivity, the self-sensing
Practical Applications of Cement-Based Sensors
Figure 10.17 Experimental results of wireless stress/strain measurement system using CBS: (top) wireless acquisition system and (bottom) relation ship between input and output of pressure-sensitive nickel powder-ﬁlled cement-based stress/strain sensors under uniaxial compression. Reprinted from Ref. , Copyright (2008), with permission from Elsevier.
pavement could accurately detect the passing vehicles, as shown in Fig. 10.18b. Similarly, the Minnesota Road Research Facility (MnROAD) used self-sensing pavement with CNT-ﬁlled CBS to detect passing vehicles . Self-sensing pavement with CBS can also yield important traﬃc data such as ﬂow rate, vehicle speed, and density .
Figure 10.18 Attempts to monitor traﬃc using cement-based sensors: (a) self-sensing pavement with embedded cement-based sensor and (b) test results to detect passing vehicles. Reprinted from Ref. , Copyright (2011), with permission from Elsevier.
270 Cement-Based Piezoresistive Sensors for Structural Monitoring
10.4 Conclusions The concept and state of the art of CBS incorporating carbon based materials were described in this chapter. Incorporation of carbon-based materials into cement composites can allow self sensing of mechanical strain. A number of studies of CBS with various carbon-based materials have been carried out over the past decade. At present, research on improving the performance and economic eﬃciency of CBS using hybrid ﬁllers and on extending the self-sensing range through dynamic factors is ongoing and their feasibilities were veriﬁed. Self-sensing performance is strongly determined by the type and concentration of carbon-based materials and especially the dispersion of nanoscale materials. By now, various methods for dispersing carbon-based materials have been introduced, including mechanical and chemical methods. However, there still remain challenges facing the manufacture of simple and large-sized CBS. These problems have to be solved and study is necessary for practical use in the ﬁeld.
References 1. Chang, P. C., Flatau, A., Liu, S. C. (2003). Review paper: health monitoring of civil infrastructure, Struct. Health Monit., 2(3), pp. 257–267. 2. Yang, Y., Annamdas, V. G. M., Wang, C., Zhou, Y. (2008). Application of multiplexed FBG and PZT impedance sensors for health monitoring of rocks, Sensors, 8(1), pp. 271–289. 3. Yoo, D., You, I., Zi, G., Lee, S. (2019). Eﬀects of carbon nanomaterial type and amount on self-sensing capacity of cement paste, Measurement, 134, pp. 750–761. 4. Banthia, N., Djeridane, S., Pigeon, M. (1992). Electrical resistivity of carbon and steel micro-ﬁber reinforced cements, Cem. Concr. Res., 22(5), pp. 804–814. 5. D’Alessandro, A., Rallini, M., Ubertini, F., Materazzi, A. L., Kenny, J. M. (2016). Investigations on scalable fabrication procedures for self-sensing carbon nanotube cement-matrix composites for SHM applications, Cem. Concr. Compos., 65, pp. 200–213.
272 Cement-Based Piezoresistive Sensors for Structural Monitoring
6. Yu, X., Kwon, E. (2009). A carbon nanotube/cement composite with piezoresistive properties, Smart Mater. Struct., 18(5), p. 55010. 7. Yoo, D.-Y., You, I., Lee, S.-J. (2017). Electrical properties of cement-based composites with carbon nanotubes, graphene, and graphite nanoﬁbers, Sensors, 17(5), p. 1064. 8. Xu, J., Zhong, W., Yao, W. (2010). Modeling of conductivity in carbon ﬁber-reinforced cement-based composite, J. Mater. Sci., 45(13), pp. 3538–3546. 9. Han, B., Ding, S., Yu, X. (2015). Intrinsic self-sensing concrete and structures: a review, Measurement, 59, pp. 110–128. 10. Lee, S. J., You, I., Zi, G., Yoo, D. Y. (2017). Experimental investigation of the piezoresistive property of cement composites with hybrid carbon ﬁbers and nanotubes, Sensors, 17(11), p. 2561. 11. Wen, S., Chung, D. D. L. (1999). Seebeck eﬀect in carbon ﬁber-reinforced cement, Cem. Concr. Res., 29(12), pp. 1989–1993. 12. Li, H., Xiao, H. G., Ou, J. P. (2006). Eﬀect of compressive strain on electrical resistivity of carbon black-ﬁlled cement-based composites, Cem. Concr. Compos., 28(9), pp. 824–828. 13. Le, J. L., Du, H., Pang, S. D. (2014). Use of 2-D Graphene Nanoplatelets (GNP) in cement composites for structural health evaluation, Compos ites Part B, 67, pp. 555–563. 14. Yoo, D. Y., Zi, G., Kang, S. T., Yoon, Y. S. (2015). Biaxial ﬂexural behavior of ultra-high-performance ﬁber-reinforced concrete with diﬀerent ﬁber lengths and placement methods, Cem. Concr. Compos., 63, pp. 51–66. 15. Chen, B., Li, B., Gao, Y., Ling, T. C., Lu, Z., Li, Z. (2017). Investigation on electrically conductive aggregates produced by incorporating carbon ﬁber and carbon black, Constr. Build. Mater., 144, pp. 106–114. 16. Han, B., Yu, X., Ou, J. (2010). Eﬀect of water content on the piezoresis tivity of MWNT/cement composites, J. Mater. Sci., 45(14), pp. 3714– 3719. 17. Li, G. Y., Wang, P. M., Zhao, X. (2007). Pressure-sensitive properties and microstructure of carbon nanotube reinforced cement composites, Cem. Concr. Compos., 29(5), pp. 377–382. 18. Han, B., Guan, X., Ou, J. (2007). Electrode design, measuring method and data acquisition system of carbon ﬁber cement paste piezoresistive sensors, Sens. Actuators, A, 135(2), pp. 360–369. 19. Han, B., Ou, J. (2007). Embedded piezoresistive cement-based stress/ strain sensor, Sens. Actuators, A, 138(2), pp. 294–298.
20. Collins, F., Lambert, J., Duan, W. H. (2012). The inﬂuences of admixtures on the dispersion, workability, and strength of carbon nanotube-OPC paste mixtures, Cem. Concr. Compos., 34(2), pp. 201–207. 21. Luo, J., Duan, Z., Li, H. (2009). The inﬂuence of surfactants on the processing of multi-walled carbon nanotubes in reinforced cement matrix composites, Phys. Status Solidi A, 206(12), pp. 2783–2790. 22. Parveen, S., Rana, S., Fangueiro, R. (2013). A review on nanomaterial dis persion, microstructure, and mechanical properties of carbon nanotube and nanoﬁber reinforced cementitious composites, J. Nanomater., 2013, p. 80. 23. Kim, H. K., Nam, I. W., Lee, H. K. (2014). Enhanced eﬀect of carbon nanotube on mechanical and electrical properties of cement composites by incorporation of silica fume, Compos. Struct., 107, pp. 60–69. 24. Konsta-Gdoutos, M. S., Metaxa, Z. S., Shah, S. P. (2010). Highly dispersed carbon nanotube reinforced cement based materials, Cem. Concr. Res., 40(7), pp. 1052–1059. 25. Kharissova, O. V., Kharisov, B. I., de Casas Ortiz, E. G. (2013). Dispersion of carbon nanotubes in water and non-aqueous solvents, RSC Adv., 3(47), p. 24812. 26. Han, B., Sun, S., Ding, S., Zhang, L., Yu, X., Ou, J. (2015). Review of nanocarbon-engineered multifunctional cementitious composites, Composites Part A, 70, pp. 69–81. 27. Sanchez, F., Ince, C. (2009). Microstructure and macroscopic properties of hybrid carbon nanoﬁber/silica fume cement composites, Compos. Sci. Technol., 69(7–8), pp. 1310–1318. 28. Fu, X., Lu, W., Chang, D. D. L. (1998). Ozone treatment of carbon ﬁber for reinforcing cement, Carbon, 36(9), pp. 1337–1345. 29. Wen, S., Chung, D. D. L. (2006). The role of electronic and ionic conduction in the electrical conductivity of carbon ﬁber reinforced cement, Carbon, 44(11), pp. 2130–2138. 30. Ibarra, L., Macias, A., Palma, E. (1996). Stress-strain and stress relaxation in oxidated short carbon ﬁber-thermoplastic elastomer composites, J. Appl. Polym. Sci., 61(13), pp. 2447–2454. 31. Tiwari, S., Bijwe, J. (2014). Surface treatment of carbon ﬁbers: a review, Procedia Technol., 14, pp. 505–512. ´ ´ 32. Delamar, M., Desarmot, G., Fagebaume, O., Hitmi, R., Pinsonc, J., Saveant, J.-M. (1997). Modiﬁcation of carbon ﬁber surfaces by electrochemical reduction of aryl diazonium salts: application to carbon epoxy compos ites, Carbon, 35(6), pp. 801–807.
274 Cement-Based Piezoresistive Sensors for Structural Monitoring
33. Pan, Z., He, L., Qiu, L., Korayem, A. H., Li, G., Zhu, J. W., et al. (2015). Mechanical properties and microstructure of a graphene oxide-cement composite, Cem. Concr. Compos., 58, pp. 140–147. 34. Azhari, F. (2008). Cement-based sensors for structural health moni toring, PhD Dissertation, University of British Columbia, Vancouver, p. 184. 35. Chiarello, M., Zinno, R. (2005). Electrical conductivity of self-monitoring CFRC, Cem. Concr. Compos., 27(4), pp. 463–469. 36. Hou, T.-C., Lynch, J. P. (2005). Conductivity-based strain monitoring and damage characterization of ﬁber reinforced cementitious structural components, Smart Struct. Mater., pp. 419–429. 37. Fu, X., Ma, E., Chung, D. D. L., Anderson, W. A. (1997). Self-monitoring in carbon ﬁber reinforced mortar by reactance measurement, Cem. Concr. Res., 27(6), pp. 845–852. 38. Han, B., Zhang, K., Yu, X., Kwon, E., Ou, J. (2012). Electrical charac teristics and pressure-sensitive response measurements of carboxyl MWNT/cement composites, Cem. Concr. Compos., 34(6), pp. 794– 800. 39. Wen, S., Chung, D. D. L. (2008). Piezoresistivity-based strain sensing in carbon ﬁber-reinforced cement, Mater. J., 104(2), pp. 171–179. 40. Ou, J., Han, B. (2008). Piezoresistive cement-based strain sensors and self-sensing concrete components, J. Intell. Mater. Syst. Struct., 20(3), pp. 329–336. 41. Azhari, F., Banthia, N. (2012). Cement-based sensors with carbon ﬁbers and carbon nanotubes for piezoresistive sensing, Cem. Concr. Compos., 34(7), pp. 866–873. 42. Sun, S., Han, B., Jiang, S., Yu, X., Wang, Y., Li, H., Ou, J. (2017). Nano graphite platelets-enabled piezoresistive cementitious composites for structural health monitoring, Constr. Build. Mater., 136, pp. 314–328. 43. Saaﬁ, M., Tang, L., Fung, J., Rahman, M., Sillars, F., Liggat, J., Zhou, X. (2014). Graphene/ﬂy ash geopolymeric composites as self-sensing structural materials, Smart Mater. Struct., 23(6), p. 65006. 44. Luo, J. L., Duan, Z. D., Zhao, T. J., Li, Q. Y. (2010). Self-sensing property of cementitious nanocomposites hybrid with nanophase carbon nanotube and carbon black, Adv. Mater. Res., 143–144, pp. 644–647. 45. Luo, J. L., Duan, Z. D., Zhao, T. J., Li, Q. Y. (2010). Hybrid eﬀect of carbon ﬁber on piezoresistivity of carbon nanotube cement-based composite, Adv. Mater. Res., 143–144, pp. 639–643.
46. Lim, M. J., Lee, H. K., Nam, I. W., Kim, H. K. (2017). Carbon nanotube/ cement composites for crack monitoring of concrete structures, Compos. Struct., 180, pp. 741–750. 47. Lee, H., Kang, D., Song, Y. M., Chung, W. (2017). Heating experiment of CNT cementitious composites with single-walled and multiwalled carbon nanotubes, J. Nanomater., 2017, p. 3691509. 48. Kim, G. M., Naeem, F., Kim, H. K., Lee, H. K. (2016). Heating and heat dependent mechanical characteristics of CNT-embedded cementitious composites, Compos. Struct., 136, pp. 162–170. 49. Han, B., Yu, X., Kwon, E., Ou, J. (2010). Piezoresistive multi-walled carbon nanotubes ﬁlled cement-based composites, Sens. Lett., 8(2), pp. 344– 348. 50. Materazzi, A. L., Ubertini, F., D’Alessandro, A. (2013). Carbon nanotube cement-based transducers for dynamic sensing of strain, Cem. Concr. Compos., 37(1), pp. 2–11. 51. Ubertini, F., Materazzi, A. L., D’Alessandro, A., Laﬂamme, S. (2014). Natural frequencies identiﬁcation of a reinforced concrete beam using carbon nanotube cement-based sensors, Eng. Struct., 60, pp. 265–275. ´ P. (2013). Multifunctional 52. Baeza, F. J., Galao, O., Zornoza, E., Garces, cement composites strain and damage sensors applied on reinforced concrete (RC) structural elements, Materials, 6(3), pp. 841–855. 53. Han, B., Yu, Y., Han, B. Z., Ou, J. P. (2008). Development of a wireless stress/strain measurement system integrated with pressure-sensitive nickel powder-ﬁlled cement-based sensors, Sens. Actuators, A, 147(2), pp. 536–543. 54. Shi, Z. Q., Chung, D. D. L. (1999). Carbon ﬁber-reinforced concrete for traﬃc monitoring and weighing in motion, Cem. Concr. Res., 29(3), pp. 435–439. 55. Han, B., Zhang, K., Yu, X., Kwon, E., Ou, J. (2011). Nickel particle based self-sensing pavement for vehicle detection, Measurement, 44(9), pp. 1645–1650. 56. Han, B., Zhang, K., Burnham, T., Kwon, E., Yu, X. (2013). Integration and road tests of a self-sensing CNT concrete pavement system for traﬃc detection, Smart Mater. Struct., 22(1), p. 15020. 57. Fu, X., Lu, W., Chung, D. D. L. (1998). Ozone treatment of carbon ﬁber for reinforcing cement, Carbon, 36, pp. 1337–1345. 58. Saaﬁ, M. (2009). Wireless and embedded carbon nanotube networks for damage detection in concrete structures, Nanotechnology, 20(39), p. 395502.
Enhancing PCM Cement-Based Composites with Nanoparticles Luisa F. Cabezaa and Anna Laura Pisellob,c a GREiA Research Group, INSPIRES Research Centre, Universitat de Lleida,
Pere de Cabrera s/n, 25001-Lleida, Spain
b CIRIAF – Interuniversity Research Center on Pollution and Environment “Mauro Felli”,
Via Duranti 67, 06125 Perugia, Italy
c Department of Engineering, University of Perugia, Via Duranti 63, 06125 Perugia,
11.1 Introduction Phase change material (PCM) has been considered for thermal energy storage (TES) in buildings since before 1980 . The use of PCM can overcome the lack of coincidence between energy supply and energy demand and can be applied in buildings as passive and active systems . Passive TES systems can enhance eﬀectively the naturally available heat energy sources in order to maintain the comfort conditions in buildings and minimize the use of mechanically assisted heating or cooling systems . These systems include increased use of ventilated facades , thermal Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
278 Enhancing PCM Cement-Based Composites with Nanoparticles
mass [5, 6], shading eﬀect using blinds , coated glazing elements , and solar heating and free cooling (night ventilation) techniques . An up-to-date review of such systems can be found in de Gracia and Cabeza (2015)  and a review of building integrated TES in Navarro et al. (2016) . PCM can be incorporated in construction materials using diﬀerent methods, such as direct incorporation, immersion, encap sulation, microencapsulation, and shape stabilization . In direct incorporation and immersion, potential leakage has to be assessed. When PCM is encapsulated or added in a shape-stabilized new material, a new layer appears in the construction system of the wall. PCM can be encapsulated prior to incorporating it into building elements. There are four primary functions of the containment capsule: to meet the requirements of strength, ﬂexibility, corrosion resistance, and thermal stability; to act as a barrier to protect the PCM from harmful interaction with the environment; to provide a suﬃcient surface for heat transfer; and to provide structural stability and easy handling.
11.2 Incorporation of PCM in Concrete, Mortar, or Cement PCM can be impregnated or mixed with concrete  or mortar [14, 15]. One of the objectives pursued here is to preserve the concrete mechanical properties, while increasing its speciﬁc heat capacity. It is interesting to highlight that the addition of PCM in concrete decreases its density, which would have an interesting impact in the building structure weight. Fabiani and Pisello  also highlighted that the combination of PCM into a cement-based matrix may require dedicated thermal characterization methods because of the adaptive performance of such composite materials. Transient techniques may be recommended at a relatively larger scale than classic experimental techniques coming from chemical analysis, such as diﬀerential scanning calorimetry. In their work, they developed a brand new technique for detecting the activation of the transition phase of PCM within the speciﬁc concrete (Figs. 11.1 and 11.2).
Incorporation of PCM in Concrete, Mortar, or Cement
Figure 11.1 Preparation of concrete samples with PCM inclusion for dynamic tests of their thermal performance at an engineering scale. Reprinted from Ref. , Copyright (2018), with permission from Elsevier.
Figure 11.2 Thermal transient proﬁles of composite materials with PCM included into concrete, detecting transition-phase temperature ranges and duration. Reprinted from Ref. , Copyright (2018), with permission from Elsevier.
Cabeza et al.  (Fig. 11.3) showed the application of encapsulated PCM in two precast concrete house-like cubicles. One cubicle was made of conventional concrete and the other one of concrete with 5% of microencapsulated PCM. The objective here was to improve the thermal performance of buildings. Results presented a 2 h delay of the maximum peak temperature in summer because of
280 Enhancing PCM Cement-Based Composites with Nanoparticles
Figure 11.3 Incorporation of microencapsulated PCM in concrete-based walls. Left: Experimental setup. Right: Thermal performance. Reprinted from Ref. , Copyright (2007), with permission from Elsevier.
the PCM eﬀect and also an internal temperature proﬁle with lower ﬂuctuations. The most commonly used method for incorporating PCM into construction materials is microencapsulation, where small PCM particles (1–1000 μm) are encapsulated in a thin solid shell, which is made from natural and/or synthetic polymers. These microcapsules can then be directly added to the construction material, for example, concrete or plaster, during their mixing process. This method allows the possibility of providing a PCM composite over a large
Enhancing PCM Microcapsules with Nanoparticles for Cement-Based Composites
area, and hence it has the advantage of a high heat transfer rate per unit volume. Other advantages are that the capsules prevent leakage and resist volume change during phase change. They also have improved chemical stability and thermal reliability as phase separation during transition is limited to microscopic distances. However, the microcapsules can aﬀect the mechanical properties of concrete and they are also relatively expensive. A number of researchers have carried out studies using microencapsulated PCM in concrete. Hunger et al.  investigated the behavior and properties of self-compacting concrete mixes that contained 1%, 3%, and 5% of microencapsulated PCM by mass of concrete. A self-compacting concrete mix was used to mitigate damage to the microcapsules during compaction. Also the PCM was added to the mix at the latest possible moment to reduce its exposure to the mixing process. The authors recommended to use shells for the microencapsulated PCM in future applications to ensure that the capsules can withstand the high alkaline environment and mechanical impact during mixing. Another study in which microencapsulated high-purity paraﬃn PCM in an aqueous dispersion was added to self-compacting concrete was carried out by Fenollera et al. . PCM dosages of 5%, 10%, 15%, 20%, and 25% of mass of cement were added to a self-compacting concrete mix, and slump, compressive strength, and density were compared in order to ﬁnd an optimum combination. From the above two studies it can be concluded that 10% (by weight of cement) or 5% (by weight of concrete) is the maximum practical content of microencapsulated PCM to be used in a concrete mix application.
11.3 Enhancing PCM Microcapsules with Nanoparticles for Cement-Based Composites If PCM is incorporated in cement-based composites in capsules with open pores, leakage will occur when the PCM melts. Therefore, Li et al. (2014)  evaluated the possibility of using three types of nano-SiO2 powder (hydrophilic fumed silica [fs1], hydrophobic
282 Enhancing PCM Cement-Based Composites with Nanoparticles
fumed silica [fs2], and precipitated silica [ps2]) to prevent such leakage in the commercial product PX25. PX25 is commercial form stable PCM from Rubitherm, containing paraﬃn in a secondary supporting structure made of fs1. PX25 was incorporated into cement paste to fabricate TES composites. Previously, to prevent paraﬃn leakage, PX25 was surface-modiﬁed by mixing it with the three diﬀerent nanosilicas separately. Because of the very high surface energy of the nanosilicas, they can easily deposit on the surfaces of PX25 particles. According to the authors, paraﬃn leakage was eliminated when fs2 or ps2 was used in a 2.3% and 9.0% mass fraction (relative to PX25), respectively. However, fs1 did not prevent leakage of paraﬃn. It should be highlighted that the authors reported that the compressive strength of cementitious composites decreased by incorporating hydrophobic nanosilica-modiﬁed PCM composites. A stated possible reason was slowdown of cement hydration due to the hydrophobic surface character of the PCM composites. In this view, PCM inclusion into concrete composites may also be used to partially absorb hydration heat during the curing process, as demonstrated by Fabiani et al.  (Fig. 11.4). Another approach to the use of nanoparticles to decrease PCM leakage in cement-based composites is to increase the capsule strength of microencapsulated PCM. Authors found that it is important that the capsule itself be physically and chemically stable within the concrete matrix. The capsule needs to be hard and sustainable to avoid being damaged during the concrete-mixing and concrete-casting processes. Park et al.  discussed the use of zeolite and zeocarbon that some researchers have used for reinforcing microcapsules to enable them to withstand high friction and impact during the concrete-mixing process. Yoo et al. (2017)  used cellulose nanocrystals (CNCs) to improve the mechanical and barrier properties of microcapsules. They used the advantageous characteristics of CNCs, such as high thermal conductivity, high stiﬀness, and low coeﬃcient of thermal expansion with a high aspect ratio, to reinforce polymeric materials, forming a dense network resulting in sustainable, ecofriendly, and versatile polymer composites. In this study, PCM micro capsules were fabricated through an interfacial polymerization of poly(urea−urethane) (PU) as a shell component (Fig. 11.3)
Enhancing PCM Microcapsules with Nanoparticles for Cement-Based Composites
Figure 11.4 Thermal dynamics of concrete hydration process with PCM inclusion .
using modiﬁed cellulose nanocrystals (hCNCs). The strength of the microcapsules was tested physically breaking them applying a load to them. The authors claimed that these microcapsules would perform better in cement-based composites than those without nanocellulose. Finally, carbon nanoparticles have been used to increase the thermal conductivity of a cement-based PCM composite . In this study, octadecane is introduced to a cement-based composite inside diatomite particles. But before, diatomite was treated with carbon nanoparticles to increase its thermal conductivity. The results showed good results in microstructure and in mechanical and thermal properties of the composites. The compressive and ﬂexural strength of the cement composites exhibited a decreasing tendency with an increase in the dosage of PCM. This phenomenon can be attributed to not only the poor mechanical strength and interface compatibility of the PCM–diatomite composite but
284 Enhancing PCM Cement-Based Composites with Nanoparticles
also the increasing porosity of the prepared cement-based ﬁnal composite. Nevertheless, the mechanical strength still satisﬁes the requirements for building applications. Although the properties of diatomite with PCM and carbon nanoparticle–enhanced diatomite with PCM were compared by the authors, this comparison was not done within the cement-based composite, not allowing us to see whether the addition of carbon nanoparticles would enhance the overall thermal performance of the ﬁnal composite.
Acknowledgments Prof. Luisa F. Cabeza would like to acknowledge the Spanish Government for funding (PRX17/00221), which allowed her to visit the University of Perugia for 6 months. Prof. Cabeza would like to thank the Catalan Government for the quality accreditation given to their research group (2017 SGR 1537). GREA is certiﬁed agent TECNIO in the category of technology developers from the Government of Catalonia. This work was partially funded by ´ y Universidades de Espana ˜ the Ministerio de Ciencia, Innovacion (RTI2018-093849-B-C31). This work is also partially supported by ICREA under the ICREA Academia program. Part of the ﬁndings also refer to SOS CITTA’, supported by Fondazione Cassa di Risparmio di Perugia 2018.0499.026. Anna Laura Pisello thanks H2CU for supporting her international cooperation and research activities.
References 1. Mehling, H., Cabeza, L. F. (2008). Heat and Cold Storage with PCM: An Up to Date Introduction Into Basics and Applications, Springer-Verlag, Berlin Heidelberg, Germany. ´ 2. Gil, A., Medrano, M., Martorell, I., Lazaro, A., Dolado, P., Zalba, B., Cabeza, L. F. (2010). State of the art on high temperature thermal energy storage for power generation. Part 1: Concepts, materials and modellization, Renewable Sustainable Energy Rev., 14, pp. 31–55. 3. Parameshwaran, R., Kalaiselvam, S., Harikrishnan, S., Elayaperumal, A. (2012). Sustainable thermal energy storage technologies for buildings: a review, Renewable Sustainable Energy Rev., 16, pp. 2394–2433.
4. Todorovic, B., Maric, B. (2002). The inﬂuence of double facades on building heat losses and cooling loads, Faculty of Mechanical Engineering, Belgrade University, Technical Report. ´ 5. Castell, A., Martorell, I., Medrano, M., Perez, G., Cabeza, L. F. (2010). Experimental study of using PCM in brick constructive solutions for passive cooling, Energy Build., 42, pp. 534–540. 6. de Gracia, A., Castell, A., Medrano, M., Cabeza, L. F. (2011). Dynamic thermal performance of alveolar brick construction system, Energy Conserv. Manage., 52, pp. 2495–2500. 7. Gratia, E., De Herde, A. (2007). The most eﬃcient position of shading devices in a double-skin fac¸ade, Energy Build., 39, pp. 364–373. 8. Viljoen, A., Dubile, J., Wilson, M., Fontoynont, M. (1997). Investigations for improving the daylighting potential of double-skinned oﬃce buildings, Sol. Energy, 59, pp. 179–194. 9. Gratia, E., De Herde, A. (2004). Natural cooling strategies eﬃciency in an oﬃce building with a double skin fac¸ades, Energy Build., 36, pp. 1139– 1152. 10. de Gracia, A., Cabeza, L. F. (2015). Phase change materials and thermal energy storage for buildings, Energy Build., 103, pp. 414–419. 11. Navarro, L., de Gracia, A., Niall, D., Castell, A., Browne, M., McCormack, S. J., Griﬃths, P., Cabeza, L. F. (2016). Thermal energy storage in building integrated termal systems: a review. Part 2: Integration as passive system, Renewable Energy, 85, pp. 1334–1356. 12. Memon, S. A. (2014). Phase change materials integrated in building walls: a state of the art review, Renewable Sustainable Energy Rev., 31, pp. 870–906. 13. Lai, C., Hokoi, S. (2014). Thermal performance of an aluminum honeycomb wallboard incorporating microencapsulated PCM, Energy Build., 73, pp. 37–47. 14. Desai, D., Miller, M., Lynch, J. P., Li, V. C. (2014). Development of thermally adaptive engineered cementitious composite for passive heat storage, Constr. Build. Mater., 67, pp. 366–372. 15. Fabiani, C., Pisello, A. L. (2018). Coupling the transient plane source method with a dynamically controlled environment to study PCM doped building materials, Energy Build., 180, pp. 122–134. ´ C., M. Nogues, ´ M., Medrano, M., Leppers, R., 16. Cabeza, L. F., Castellon, Zubillaga, O. (2007). Use of microencapsulated PCM in concrete walls for energy savings, Energy Build., 39, pp. 113–119.
286 Enhancing PCM Cement-Based Composites with Nanoparticles
17. Hunger, M., Entrop, A. G., Mandilaras, I., Brouwers, H. J. H., Founti, M. (2009). The behavior of self-compacting concrete containing micro encapsulated phase change materials, Cem. Concr. Compos., 31(10), pp. 731–743. 18. Fenollera, M., M´ıguez, J. L., Goicoechea, I., Lorenzo, J., Alvarez, M. A. (2013). The inﬂuence of phase change materials on the properties of self-compacting concrete, Materials, 6(8), pp. 3530–3546. 19. Fabiani, C., Pisello, A. L., D’Alessandro, A., Ubertini, F., Cabeza, L. F., Cotana, F. (2014). Eﬀect of PCM on the hydration process of cement based mixtures: a novel thermo-mechanical investigation, Materials, 11(6), p. 871. 20. Park, S. K., Jay Kim, J. H., Nam, J. W., Hung, D. P., Kim, J. K. (2009). Development of antifungal mortar and concrete using zeolite and zeocarbon microcapsules, Cem. Concr. Compos., 31, pp. 447–453. 21. Yoo, Y., Martinez, C., Youngblood, J. P. (2017). Synthesis and character ization of microencapsulated phase change materials with poly(ure uretane) shells containing cellulose nanocrystals, ACS Appl. Mater. Interfaces, 9, pp. 31763–31776. 22. Qian, T., Li, J. (2018). Octadecane/C-decorated diatomite composite phase change material with enhanced thermal conductivity as aggregate for developing structuralefunctional integrated cement for thermal energy storage, Energy, 142, pp. 234–249.
Cement-Based Composites with PCMs and Nanoinclusions for Thermal Storage Manila Chieruzzi and Luigi Torre Civil and Environmental Engineering Department, University of Perugia, Strada di Pentima 4, 05100 Terni, Italy [email protected]; [email protected]
Carbon dioxide is one of the gases responsible for greenhouse gas emissions produced mainly by the burning of fossil fuels. Solid materials like concrete and structural cement can be used for thermal energy storage (TES). Cement-based materials can store heat (as sensible heat) but this ability needs to be improved. To enhance the eﬃciency and thermal performance of cementitious materials (in particular to reduce the energy demands for heating and cooling), phase change materials (PCMs) can be used. They can store and release a large amount of thermal energy (in form of latent heat) during a phase change (usually melting/solidiﬁcation). The introduction of PCMs into cement-based materials can increase the total energy stored, thus reducing energy consumption. However, the most common PCMs suitable for cement-based materials for building applications have low thermal storage properties. Research is underway in order to develop other kinds
Nanotechnology in Cement-Based Construction Edited by Antonella D’Alessandro, Annibale Luigi Materazzi, and Filippo Ubertini c 2020 Jenny Stanford Publishing Pte. Ltd. Copyright � ISBN 978-981-4800-76-1 (Hardcover), 978-0-429-32849-7 (eBook) www.jennystanford.com
288 Cement-Based Composites with PCMs and Nanoinclusions for Thermal Storage
of PCMs to improve latent heat storage. In recent years, the addition of nanoparticles seems to be very promising to further enhance the thermal properties of PCMs. This chapter reports the studies that have been carried out by many researchers on cement-based composites with PCMs for TES and the use of nanoinclusions.
12.1 Introduction The increase in the global energy demand is an important issue in the past decades, with the consequent increase of greenhouse gas emissions. The aim is to reduce the gas emissions by 20% by 2020. Cement-based materials are greatly involved in this issue since the construction ﬁeld represents one of the main contributors to energy consumption. The challenge is to reduce the energy demand of building constructions by enhancing their thermal energy storage (TES) capability. TES systems represent an addition of stored heat that can be used in later times. The use of phase change materials (PCMs) as TES materials added into cement-based materials is becoming increasingly im portant. The energy stored by PCMs during their melting can be used later during their solidiﬁcation; at this time they can release energy to the environment, thus reducing the need for electricity to maintain a certain comfort temperature. The introduction of PCMs into cement-based materials can be done in several ways: They can be directly immersed into cements or directly added in the form of microcapsules. They can also be contained in a porous matrix able to avoid PCM leakage during the melting phase. Several researchers investigated the diﬀerent methods of PCM incorporation into cements and the eﬀect of the addition of these materials on the thermal performance of cement based materials. The purpose of this chapter is to report the improvements achieved in TES using PCMs in cement-based materials.
Thermal Energy Storage
After a brief introduction on the types of TES, the chapter focuses on the experimental characterization of diﬀerent PCMs and the mechanisms to realize cement-based composites with PCMs to be used as thermal storage media. The next step of the actual research is to further improve the thermal storage behavior of cement-based materials with the use of nanoinclusions into PCMs. Thus, the eﬀect of their addition into PCMs for cement-based materials will be reported here. These new composite materials made of cement-based materials, PCMs, and nanoinclusions may represent new solutions for the enhancement of the thermal storage ability of constructions materials.
12.2 Thermal Energy Storage Energy storage is the temporary storage of energy that can be used at a later time, thus reducing the time or rate mismatch between energy supply and demand. In TES systems, heat is transferred to a storage media and released at a later time [15, 20]. In particular, in solar energy systems the heat stored during the day can be preserved and released during the night. The use of heat storage in buildings can help to reduce the use of electricity, with consequent energy saving [17, 23, 45]. To make a TES system competitive with respect to other forms of energies the material used as storage media must be low cost, available in big quantities, and easy to introduce. Moreover, the storage material must have a high energy density, chemical stability, low heat losses, and low environmental impact. Thermal storage can be sensible heat thermal energy storage (SHTES) or latent heat thermal energy storage (LHTES), with a phase transformation occurring. On the basis of storage temper ature, TES can be divided into four categories: cold- (>20◦ C), low- (20◦ C–150◦ C), medium- (150◦ C–300◦ C), and high- (